MANUFACTURING GUIDE

Dental LT Clear V2 ResinEN

Manufacturing Guide

TRÜretim Kılavuzu

DE

Fertigungsleitfaden

RO

Ghid de fabricație

FR

Guide de fabrication

NO

ProduksjonsveiledningIT

Guida alla produzione

LVRažošanas rokasgrāmata

ES

Guía de fabricaciónLT

Gamybos vadovasPT

Guia do FabricanteET

Tootmisjuhend

NL

Productiegids

SK

Sprievodca výrobou

DA

Fremstillingsvejledning

SL

Priročnik za izdelavo

SV

Guide för tillverkning

PL

Przewodnik produkcyjny

FIValmistusopas

RUРуководство по производству

CSPrůvodce výrobou

BGРъководство за производство

HU

Gyártási útmutató

JA

マニュファクチャリングガイド

ELΟδηγός κατασκευής

ZH

Prepared: 02/29/2024 PRNT-0099 Rev 02

制造指南Specific Manufacturing Considerations
Dental LT Clear V2 Resin specifications have been validated using the hardware and parametersindicated below. For biocompatibility compliance, validation used a dedicated resin tank and mixer,
build platform, wash unit and post-processing equipment that were not mixed with any other resins.

1. Hardware:a. Formlabs 3D Printer: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Print Accessories: Formlabs Build Platforms, Formlabs Resin Tanks

2. Software:a. Formlabs PreForm

3. Printing Parameters:
a. Part Orientation: Intaglio surface facing away from the build platform at a 0 - 40° tilted angleb. Layer Thickness: 100 μm
c. Part Thickness:• Occlusal Surfaces: 2 mm minimum• Walls: 1 mm minimum

4. Recommended Post-Processing Equipment and Accessories:
a. Formlabs Processing Accessories: Form Auto, Resin Pumping Systemb. Formlabs Validated Wash Unit: Form Wash, Form Wash (2nd Generation), Form Wash L, Ultrasonic
Wash Unitc. Formlabs Validated Cure Unit: Form Cure, Form Cure L, Fast CureA. PRINTING
1. Shake cartridge: Shake the cartridge before every print job. Color deviations and print failures
may occur if the cartridge is shaken insufficiently.
2. Set up: Insert resin cartridge into a compatible Formlabs 3D printer. Insert resin tank and attach
mixer to the tank.
3. Printing:a. Prepare a print job using PreForm software. Import desired part STL file.
b. Orient and generate supports.
c. Send the print job to the printer.
d. Begin print by selecting a print job from the print menu. Follow any prompts or dialogs shownon the printer screen. Printer will automatically complete the print.

B. PART REMOVAL
Remove the build platform from the printer. To remove parts from the build platform, wedge the part
removal tool under the printed part raft, and rotate the tool. Formlabs Build Platform 2 or Build Platform 2L
may be used for easy, tool free removal. For detailed techniques visit support.formlabs.com.

C. WASHING
Place the printed parts in a Formlabs-validated wash unit with 99% Isopropyl Alcohol.
1. Form Wash, Form Wash (2nd Generation) - High speed*, or Form Wash L:a. Wash for 15 minutes or until clean in Form Wash or Form Wash L.
b. Remove parts from the wash unit and soak in fresh Isopropyl Alcohol for 5 minutes.
c. If parts do not appear clean after washing, consider replacing used Isopropyl Alcohol in thewash unit with fresh solvent.
*For Form Wash (2nd Gen), High speed settings are validated for use.
2. Ultrasonic Wash Unit:ENGLISH

Dental LT Clear V2 Resin is a light-curable polymer-based resin designed for the fabrication of
biocompatible, long-term use, removable dental and orthodontic appliances such as occlusal splints,
night guards, mouthguards, and/or bleaching trays by additive manufacturing. This Manufacturing
Guide will give equipment, printing and post-processing recommendations and requirements toensure the correct and safe usage of this material.

NOTE: Using Isopropyl Alcohol in an ultrasonic bath presents a risk of fire or explosion. When using
an ultrasonic wash read and follow all safety recommendations from the ultrasonic wash manufacturer.
a. Use clean 99% Isopropyl Alcohol for each wash.
b. Place parts in a secondary disposable plastic container or plastic resealable bag then fill with
99% Isopropyl Alcohol, ensuring parts are fully submerged.
c. Place the secondary container in the ultrasonic unit water bath and sonicate for 2 minutes oruntil clean.**Washing efficacy depends on the ultrasonic unit size and power. Formlabs testing was conductedwith ultrasonic units at 36 W/L or higher.

D. DRYING
1. Remove parts from Isopropyl Alcohol and leave to air dry at room temperature for at least 30 minutes.
NOTE: Dry times can vary depending on the design of parts and ambient conditions. Do not letparts sit in Isopropyl Alcohol for longer than needed.
2. Inspect printed parts to ensure that parts are clean and dry. No residual solvent, excess liquid resinor residue particles should remain on the surface before proceeding to subsequent steps.
3. If the residual solvent is still present, dry parts longer. If resin residue is still visible, rewash parts
until clean and dry.

E. POST-CURING
Place the printed parts in a Formlabs-validated post-curing unit and cure for the required time.
1. Form Cure or Form Cure L:
a. Cure for 60 minutes at 60 °C
b. Allow the Form Cure or Form Cure L unit to cool down to room temperature between cure
cycles.
2. Fast Cure:a. Cure for 6 minutes at Light Intensity 5b. Allow the Fast Cure unit to cool for at least 10 minutes between cure cycles.

F. SUPPORT REMOVAL & POLISHING
1. Support marks can cause abrasion if not removed and polished. Remove supports using a cutting
disk and handpiece, cutting plier, or other appropriate finishing tools.
2. Polish the printed appliances using typical dental polishing methods prior to patient use.
3. Inspect the parts for any cracks. Discard if any damage or cracks are detected.

G. CLEANING & DISINFECTION
1. Fully post-processed parts can be cleaned using a dedicated soft toothbrush with neutral soap
and room-temperature water. Do not use toothpaste or any other cleaning products on parts
printed with Dental LT Clear V2 Resin.
2. The appliances may be cleaned and disinfected according to facility protocols. Tested disinfection
method: soaking the finished appliance in fresh 70% IPA for 5 minutes. Do not leave the part in thealcohol solution for longer than 5 minutes.
3. After cleaning and disinfection inspect the part for damage or cracks to ensure that the integrityof the designed part meets performance requirements. Discard if any damage or cracks aredetected.

H. HAZARDS, STORAGE & DISPOSAL
1. Cured resin is non-hazardous and may be disposed of as regular waste.
2. See SDS for more information at support.formlabs.com.

Spezifische Überlegungen zur Fertigung
Die Spezifikationen von Dental LT Clear Resin V2 wurden unter Verwendung der unten angegebenen
Hardware und Parameter validiert. Um die Biokompatibilität zu gewährleisten, wurde für die
Validierung ein dedizierter Harztank mit Mischer, eine dedizierte Konstruktionsplattform undWascheinheit sowie dedizierte Nachbearbeitungsgeräte genutzt, die nicht mit anderen Harzen in
Kontakt gekommen sind.

1. Hardware:a. Formlabs-3D-Drucker: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Druck-Zubehör: Formlabs Konstruktionsplattformen, Formlabs Harztanks

2. Software:a. Formlabs PreForm

3. Druckparametera. Ausrichtung: Intagliofläche zeigt in einem von 0 bis 40° geneigten Winkel von derKonstruktionsplattform weg.
b. Schichtdicke: 100 μm
c. Druckteildicke:• Okklusionsfläche: mindestens 2 mm
• Wände: mindestens 1 mm

4. Empfohlene Nachbearbeitungsgeräte und Zubehör:
a. Formlabs-Bearbeitungszubehör: Form Auto, Resin Pumping Systemb. Validierte Formlabs Wascheinheit: Form Wash, Form Wash (2. Generation), Form Wash L,
Ultraschall-Waschgerät
c. Validierte Formlabs Aushärteeinheit: Form Cure, Form Cure L, Fast Cure

A. DRUCKEN
1. Kartusche schütteln: Schütteln Sie die Kartusche vor jedem Druckauftrag. Wenn die Kartusche
nicht ausreichend geschüttelt wird, können Farbabweichungen und Fehldrucke auftreten.
2. Einrichtung: Setzen Sie die Harzkartusche in einen kompatiblen Formlabs-3D-Drucker ein.
Setzen Sie den Harzbehälter ein und befestigen Sie den Mischer am Tank.
3. Druck:a. Bereiten Sie einen Druckauftrag mit der Software PreForm vor. Importieren Sie die STL-Datei
des gewünschten Teils.
b. Richten Sie das Modell aus und generieren Sie Stützstrukturen.
c. Senden Sie den Druckauftrag an den Drucker.
d. Beginnen Sie den Druckvorgang durch Auswahl eines Druckauftrags aus dem Menü „Print“(Druck). Befolgen Sie alle Aufforderungen oder Dialoge, die auf dem Druckerbildschirmangezeigt werden. Der Drucker schließt den Druckvorgang automatisch ab.

B. ENTFERNEN DER TEILE
Entnehmen Sie die Konstruktionsplattform aus dem Drucker. Um Teile von der Konstruktionsplattform zu
entfernen, klemmen Sie das Ablösewerkzeug unter das Druckteil-Raft und drehen Sie das Werkzeug.
Für ein einfaches, werkzeugloses Entfernen können die Formlabs Build Platform 2 oder die
Build Platform 2L verwendet werden. Detaillierte Techniken finden Sie auf support.formlabs.com.

DEUTSCH

Dental LT Clear Resin V2 ist ein lichthärtendes Kunstharz auf Polymerbasis für die Herstellung
von biokompatiblen, langfristig verwendbaren, herausnehmbaren zahnmedizinischen undkieferorthopädischen Anwendungen wie Okklusionsschienen, Nachtschienen, Mundschutz und/oder
Bleaching-Schienen mittels additiver Fertigung. Dieser Fertigungsleitfaden enthält Empfehlungenbezüglich Geräte, Druck und Nachbearbeitung, damit die korrekte und sichere Verwendung dieses
Materials gewährleistet ist.

C. WASCHEN
Legen Sie die Druckteile in ein von Formlabs geprüftes Waschgerät mit 99%igem Isopropylalkohol.
1. Form Wash, Form Wash (2. Generation) für hohe Drehzahlen* oder Form Wash L:a. Waschen Sie die Teile in einem Form Wash oder Form Wash L für 15 Minuten oder bis sie
komplett sauber sind.
b. Nehmen Sie die Teile aus dem Waschgerät und tauchen Sie sie für 5 Minuten infrischen Isopropylalkohol.
c. Wenn die Teile nach dem Waschen nicht sauber erscheinen, sollten Sie den verwendeten
Isopropylalkohol im Waschgerät durch frisches Lösungsmittel ersetzen.
*Für Form Wash (2. Generation) sind die Einstellungen für hohe Drehzahl für die Verwendung bestätigt.
2. Ultraschall-Waschgerät:
ANMERKUNG: Bei der Verwendung von Isopropylalkohol in einem Ultraschallbad besteht Brandund Explosionsgefahr. Wenn Sie ein Ultraschallgerät verwenden, lesen und befolgen Sie alle
Sicherheitsempfehlungen des Herstellers des Ultraschallgeräts.
a. Verwenden Sie für jeden Waschvorgang sauberen 99%igen Isopropylalkohol.
b. Platzieren Sie die Teile in einen zweiten Einweg-Plastikbehälter oder einen
wiederverschließbaren Plastikbeutel und füllen Sie ihn mit 99%igem Isopropylalkohol, sodass
die Teile vollständig bedeckt sind.
c. Platzieren Sie den Sekundärbehälter in das Wasserbad des Ultraschallgeräts und beschallen
Sie ihn für 2 Minuten oder bis die Teile sauber sind.**Die Wirksamkeit der Reinigung hängt von der Größe und Leistung des Ultraschallgeräts ab.
Die Formlabs-Tests wurden mit Ultraschallgeräten bei 36 W/L oder höher durchgeführt.

D. TROCKNEN
1. Nehmen Sie die Teile aus dem Isopropylalkohol und lassen Sie sie mindestens 30 Minuten langbei Raumtemperatur an der Luft trocknen. ANMERKUNG: Die Trockenzeiten können je nach
Teiledesign und Umgebungsbedingungen variieren. Lassen Sie die Teile nicht länger als nötig in
Isopropylalkohol liegen.
2. Untersuchen Sie die Druckteile und stellen Sie sicher, dass sie sauber und trocken sind. Es
dürfen keine Lösungsmittelreste, überschüssiges flüssiges Kunstharz oder Partikelreste auf der
Oberfläche verbleiben, bevor die nachfolgenden Schritte ausgeführt werden.
3. Wenn noch Lösungsmittelreste vorhanden sind, lassen Sie die Teile länger trocknen. Wenn nochHarzreste sichtbar sind, waschen Sie die Teile erneut, bis sie sauber und trocken sind.

E. NACHHÄRTUNG
Platzieren Sie die Druckteile in ein von Formlabs validiertes Nachhärtegerät und lassen Sie sie die
erforderliche Zeit aushärten.
1. Form Cure oder Form Cure L:
a. Aushärtung für 60 Minuten bei 60 °C
b. Lassen Sie das Form-Cure-Gerät oder Form-Cure-L-Gerät zwischen den Aushärtezyklen auf
Raumtemperatur abkühlen.
2. Fast Cure:a. Aushärtung für 6 Minuten bei Lichtintensität 5b. Lassen Sie das Fast-Cure-Gerät zwischen den Aushärtezyklen mindestens 10 Minuten
lang abkühlen.

F. STÜTZEN ENTFERNEN & POLITUR
1. Stützspuren können Abrasion verursachen, wenn sie nicht entfernt und abgeschliffen werden.
Entfernen Sie die Stützen mit einer Schneidscheibe und einem Handstück, einer Trennzangeoder einem anderen geeigneten Fertigstellungswerkzeug.
2. Polieren Sie die gedruckten Anwendungen vor der Verwendung durch den Patienten mit denüblichen zahnmedizinischen Poliermethoden.
3. Untersuchen Sie die Teile auf Risse. Entsorgen Sie die Teile, falls Sie Beschädigungen oder
Risse feststellen.

G. REINIGUNG UND DESINFEKTION
1. Vollständig nachbearbeitete Teile können mit einer eigens dafür bestimmten weichen Zahnbürste,
Neutralseife und zimmertemperiertem Wasser gereinigt werden. Verwenden Sie keine Zahnpasta
und keine anderen Reinigungsmittel bei Druckteilen aus Dental LT Clear Resin V2.
2. Die dentalen Anwendungen können gemäß den betriebsinternen Anweisungen gereinigt unddesinfiziert werden. Geprüfte Desinfektionsmethode: Eintauchen der fertigen Anwendung in frischen
70%igen IPA für 5 Minuten. Lassen Sie das Teil nicht länger als 5 Minuten in der Alkohollösung.
3. Prüfen Sie das Teil nach der Reinigung und Desinfektion auf Schäden oder Risse, um
sicherzustellen, dass die Integrität des entworfenen Teils den Leistungsanforderungen entspricht.
Entsorgen Sie die Teile, falls Sie Beschädigungen oder Risse feststellen.

H. GEFAHREN, LAGERUNG UND ENTSORGUNG
1. Ausgehärtetes Harz ist nicht gefährlich und kann als normaler Hausmüll entsorgt werden.
2. Weitere Informationen finden Sie im SDB unter support.formlabs.com.

Considérations particulières relatives à la fabrication
Les spécifications de Dental LT Clear Resin (V2) ont été validées lors de l’utilisation du matériel etdes paramètres indiqués ci-dessous. Afin d’assurer la biocompatibilité, la validation a utilisé un bac
à résine, un mélangeur, une plateforme de fabrication, une unité de lavage et un équipement depost-traitement dédiés qui n’ont pas été mélangés avec d’autres résines.

1. Matériel :a. Imprimante 3D Formlabs : Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Accessoires d’impression : plateformes de fabrication Formlabs, bacs à résine Formlabs

2. Logiciel :a. PreForm de Formlabs

3. Paramètres d’impression :a. Orientation des pièces : la surface intrados est orientée à l’opposé à la plateforme de fabrication,
à un angle d’inclinaison de 0 à 40°
b. Épaisseur de couche : 100 μm
c. Épaisseur de la pièce :• Surfaces occlusales : 2 mm au minimum• Parois : 1 mm au minimum

4. Équipement et accessoires de post-traitement recommandés :a. Accessoires de traitement Formlabs : Form Auto, Resin Pumping Systemb. Unité de lavage validée par Formlabs : Form Wash, Form Wash (2e génération), Form Wash L,
unité de lavage à ultrasonsc. Unité de polymérisation validée par Formlabs : Form Cure, Form Cure L, Fast Cure

A. IMPRESSION
1. Agitation de la cartouche : secouez la cartouche avant chaque impression. Une agitation
insuffisante de la cartouche peut entraîner des écarts de couleur ou des erreurs d’impression.
2. Installation : insérez la cartouche de résine dans une imprimante 3D Formlabs compatible.
Insérez le bac à résine et fixez le mélangeur au bac.
3. Impression :a. Préparez une tâche d’impression à l’aide du logiciel PreForm. Importez le fichier STL
de la pièce souhaitée.
b. Procédez à l’orientation et générez les supports.
c. Envoyez la tâche d’impression à l’imprimante.
d. Démarrez l’impression en sélectionnant la tâche d’impression dans le menu d’impression.
Suivez toutes les instructions ou boîtes de dialogue affichées sur l’écran de l’imprimante.
L’imprimante va automatiquement effectuer l’impression.

B. RETRAIT DES PIÈCES
Retirez la plateforme de fabrication de l’imprimante. Pour retirer les pièces, calez l’outil pour retirer lespièces de la plateforme sous la base de chaque pièce imprimée et faites tourner l’outil. La Build Platform 2
ou la Build Platform 2L de Formlabs peuvent être utilisées pour un retrait facile et sans outil. Pour destechniques plus détaillées, consultez support.formlabs.com.

FRANÇAIS

Dental LT Clear Resin (V2) est une résine à base de polymère photopolymérisable conçue pourréaliser par fabrication additive des dispositifs dentaires et orthodontiques amovibles biocompatibles
pour usage à long terme, tels que des gouttières occlusales, des appareils de nuit, des protège-dents
et/ou des gouttières de blanchiment. Ce guide de fabrication fournit des recommandations et desexigences en matière d’équipement, d’impression et de post-traitement afin de garantir une utilisation
correcte et sans danger de ce matériau.

C. LAVAGE
Placez les pièces imprimées dans une unité de lavage validée par Formlabs avec de l’alcool
isopropylique à 99 %.
1. Form Wash, Form Wash (2e génération) - Grande vitesse* ou Form Wash L :a. Lavez la pièce dans la Form Wash ou la Form Wash L pendant 15 minutes ou jusqu’à ce qu’elle
soit propre.
b. Retirez les pièces de l’unité de lavage et laissez-les tremper dans de l’alcool isopropyliquepropre pendant 5 minutes.
c. Si les pièces ne semblent pas propres après le lavage, envisagez de remplacer l’alcool
isopropylique usagé dans l’unité de lavage par du solvant propre.
*Les paramètres de grande vitesse de la Form Wash (2e génération) sont validés pour l’utilisation.
2. Unité de lavage à ultrasons :REMARQUE : L’utilisation d’alcool isopropylique dans un bain à ultrasons présente un risqued’incendie ou d’explosion. Lors de l’utilisation d’un appareil de lavage à ultrasons, lisez et respectez
toutes les recommandations de sécurité du fabricant de l’appareil.
a. Utilisez de l’alcool isopropylique propre à 99 % pour chaque lavage.
b. Placez les pièces dans un récipient secondaire en plastique jetable ou dans un sac en
plastique refermable, puis remplissez-le d’alcool isopropylique à 99 %, en veillant à ce que lespièces soient entièrement immergées.
c. Placez le récipient secondaire dans le bain de l’unité à ultrasons et effectuez la sonication
pendant 2 minutes ou jusqu’à ce que la pièce soit propre*.
* L’efficacité du lavage dépend de la taille et de la puissance de l’appareil à ultrasons. Les essaisde Formlabs ont été réalisés avec des appareils à ultrasons de 36 W/L ou plus.

D. SÉCHAGE
1. Retirez les pièces de l’alcool isopropylique et laissez-les sécher à l’air libre à températureambiante pendant au moins 30 minutes. REMARQUE : Les temps de séchage peuvent varier enfonction du design des pièces et des conditions ambiantes. Ne laissez pas les pièces reposerdans l’alcool isopropylique plus longtemps que nécessaire.
2. Inspectez les pièces imprimées afin de vérifier qu’elles sont bien propres et sèches. Leurs surfaces
doivent impérativement être débarrassées de tout reste de solvant, résine liquide en excès ou
particules résiduelles avant de passer aux étapes suivantes.
3. Si du solvant résiduel est encore présent, faites sécher les pièces plus longtemps. Si des résidus
de résine sont encore visibles, lavez à nouveau les pièces jusqu’à ce qu’elles soient propreset sèches.

E. POST-POLYMÉRISATION
Placez les pièces imprimées dans une unité de post-polymérisation validée par Formlabs etpolymérisez-les pendant la durée requise.
1. Form Cure ou Form Cure L :a. Polymérisez les pièces pendant 60 minutes à 60 °C.
b. Laissez la Form Cure ou la Form Cure L refroidir jusqu’à température ambiante entre les cycles
de polymérisation.
2. Fast Cure :a. Polymérisez les pièces pendant 6 minutes à l’intensité lumineuse 5.
b. Laissez la Fast Cure refroidir pendant 10 minutes au minimum entre les cycles de polymérisation.

F. RETRAIT DES SUPPORTS ET POLISSAGE
1. Les traces de support peuvent provoquer une abrasion si elles ne sont pas retirées et polies.
Retirez les supports à l’aide d’un disque de coupe et d’une pièce à main, d’une pince coupante ou
d’autres outils de finition appropriés.
2. Polissez les dispositifs imprimés à l’aide des méthodes de polissage dentaire habituelles avant
utilisation par le patient.
3. Vérifiez que les pièces ne sont pas fissurées. En cas de dommage ou de fissure, jetez-les.

G. NETTOYAGE ET DÉSINFECTION
1. Une fois le post-traitement terminé, les pièces peuvent être nettoyées avec une brosse à dents
souple dédiée, un savon neutre et de l’eau à température ambiante. N’utilisez pas de dentifrice ou
d’autres produits de nettoyage sur les pièces imprimées avec Dental LT Clear Resin (V2).
2. Les dispositifs peuvent être nettoyés et désinfectés dans le respect des protocoles del’établissement. Méthode de désinfection testée : trempage du dispositif fini dans de l’alcool
isopropylique propre à 70 % pendant 5 minutes. Ne laissez pas la pièce dans une solution d’alcool
pendant plus de 5 minutes.
3. Après le nettoyage et la désinfection, vérifiez que la pièce n’est pas endommagée ou fissurée afin
de vous assurer que l’intégrité de la pièce conçue répond aux exigences de performance. En cas
de dommage ou de fissure, jetez la pièce.

H. DANGERS, STOCKAGE ET ÉLIMINATION
1. La résine polymérisée n’est pas dangereuse et peut être éliminée avec les déchets ordinaires.
2. Pour plus d’informations, consultez la FDS sur le site support.formlabs.com.

Considerazioni specifiche sulla produzione
Le specifiche relative alla Dental LT Clear Resin (V2) sono state convalidate utilizzando l’hardwaree i parametri indicati di seguito. Al fine di garantire la conformità alle direttive di biocompatibilità,la convalida è stata eseguita utilizzando un serbatoio resina, un miscelatore, una piattaforma distampa, un’unità di lavaggio e un’attrezzatura di post-elaborazione dedicati, non usati con altre resine.

1. Hardware:a. Stampante 3D Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Accessori per la stampa: piattaforme di stampa Formlabs, serbatoi resina Formlabs

2. Software:a. PreForm di Formlabs

3. Parametri di stampa:
a. Orientamento delle parti: superfici a intaglio rivolte in direzione opposta rispetto alla piattaforma
di stampa, con un’inclinazione compresa tra 0 e 40°
b. Spessore dello strato: 100 μm
c. Spessore della parte:• Superfici occlusali: minimo 2 mm
• Pareti: minimo 1 mm

4. Attrezzatura e accessori raccomandati per la post-elaborazione:a. Accessori di lavorazione Formlabs: Form Auto, Resin Pumping Systemb. Unità di lavaggio convalidata Formlabs: Form Wash, Form Wash (seconda generazione),
Form Wash L, unità di lavaggio a ultrasuonic. Unità di polimerizzazione convalidata Formlabs: Form Cure, Form Cure L, Fast Cure

A. STAMPA
1. Agitazione della cartuccia: agita la cartuccia prima di ogni lavoro di stampa. Nel caso in cuila cartuccia non sia stata agitata a sufficienza potrebbero verificarsi variazioni cromatiche ederrori di stampa.
2. Impostazione: inserisci la cartuccia di resina in una stampante 3D Formlabs compatibile.
Inserisci il serbatoio resina e collega il miscelatore al serbatoio.
3. Stampa:
a. Prepara un lavoro di stampa utilizzando il software PreForm. Importa il file STL
della parte desiderata.
b. Orienta e genera i supporti.
c. Invia il lavoro di stampa alla stampante.
d. Avvia la stampa selezionando il lavoro di stampa dall’apposito menu. Segui le istruzioni ole finestre di dialogo visualizzate sullo schermo della stampante. La stampante completerà
la stampa in modo automatico.

B. RIMOZIONE DELLE PARTI
Rimuovi la piattaforma di stampa dalla stampante. Per rimuovere le parti, inserisci l’apposito strumento
sotto la base della parte stampata e ruotalo. Usa la Build Platform 2 o la Build Platform 2L di Formlabs
per una rimozione semplice e senza strumenti. Per tecniche dettagliate, visita support.formlabs.com.

C. LAVAGGIO
Posiziona le parti stampate in un’unità di lavaggio convalidata da Formlabs con alcool isopropilico
al 99%.

ITALIANOLa Dental LT Clear Resin (V2) è una resina a base di polimeri fotopolimerizzabili progettata per lafabbricazione, mediante la produzione additiva, di apparecchi odontoiatrici e ortodontici estraibili,
come bite occlusali e per uso notturno, paradenti e/o mascherine per lo sbiancamento, che siano
biocompatibili e adatti per un utilizzo a lungo termine. Consulta questa guida alla produzione perconoscere le raccomandazioni e i requisiti in merito a stampa, post-elaborazione e apparecchi,
al fine di garantire l’uso corretto e sicuro di questo materiale.

1. Form Wash, Form Wash (seconda generazione)* o Form Wash L:
a. Lava le parti in una Form Wash o Form Wash L per 15 minuti o finché non sono pulite.
b. Rimuovi le parti dall’unità di lavaggio e immergile in alcool isopropilico pulito per cinque minuti.
c. Se le parti non risultano pulite dopo il lavaggio, sostituisci l’alcool isopropilico con solvente pulito.
*Per la Form Wash (seconda generazione), le impostazioni di alta velocità sono convalidate per l’uso.
2. Unità di lavaggio a ultrasuoni:
NOTA: l’utilizzo di alcool isopropilico in un bagno a ultrasuoni presenta un rischio di incendio oesplosione. Quando utilizzi un lavaggio ad ultrasuoni, leggi e segui tutte le disposizioni di sicurezza
fornite dall’azienda produttrice.
a. Utilizza alcool isopropilico al 99% pulito in ogni lavaggio.
b. Posiziona le parti in un contenitore in plastica monouso secondario o in un sacchetto diplastica richiudibile, quindi versa alcool isopropilico al 99% assicurandoti che le parti sianocompletamente immerse.
c. Posiziona il contenitore secondario nel bagno d’acqua dell’unità a ultrasuoni e applica gli
ultrasuoni per due minuti o finché le parti non sono pulite.**L’efficacia del lavaggio dipende dalle dimensioni e dalla potenza dell’unità a ultrasuoni. I test di
Formlabs sono stati condotti con unità a ultrasuoni a una potenza di 36 W/L o superiore.

D. ASCIUGATURA
1. Rimuovi le parti dall’alcool isopropilico e lasciale asciugare a temperatura ambiente per almeno
30 minuti. NOTA: i tempi di asciugatura possono variare a seconda del design delle parti
e delle condizioni ambientali. Non lasciare le parti immerse nell’alcool isopropilico più a lungodel necessario.
2. Ispeziona le parti stampate per assicurarti che siano pulite e asciutte. Prima di passare alle fasi
successive, accertati che sulla superficie non sia rimasto alcun residuo di solvente, resina liquidain eccesso o frammenti.
3. Se noti residui di solvente, lascia asciugare le parti più a lungo. Se noti residui di resina, lava
nuovamente le parti finché non saranno pulite e asciutte.

E. POLIMERIZZAZIONE POST-STAMPA
Posiziona le parti stampate in un’unità di polimerizzazione post-stampa convalidata da Formlabs ed
esegui la polimerizzazione per il tempo richiesto.
1. Form Cure o Form Cure L:
a. Polimerizza per 60 minuti a 60 °C.
b. Lascia che l’unità Form Cure o Form Cure L si raffreddi fino a temperatura ambiente tra un ciclo
di polimerizzazione e il successivo.
2. Fast Cure:a. Polimerizza per sei minuti con intensità luminosa pari a 5.
b. Lascia raffreddare l’unità Fast Cure per almeno dieci minuti tra un ciclo di polimerizzazione
e il successivo.

F. RIMOZIONE DEI SUPPORTI E LUCIDATURA
1. I segni lasciati dai supporti possono causare abrasioni se non vengono rimossi e lucidati.
Rimuovi i supporti utilizzando un disco da taglio e un manipolo, una tronchesina o altri strumenti
di finitura appropriati.
2. Prima dell’uso da parte dei pazienti, lucida gli apparecchi stampati usando i tipici metodi dilucidatura odontoiatrica.
3. Ispeziona le parti per individuare eventuali crepe. Scarta le parti se rilevi danni o crepe.

G. PULIZIA E DISINFEZIONE
1. Le parti completamente post-elaborate possono essere pulite usando un apposito spazzolino dadenti morbido, con sapone neutro e acqua a temperatura ambiente. Non usare dentifricio o altri
detergenti sulle parti stampate con la Dental LT Clear Resin (V2).

2. Gli apparecchi possono essere puliti e disinfettati secondo i protocolli della struttura. Metodo didisinfezione testato: immersione dell’apparecchio in alcool isopropilico al 70% pulito per cinqueminuti. Non lasciare la parte nella soluzione di alcool per più di cinque minuti.
3. Dopo la pulizia e la disinfezione, ispeziona la parte per verificare la presenza di eventuali danni ocrepe e assicurarti che l’integrità della parte progettata soddisfi i requisiti di prestazione. Scarta leparti se rilevi danni o crepe.

H. PERICOLI, CONSERVAZIONE E SMALTIMENTO
1. La resina polimerizzata non è pericolosa e può essere smaltita come un rifiuto comune.
2. Per ulteriori informazioni, consulta la scheda dati di sicurezza all’indirizzo support.formlabs.com.

Consideraciones específicas de fabricación
Las especificaciones de la Dental LT Clear Resin V2 se han validado utilizando el hardware y losparámetros indicados a continuación. Para verificar la biocompatibilidad de la resina, el proceso devalidación utilizó un tanque de resina, un mezclador, una base de impresión, una unidad de lavado yequipamiento de posacabado dedicados expresamente al material, que no se mezclaron con ninguna
otra resina.

1. Hardware:a. Impresora 3D de Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Accesorios de impresión: Bases de impresión de Formlabs, tanques de resina de Formlabs

2. Software:a. PreForm de Formlabs

3. Parámetros de impresión:a. Orientación de la pieza: La superficie interior debe apuntar en sentido contrario a la basede impresión, con una inclinación de 0-40°
b. Grosor de capa: 100 μm
c. Grosor de la pieza:• Superficies oclusales: 2 mm mínimo
• Paredes: 1 mm mínimo

4. Equipamiento y accesorios recomendados para el posacabado:a. Accesorios de procesamiento de Formlabs: Form Auto, Resin Pumping Systemb. Unidad de lavado validada por Formlabs: Form Wash, Form Wash (2.ª generación), Form Wash L,
unidad de limpieza ultrasónica
c. Unidad de curado validada por Formlabs: Form Cure, Form Cure L, Fast Cure

A. IMPRESIÓN
1. Agitado del cartucho: Agita el cartucho antes de cada trabajo de impresión. Pueden darse
divergencias en el color y fallos de impresión si no se agita el cartucho lo suficiente.
2. Preparación: Inserta el cartucho de resina en una impresora 3D compatible de Formlabs.
Introduce el tanque de resina y acopla el mezclador al tanque.
3. Impresión:a. Prepara una impresión utilizando el software PreForm. Importa el archivo STL de la pieza deseada.
b. Orienta y genera los soportes.
c. Envía tu proyecto a la impresora.
d. Inicia la impresión seleccionando un proyecto en el menú de impresión. Sigue las instrucciones
o los diálogos que aparezcan en la pantalla de la impresora. La impresora completará
automáticamente la impresión.

B. EXTRACCIÓN DE LA PIEZA
Retira la base de impresión de la impresora. Para quitar las piezas de la base de impresión, coloca laherramienta para retirar piezas debajo de la base de la pieza impresa y gira la herramienta. Se puede
utilizar la Build Platform 2 o la Build Platform 2L de Formlabs para asegurar una extracción sencillay sin herramientas. Si deseas conocer las técnicas con detalle, visita support.formlabs.com.

C. LAVADO
Coloca las piezas impresas en una unidad de lavado validada por Formlabs con alcohol isopropílico
al 99 %.

ESPAÑOLLa Dental LT Clear Resin V2 es una resina fotopolimerizable diseñada para la fabricación aditiva deaparatos dentales y para ortodoncia removibles, biocompatibles y para un uso prolongado, como
férulas oclusales, férulas de descarga, protectores bucales y/o cubetas de blanqueamiento. Esta
guía de fabricación ofrece recomendaciones y requisitos de equipamiento, impresión y posacabadopara garantizar el uso correcto y seguro de este material.

1. Form Wash, Form Wash (2.ª generación) a alta velocidad* o Form Wash L:
a. Lava las piezas en la Form Wash o la Form Wash L durante 15 minutos o hasta que estén limpias.
b. Retira las piezas de la unidad de lavado y báñalas en alcohol isopropílico limpio durante 5 minutos.
c. Si las piezas no parecen estar limpias después del lavado, considera reemplazar el alcohol
isopropílico usado de la unidad de lavado por disolvente nuevo.
*En el caso de la Form Wash (2ª generación), los ajustes de alta velocidad están validados para su uso.
2. Unidad de limpieza ultrasónica:
NOTA: Utilizar alcohol isopropílico en un baño ultrasónico presenta un riesgo de incendio o explosión.
Cuando utilices un baño ultrasónico, lee y sigue todas las recomendaciones de seguridad delfabricante del baño ultrasónico.
a. Utiliza alcohol isopropílico al 99 % para cada limpieza.
b. Coloca las piezas en un recipiente de plástico desechable secundario o en una bolsa deplástico con cierre resellable y, a continuación, llénalo con alcohol isopropílico al 99 %,asegurándote de que las piezas queden totalmente sumergidas.
c. Coloca el recipiente secundario en el baño de agua de la unidad ultrasónica y somete laspiezas a ultrasonidos durante 2 minutos o hasta que estén limpias.**La eficacia del lavado depende del tamaño y la potencia de la unidad ultrasónica. Los ensayos
de Formlabs se realizaron con unidades ultrasónicas a 36 W/L o más.

D. SECADO
1. Saca las piezas del alcohol isopropílico y deja que se sequen al aire a temperatura ambiente
durante como mínimo 30 minutos. NOTA: Los tiempos de secado pueden variar según el diseño
de las piezas y las condiciones ambientales. No dejes las piezas en alcohol isopropílico mástiempo del necesario.
2. Inspecciona las piezas impresas para asegurarte de que estén limpias y secas. No deberían
quedar residuos de disolvente, resina líquida sobrante ni partículas residuales en la superficie
antes de pasar a pasos posteriores.
3. Si todavía queda disolvente residual, seca las piezas durante más tiempo. Si todavía hay residuos
de resina visibles, vuelve a lavar las piezas hasta que estén limpias y secas.

E. POSCURADO
Coloca las piezas impresas en una unidad de poscurado validada por Formlabs y cúralas durante eltiempo necesario.
1. Form Cure o Form Cure L:
a. Realiza un curado durante 60 minutos a 60 °C
b. Deja que la Form Cure o la Form Cure L se enfríe hasta la temperatura ambiente entre ciclos
de curado.
2. Fast Cure:a. Realiza un curado durante 6 minutos a intensidad de luz 5
b. Deja que la Fast Cure se enfríe durante al menos 10 minutos entre ciclos de curado.

F. RETIRADA Y PULIDO DE SOPORTES
1. Las marcas de los soportes pueden causar abrasión si no se eliminan y se pulen. Retira lossoportes utilizando un disco de corte y una fresa de mano, alicates de corte u otras herramientas
de acabado adecuadas.
2. Pule los aparatos que imprimas con los métodos de pulido odontológicos habituales antes de que
los usen los pacientes.
3. Inspecciona las piezas para comprobar que no tengan grietas. Desecha las piezas si detectas
daños o grietas.

G. LIMPIEZA Y DESINFECCIÓN
1. Las piezas que ya hayan pasado por un posacabado completo se pueden limpiar con un cepillo
de dientes suave de uso exclusivo para ello, con jabón neutro y agua a temperatura ambiente.

No uses pasta de dientes ni ningún otro producto de limpieza con las piezas impresas
con la Dental LT Clear Resin V2.
2. Los aparatos se pueden limpiar y desinfectar de acuerdo con los protocolos del establecimiento.
Método de desinfección probado: consiste en sumergir el aparato acabado en alcohol isopropílico
nuevo al 70 % durante 5 minutos. No dejes la pieza sumergida en la solución alcohólica durantemás de 5 minutos.
3. Después de la limpieza y la desinfección, inspecciona la pieza para comprobar que no tiene
daños o grietas y que su integridad satisface los requisitos de rendimiento. Desecha las piezas si
detectas daños o grietas.

H. PELIGROS, ALMACENAMIENTO Y ELIMINACIÓN
1. La resina curada no es peligrosa y se puede desechar junto con los residuos habituales.
2. Si necesitas más información, consulta las FDS en support.formlabs.com.

Considerações específicas de fabricoAs especificações da Dental LT Clear V2 Resin foram validadas utilizando o hardware e os parâmetros
indicados abaixo. Para garantir a conformidade com a biocompatibilidade, a validação utilizou um
tanque de resina e um misturador dedicados, uma plataforma de impressão, uma unidade de lavagem
e equipamento de pós-processamento que não foram misturados com quaisquer outras resinas.

1. Hardware:a. Impressora 3D Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Acessórios de impressão: plataformas de impressão Formlabs, tanques de resina Formlabs

2. Software:a. PreForm da Formlabs

3. Parâmetros de impressão:a. Orientação da peça: superfície com entalhe voltada para fora da plataforma de impressão com umângulo de inclinação de 0-40°.
b. Espessura da camada: 100 μm
c. Espessura da peça:• Superfícies oclusais: 2 mm no mínimo
• Paredes: 1 mm no mínimo

4. Equipamento e acessórios de pós-processamento recomendados:a. Acessórios de processamento Formlabs: Form Auto, sistema de bombeamento de resina
b. Unidade de lavagem validada Formlabs: Form Wash, Form Wash (2.ª geração), Form Wash L,
unidade de lavagem por ultrassonsc. Equipamento de cura validado pela Formlabs: Form Cure, Form Cure L, Fast Cure

A. IMPRESSÃO
1. Agitar o cartucho: agitar o cartucho antes de cada trabalho de impressão. Podem ocorrer
divergências de cor e falhas na impressão se o cartucho não for bem agitado.
2. Configuração: Introduzir o depósito de resina e ligar o misturador ao depósito.
3. Impressão:a. Prepare uma impressão usando o software PreForm. Importe ficheiro STL da peça desejada.
b. Oriente e gira os suportes.
c. Envie o trabalho de impressão para a impressora.
d. Comece a impressão selecionando um trabalho de impressão no menu de impressão. Sigaquaisquer indicações ou diálogos mostrados no ecrã da impressora. A impressora concluirá
automaticamente a impressão.

B. REMOÇÃO DE PEÇAS
Remova a plataforma de impressão da impressora. Para remover peças da plataforma de impressão,coloque a ferramenta de remoção de peças sob a base de peças impressas e rode a ferramenta.
A Formlabs Build Platform 2 ou Build Platform 2L pode ser utilizada para uma remoção fácil e sem
ferramentas. Para técnicas detalhadas, consulte support.formlabs.com.

C. LAVAGEM
Colocar as peças impressas num equipamento unidade de lavagem validado pela Formlabs com
álcool isopropílico a 99%.

PORTUGUÊS

A Dental LT Clear V2 Resin é uma resina à base de polímeros fotopolimerizáveis concebidapara o fabrico de aparelhos dentários e odontológicos amovíveis biocompatíveis e de utilização
prolongada, tais como placas oclusais, placas miorrelaxantes, protetores bucais e/ou moldeirasde branqueamento, através de fabrico aditivo. Este Guia do Fabricante fornece recomendações
e requisitos relativos ao equipamento, impressão e pós-processamento para garantir a utilização
correta e segura deste material.

1. Form Wash, Form Wash (2.ª geração) - Alta velocidade* ou Form Wash L:
a. Lavar durante 15 minutos ou até estar limpo, na Form Wash ou Form Wash L.
b. Remova as peças do equipamento de lavagem e mergulhe em álcool isopropílico novo
durante 5 minutos.
c. Se as peças não parecerem limpas após a lavagem, considere a substituição do álcool
isopropílico usado na unidade de lavagem por solvente novo.
*Para a Form Wash (2.ª geração), são validadas para utilização as definições de alta velocidade.
2. Unidade de lavagem por ultrassons:
NOTA: a utilização de álcool isopropílico num banho de ultrassons provoca risco de incêndio ou
explosão. Quando utilizar uma lavagem por ultrassons, leia e siga todas as recomendações desegurança do fabricante da lavagem por ultrassons.
a. Utilizar álcool isopropílico novo a 99% para cada lavagem.
b. Colocar as peças num recipiente de plástico descartável secundário ou num saco de plásticoque possa voltar a ser fechado e encher com álcool isopropílico a 99%, assegurando que as
peças ficam totalmente submersas.
c. Colocar o recipiente secundário no banho de água do equipamento de ultrassons e aplicar
ultrassons durante 2 minutos ou até estar limpo.**A eficácia da lavagem depende do tamanho e da potência do equipamento de ultrassons. Os testes
da Formlabs foram realizados com unidades de ultrassons a 36 W/L ou mais.

D. SECAGEM
1. Retirar as peças do álcool isopropílico e deixar secar ao ar, à temperatura ambiente, durante
pelo menos 30 minutos. Observação: os tempos de secagem podem variar em função do design
das peças e das condições ambientais. Não deixar as peças em álcool isopropílico durante mais
tempo do que o necessário.
2. Inspecione as peças impressas para assegurar que estas estão limpas e secas. A superfície não
deve apresentar resíduos de solvente, excesso de resina líquida ou resíduos de partículas antes
de prosseguir com os passos seguintes.
3. Se ainda estiverem presentes resíduos de solvente deixe as peças secar mais tempo. Se ainda
estiverem visíveis resíduos de resina, volte a lavar as peças até ficarem limpas e deixe secar.

E. PÓS-CURA
Colocar as peças impressas num equipamento de pós-cura validado pela Formlabs e curar durante o
tempo necessário.
1. Form Cure ou Form Cure L:
a. Cura durante 60 minutos a 60 °C
b. Deixar o equipamento Form Cure ou Form Cure L arrefecer até à temperatura ambiente entre
os ciclos de cura.
2. Cura rápida:a. Cura durante 6 minutos a uma intensidade luminosa de 5b. Deixar o equipamento Fast Cure arrefecer durante pelo menos 10 minutos entre os ciclos de cura.

F. REMOÇÃO DE SUPORTES E POLIMENTO
1. As marcas de suporte podem causar abrasão se não forem removidas e polidas. Removeros suportes utilizando um disco de corte e uma peça de mão, um alicate de corte ou outras
ferramentas de acabamento adequadas.
2. Polir os aparelhos impressos utilizando os métodos de polimento dentário habituais antes dautilização pelo paciente.
3. Inspecione as peças para verificar se existem fendas. Descarte se forem detetados danos ou fendas.

G. LIMPEZA E DESINFEÇÃO
1. As peças totalmente pós-processadas podem ser limpas utilizando uma escova de dentes macia
apenas para esse fim, sabão neutro e água à temperatura ambiente. Não utilize pasta de dentes
ou quaisquer outros produtos de limpeza em peças impressas com Dental LT Clear V2 Resin.

2. Os guias podem ser limpos e desinfetados de acordo com os protocolos de instalação. Método
de desinfeção testado: mergulhar o guia acabado em álcool isopropílico novo a 70 % durante
5 minutos. Não deixe a peça em solução de álcool por um período superior a 5 minutos.
3. Após a limpeza e desinfeção, inspecione a peça quanto a danos ou fissuras para garantir que
a integridade da peça concebida cumpre os requisitos de desempenho. Descarte se forem
detetados danos ou fendas.

H. PERIGOS, ARMAZENAMENTO E ELIMINAÇÃO
1. A resina curada não é perigosa e pode ser descartada como lixo comum.
2. Consulte a FDS para obter mais informações em support.formlabs.com.

Specifieke productieoverwegingen
De specificaties van Dental LT Clear V2 Resin zijn gevalideerd met de hieronder aangegeven hardwareen parameters. Voor de naleving van de biocompatibiliteit werden bij de validatie een speciale harstank,een bouwplatform, een wasinstallatie en nabewerkingsapparatuur gebruikt die niet met andere harsen
werden gemengd.

1. Hardware:a. Formlabs 3D-printer: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Printaccessoires: Formlabs Build Platforms, Formlabs harstanks

2. Software:a. Formlabs PreForm

3. Printparameters:a. Oriëntatie onderdeel: Intagliovlak afgewend van het bouwplatform in een gekantelde hoek van
0 - 40°b. Laagdikte: 100 μm
c. Dikte onderdeel:• Occlusale oppervlakken: minimaal 2 mm
• Muren: 1 mm minimaal

4. Aanbevolen nabewerkingsapparatuur en accessoires:a. Verwerkingsaccessoires van Formslabs: Form Auto, Resin Pumping Systemb. Formlabs gevalideerde wasinstalltie: Form Wash, Form Wash (2e generatie), Form Wash L,
Ultrasonic Wash Unitc. Formlabs gevalideerde uithardingsunit: Form Cure, Form Cure L, Fast CureA. PRINTEN
1. Cartridge schudden: Schud de cartridge voor elke afdruktaak. Er kunnen zich kleurafwijkingen en
printgebreken voordoen als de cartridge onvoldoende wordt geschud.
2. Set up: Plaats de harstank en bevestig de mixer aan de tank.
3. Printen:
a. Bereid een printopdracht voor met behulp van de PreForm-software. Importeer het gewenste
STL-bestand voor het onderdeel.
b. Oriënteer en genereer ondersteuningen.
c. Stuur de printopdracht naar de printer.
d. Begin met printen door een printtaak te selecteren in het printmenu. Volg alleaanwijzingen of dialoogvensters die op het printerscherm verschijnen. De printer zal het
printen automatisch voltooien.

B. ONDERDELEN VERWIJDEREN
Verwijder het bouwplatform van de printer. Om onderdelen van het bouwplatform te verwijderen, klemt
u het instrument voor het verwijderen van onderdelen onder het geprinte onderdeel en draait u het
gereedschap. Formlabs Build Platform 2 of Build Platform 2L kan worden gebruikt voor eenvoudige
verwijdering zonder gereedschap. Raadpleeg support.formlabs.com voor gedetailleerde technieken.

C. SPOELEN
Plaats de geprinte onderdelen in een door Formlabs gevalideerde wasunit met 99% isopropylalcohol.
1. Form Wash, Form Wash (2e generatie) - hoge snelheid*, of Form Wash L:a. Was 15 minuten of tot ze schoon zijn in Form Wash of Form Wash L.
b. Haal de onderdelen uit de wasunit en laat ze 5 minuten weken in verse isopropylalcohol.

NEDERLANDS

Dental LT Clear V2 Resin is een lichtuithardende hars op polymeerbasis, ontworpen voor devervaardiging van biocompatibele, verwijderbare tandheelkundige en orthodontische hulpmiddelenvoor langdurig gebruik, zoals occlusale spalken, nachtbeschermers, gebitsbeschermers en/of
bleeklepels door middel van additieve productie. Deze productiegids geeft aanbevelingen voor
apparatuur, afdrukken en nabewerking en vereisten voor een correct en veilig gebruik van dit materiaal.

c. Als onderdelen na het wassen niet schoon lijken, kunt u overwegen om de gebruikte
isopropylalcohol in de waseenheid te vervangen door een vers oplosmiddel.
*Voor Form Wash (2e generatie) zijn de instellingen voor hoge snelheid gevalideerd voor gebruik.
2. Ultrasone wasunit:
OPMERKING: Het gebruik van isopropylalcohol in een ultrasoon bad houdt een risico van brand of
explosie in. Wanneer u een ultrasone wassing gebruikt, moet u alle veiligheidsaanbevelingen van defabrikant van de ultrasone wassing lezen en opvolgen.
a. Gebruik schone 99% isopropylalcohol voor elke wassing.
b. Plaats de onderdelen in een tweede plastic wegwerpcontainer of plastic hersluitbare zak en
vul deze met 99% isopropylalcohol, zodat de onderdelen volledig ondergedompeld zijn.
c. Plaats de secundaire container in het waterbad van de ultrasone eenheid en soniceer
gedurende 2 minuten of tot hij schoon is.**De wasefficiëntie hangt af van de grootte en het vermogen van de ultrasone unit. Formlabs testte
met ultrasone units bij 36 W/l of hoger.

D. DROGEN
1. Haal de onderdelen uit de isopropylalcohol en laat ze ten minste 30 minuten bij kamertemperatuur
aan de lucht drogen. OPMERKING: De droogtijd kan variëren afhankelijk van het ontwerp
van onderdelen en omgevingsomstandigheden. Laat onderdelen niet langer dan nodig in
isopropylalcohol zitten.
2. Inspecteer de geprinte onderdelen om te controleren of deze schoon en droog zijn. Er mogen
geen resten oplosmiddel, overtollige vloeibare hars of residudeeltjes op het oppervlak
achterblijven voordat met de volgende stappen wordt begonnen.
3. Als het resterende oplosmiddel nog aanwezig is, laat de onderdelen langer drogen. Als er nog
harsresten zichtbaar zijn, reinigt u de onderdelen opnieuw totdat ze schoon zijn en laat u ze drogen.

E. UITHARDEN
Plaats de geprinte onderdelen in een door Formlabs gevalideerde post-uithardingsunit en laat ze
gedurende de vereiste tijd uitharden.
1. Form Cure of Form Cure L:
a. Uitharden gedurende 60 minuten bij 60 °C
b. Laat de Form Cure of Form Cure L-unit tussen twee uithardingscycli afkoelen tot kamertemperatuur.
2. Snelle uitharding:a. 6 minuten uitharden bij lichtintensiteit 5b. Laat de Fast Cure-unit tussen de uithardingscycli minstens 10 minuten afkoelen.

F. ONDERSTEUNING VERWIJDEREN & POLIJSTEN
1. Steunsporen kunnen slijtage veroorzaken als ze niet worden verwijderd en gepolijst.
Verwijder ondersteuningen met behulp van een snijschijf en handstuk, een snijtang of
ander geschikt afwerkingsgereedschap.
2. Polijst de geprinte hulpmiddelen met de gebruikelijke tandpolijstmethoden vóór gebruik doorde patiënt.
3. Controleer de onderdelen op scheuren. Gooi een onderdeel weg indien er beschadigingen of
scheuren worden geconstateerd.

G. REINIGING EN DESINFECTIE
1. Volledig nabewerkte onderdelen kunnen worden gereinigd met een speciale zachte
tandenborstel met neutrale zeep en water op kamertemperatuur. Gebruik geen schurendeschoonmaakproducten op met Dental LT Clear V2 Resin geprinte onderdelen.
2. De apparaten kunnen worden gereinigd en gedesinfecteerd volgens de protocollen van defaciliteit. Geteste desinfectiemethoden omvatten ook het 5 minuten onderdompelen van detoestellen in een verse IPA-oplossing van 70%. Laat het onderdeel niet langer dan 5 minuten in
een alcoholoplossing liggen.

3. Inspecteer het onderdeel na reiniging en desinfectie op schade of barsten om ervoor te zorgen
dat de integriteit van het ontworpen onderdeel voldoet aan de prestatie-eisen. Gooi een onderdeel
weg indien er beschadigingen of scheuren worden geconstateerd.

H. GEVAREN, OPSLAG EN VERWIJDERING
1. Uitgeharde kunsthars is ongevaarlijk en kan bij het normale afval worden weggegooid.
2. Zie SDS voor meer informatie op support.formlabs.com.

Særlige forhold i forbindelse med fremstilling
Specifikationerne for Dental LT Clear V2 Resin er blevet valideret ved hjælp af den hardware og deparametre, der er angivet nedenfor. For at overholde biokompatibiliteten brugte valideringen en
dedikeret resintank og mixer, byggeplatform, vaskeenhed og efterbehandlingsudstyr, som ikke var
blandet med andre resiner.

1. Hardware:a. Formlabs 3D-printer: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Printtilbehør: Formlabs Build Platforms, Formlabs Resin Tanks

2. Software:a. Formlabs PreForm

3. Printparametre:a. Orientering: Dybtrykt overflade, der vender væk fra byggeplatformen ved en skrå vinkel på 0-40°
b. Lagtykkelse: 100 μm
c. Delens tykkelse:• Okklusale flader: mindst 2 mm
• Vægge: mindst 1 mm

4. Anbefalet udstyr og tilbehør til efterbehandling:a. Formlabs Processing tilbehør: Form Auto, Resin Pumping Systemb. Formlabs valideret vaskeenhed: Form Wash, Form Wash (2. generation), Form Wash L,
Ultralydsvaskeenhedc. Formlabs’ godkendte hærdningsstation: Form Cure, Form Cure L, Fast CureA. PRINTNING
1. Ryst patronen: Ryst patronen før hvert printjob. Farveafvigelser og udskrivningsfejl kan forekomme,
hvis patronen ikke rystes nok.
2. Opsætning: Indsæt resinpatronen i en kompatibel Formlabs 3D-printer. Sæt resintanken i,og fastgør mixeren til beholderen.
3. Printning:a. Forbered en printopgave ved hjælp af PreForm-software. Importér STL-filen for den ønskede del.
b. Tilpas retning, og generer støttestrukturer.
c. Send printjobbet til printeren.
d. Start printningen ved at vælge et printjob i printmenuen. Følg beskeder eller dialogbokse,der vises på printerskærmen. Printeren gennemfører automatisk printet.

B. UDTAGNING AF DELE
Fjern konstruktionsplatformen fra printeren. Delen fjernes fra konstruktionsplatformen ved at kile
udtagningsværktøjet ind under den printede del og dreje værktøjet. Formlabs Build Platform 2 eller
Formlabs Build Platform 2L kan bruges til nem, udtagning uden værktøj. Du kan finde udførlige
fremgangsmåder på support.formlabs.com.

C. VASK
Placer de printede dele i en Formlabs-valideret vaskeenhed med 99 % isopropylalkohol.
1. Form Wash, Form Wash (2. generation) – High speed* eller Form Wash L
a. Vask i 15 minutter, eller indtil de er rene i Form Wash eller Form Wash L.
b. Fjern delene fra vaskeenheden, og læg dem i blød i frisk isopropylalkohol i 5 minutter.
c. Hvis delene ikke ser rene ud efter vask, skal du overveje at udskifte den brugte
isopropylalkohol i vaskeenheden med frisk opløsningsmiddel.

DANSK

Dental LT Clear V2 Resin er en lyshærdende polymerbaseret resin designet til fremstilling af biokompatible,
aftagelige tand- og tandreguleringsapparater til langvarig brug, såsom okklusionsskinner, natbøjler,
tandbeskyttere og/eller blegebakker ved hjælp af additiv fremstilling. Denne fremstillingsvejledningindeholder anbefalinger og krav til udstyr, printning og efterbehandling for at sikre korrekt og sikker
brug af dette materiale.

*For Form Wash (2. generation) er indstillingerne for høj hastighed valideret til brug.
2. Ultrasonic Wash Unit:BEMÆRK: Anvendelse af ultralydsbade med isopropylalkohol udgør en risiko for brand eller
eksplosion. Når du bruger en ultralydsvask, skal du læse og følge alle sikkerhedsanbefalinger fra
producenten af ultralydsvaskestationen.
a. Brug ren 99 % isopropylalkohol til hver vask.
b. Anbring delene i en anden engangsbeholder af plast eller en genlukkelig plastpose,og fyld den med 99 % isopropylalkohol, så delene er helt nedsænket.
c. Anbring den anden beholder i ultralydsapparatets vandbad, og lydbehandl i 2 minutter,eller indtil den er ren.**Vaskeeffektiviteten afhænger af ultralydsapparatets størrelse og effekt. Formlabs test blev udført
med ultralydsapparat ved 36 W/L eller højere.

D. TØRRING
1. Fjern delene fra isopropylalkoholen, og lad dem lufttørre ved stuetemperatur i mindst 30 minutter.
BEMÆRK: Tørretider kan variere afhængigt af delenes design og omgivende forhold. Lad ikke
delene ligge i isopropylalkohol længere end nødvendigt.
2. Kontrollér de printede dele for at sikre, at de er rene og tørre. Der må ikke være rester af
opløsningsmiddel, overskydende flydende resin eller restpartikler tilbage på overfladen, før man
går videre til de efterfølgende trin.
3. Hvis der stadig er rester af opløsningsmiddel, skal delene tørre længere. Hvis der stadig er synlige
rester af resin, skal delene vaskes igen, til de er rene og tørre.

E. EFTERHÆRDNING
Placer de printede dele i en Formlabs-valideret efterhærdningsenhed, og lad hærde i den påkrævede tid.
1. Form Cure eller Form Cure L:a. Hærd i 60 minutter ved 60 °C
b. Lad Form Cure- eller Form Cure L-enheden køle ned til stuetemperatur mellemhærdningscyklusserne.
2. Hurtig hærdning:a. Hærdning i 6 minutter ved lysintensitet 5b. Lad Fast Cure-enheden køle af i mindst 10 minutter mellem hærdningscyklusserne.

F. FJERNELSE AF STØTTE OG POLERING
1. Støttemærker kan forårsage slid, hvis de ikke fjernes og poleres. Fjern støttepunkterne ved hjælp
af en skæreskive og et skæreværktøj en skæretang eller andet egnet efterbehandlingsværktøj.
2. Poler de printede apparater med almindelige tandpoleringsmetoder, før de tages i brug af patienten.
3. Efterse delene for revner. Kassér delene, hvis der konstateres skader eller revner.

G. RENGØRING OG DESINFEKTION
1. De færdige dele kan rengøres med en blød tandbørste med neutral sæbe og vand ved
stuetemperatur. Brug ikke tandpasta eller andre rengøringsmidler på dele, der er printet med
Dental LT Clear V2 Resin.
2. Enhederne kan renses og desinficeres i henhold til facilitetsprotokollerne. Afprøvet
desinfektionsmetode: Det færdige apparat lægges i blød i frisk 70 % IPA i 5 minutter. Lad ikke
delen ligge i alkoholopløsningen i mere end 5 minutter.
3. Efter rengøring og desinfektion inspiceres delen for skader eller revner for at sikre, at delen
opfylder kravene til ydeevne. Kassér delene, hvis der konstateres skader eller revner.

H. FARER, OPBEVARING OG BORTSKAFFELSE
1. Hærdet resin er ufarligt og kan bortskaffes som almindeligt affald.
2. Se SDS for flere oplysninger på support.formlabs.com.

Särskild information om tillverkning
Specifikationerna för Dental LT Clear V2 Resin har validerats med hjälp av den hårdvara och deparametrar som anges nedan. För att uppfylla kraven på biokompatibilitet användes vid valideringenen särskild hartstank och blandare, en byggplattform, en tvättenhet och efterbehandlingsutrustning
som inte hade varit blandade med några andra hartser.

1. Maskinvara:a. Formlabs 3D-skrivare: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Tillbehör för utskrift: Formlabs byggplattformar, Formlabs hartstankar

2. Programvara:a. Formlabs PreForm

3. Utskriftsparametrar:a. Objektets orientering: Intaglio-ytan vänds bort från byggplattformen i en 0–40° lutad vinkel
b. Skikttjocklek: 100 μm
c. Objektets tjocklek:• Ocklusala ytor: minst 2 mm
• Väggar: minst 1 mm

4. Rekommenderad utrustning och tillbehör för efterbearbetning:a. Formlabs-tillbehör för bearbetning: Form Auto, pumpningssystem för harts
b. Formlabs-validerad tvättenhet: Form Wash, Form Wash (2:a generationen), Form Wash L, ultraljudstvätt
c. Av Formlabs validerade härdningsenheter: Form Cure, Form Cure L, Fast CureA. UTSKRIFT
1. Skaka patronen: Skaka patronen före varje utskrift. Om patronen inte skakas tillräckligt kan
färgavvikelser eller utskriftsfel inträffa.
2. Ställ in: För in hartspatronen i en kompatibel Formlabs 3D-skrivare. Sätt i hartstanken och koppla
blandaren till tanken.
3. Utskrift:a. Förbered en utskrift med programvaran PreForm. Importera STL-filen för önskat objekt.
b. Orientera och skapa stöd.
c. Skicka utskriftsjobbet till skrivaren.
d. Starta utskriften genom att välja en utskrift i utskriftsmenyn. Följ eventuella meddelanden eller
dialogfönster som visas på skrivardisplayen. Skrivaren slutför utskriften automatiskt.

B. BORTTAGNING AV OBJEKT
Ta bort byggplattformen från skrivaren. För att ta bort objekt från byggplattformen, kila fast verktyget
för borttagning av objekt under det utskrivna objektet och rotera verktyget. Formlabs Build Platform 2eller Build Platform 2L kan användas för enkel, verktygsfri borttagning. För mer information om tekniker,
se support.formlabs.com.

C. TVÄTTA
Placera de utskrivna objekten i en Formlabs-validerad tvättenhet med 99 % isopropylalkohol.
1. Form Wash, Form Wash (2:a generationen) – High speed*, eller Form Wash L:
a. Tvätta i 15 minuter eller tills den är ren i Form Wash eller Form Wash L.
b. Ta ut objekten ur tvättenheten och blötlägg dem i färsk isopropylalkohol i 5 minuter.
c. Om objekten inte ser rena ut efter tvättning kan du överväga att ersätta den använda
isopropylalkoholen i tvättenheten med nytt lösningsmedel.

SVENSKA

Dental LT Clear V2 Resin är ett polymerbaserat harts som är lätt härdbart och avsett för additiv
tillverkning av biokompatibla, avtagbara tand- och tandregleringsskenor som bettskenor,
stabiliseringsskenor, tandskydd och/eller blekningsskenor för långvarig användning. Denna
tillverkningsguide innehåller rekommendationer och krav för utrustning, utskrift och efterbearbetning
för att säkerställa korrekt och säker användning av detta material.

* För Form Wash (2:a generationen) har inställningar för hög hastighet validerats för användning.
2. Ultraljudstvätt:
NOTERING: Användning av isopropylalkohol i ultraljudsbad medför risk för brand eller explosion.
När du använder en ultraljudstvätt ska du läsa och följa alla säkerhetsföreskrifter från tillverkaren
av ultraljudstvätten.
a. Använd ren 99 % isopropylalkohol för varje tvätt.
b. Placera objekten i en sekundär engångsbehållare av plast eller en återförslutningsbar
plastpåse och fyll sedan på med 99 % isopropylalkohol, och se till att objekten är helt
nedsänkta.
c. Placera den sekundära behållaren i ultraljudsenhetens vattenbad och ultraljudsbehandla i
2 minuter eller tills den är ren.**Tvätteffektiviteten beror på ultraljudsenhetens storlek och effekt. Formlabs tester utfördes med
ultraljudsenheter på 36 W/L eller högre.

D. TORKNING
1. Avlägsna objekten från isopropylalkoholen och låt dem lufttorka i rumstemperatur i minst
30 minuter. NOTERING: Torkningstiderna kan variera beroende på objektens form ochomgivningsförhållanden. Låt inte objekten ligga i isopropylalkohol längre än nödvändigt.
2. Kontrollera att de utskrivna objekten är rena och torra. Inga rester av lösningsmedel, överskott av
flytande harts eller restpartiklar får finnas kvar på ytan när du fortsätter med efterföljande steg.
3. Om rester av lösningsmedel fortfarande finns kvar, torka objekten längre. Om rester av harts
fortfarande syns ska objekten tvättas tills de är rena och torra.

E. EFTERHÄRDNING
Placera de utskrivna objekten i en Formlabs-validerad efterhärdningsenhet och härda under den tid
som krävs.
1. Form Cure eller Form Cure L:a. Härda i 60 minuter vid 60 °C
b. Låt Form Cure- eller Form Cure L-enheten svalna till rumstemperatur mellan härdningscyklerna.
2. Snabbhärdning:a. Härdning i 6 minuter vid ljusintensitet 5b. Låt Fast Cure-enheten svalna i minst 10 minuter mellan härdningscyklerna.

F. BORTTAGNING OCH POLERING AV STÖD
1. Stödmärken kan orsaka nötning om de inte avlägsnas och poleras. Ta bort stöden med hjälp av en
kapskiva och ett handstycke, en kaptång eller andra lämpliga efterbehandlingsverktyg.
2. Polera de utskrivna enheterna med vanliga dentala poleringsmetoder innan de används av patienten.
3. Kontrollera om det finns sprickor i objekten. Kassera om skada eller sprickor upptäcks.

G. RENGÖRING OCH DESINFEKTION
1. Helt efterbearbetade objekt kan rengöras med en särskild mjuk tandborste med neutralt
rengöringsmedel och rumstempererat vatten. Använd inte tandkräm eller andra rengöringsmedel
på objekt som skrivits ut med Dental LT Clear V2 Resin.
2. Skenorna kan rengöras och desinficeras enligt verksamhetens regler. Testad desinfektionsmetod:
den färdiga skenan läggs i 70 % IPA under 5 minuter. Låt inte objekten ligga i alkohollösningen imer än 5 minuter.
3. Efter rengöring och desinfektion, inspektera objektet för skada eller sprickor för att säkerställa
att integriteten hos den slutliga produkten uppfyller prestandakraven. Kassera om skada eller
sprickor upptäcks.

H. FAROR, FÖRVARING OCH KASSERING
1. Härdad harts är ofarligt och kan kasseras som vanligt avfall.
2. Se SDS för mer information på support.formlabs.com.

Erityisiä valmistukseen liittyviä huomioita
Dental LT Clear Resin V2 -hartsin tekniset tiedot on validoitu alla mainittujen laitteistojen ja
parametrien avulla. Bioyhteensopivuuden varmistamiseksi validointi tehtiin erillisellä hartsisäiliöllä
ja sekoittimilla, rakennusalustalla, pesuyksiköllä ja jälkikäsittelylaitteistolla, joita ei käytetty muiden
hartsien kanssa.

1. Laitteisto:
a. Formlabs-3D-tulostin: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Tulostustarvikkeet: Formlabs-rakennusalustat, Formlabs-hartsisäiliöt

2. Ohjelmisto:
a. Formlabs PreForm

3. Tulostusparametrit:a. Osan suuntaus: Kaiverrettava pinta poispäin rakennusalustasta 0–40 °:een kallistuskulmassab. Kerrospaksuus: 100 μm
c. Kappaleen paksuus:• Purupinnat: vähintään 2 mm
• Seinämät: vähintään 1 mm

4. Suositeltu jälkikäsittelylaitteisto ja lisävarusteet:a. Formlabsin käsittelytarvikkeet: Form Auto, Resin Pumping Systemb. Formlabsin validoitu pesuyksikkö: Form Wash, Form Wash L (2. sukupolvi), Form Wash L,
ultraäänipesuyksikkö
c. Formlabsin validoitu kovetusyksikkö: Form Cure, Form Cure L, Fast CureA. TULOSTAMINEN
1. Ravista hartsipatruuna: Ravista patruuna ennen jokaista tulostustyötä. Jos patruuna ei ravisteta
riittävästi, seurauksena voi olla väripoikkeamia ja tulostusvirheitä.
2. Kokoonpano: Aseta hartsipatruuna yhteensopivaan Formlabs 3D-tulostimeen. Aseta hartsisäiliö
paikalleen ja kiinnitä sekoitin säiliöön.
3. Tulostaminen:
a. Valmistele tulostustyö PreForm-ohjelmalla. Tuo halutun kappaleen STL-tiedosto.
b. Suuntaa ja luo tuet.
c. Lähetä tulostustyö tulostimeen.
d. Aloita tulostus valitsemalla tulostustyö tulostusvalikosta. Noudata tulostimen näytössä näytettyjen
kehotteiden tai valintaikkunoiden ohjeita. Tulostin suorittaa tulostuksen automaattisesti.

B. KAPPALEEN IRROTTAMINEN
Poista rakennusalusta tulostimesta. Kun haluat poistaa osia rakennusalustalta, vie kappaleen irrotustyökalu
tulosteen alustan alle ja kierrä työkalua. Formlabs Build Platform 2- tai Build Platform 2L -alustan
avulla se voidaan poistaa helposti ja ilman työkaluja. Katso yksityiskohtainen menetelmä osoitteessa
support.formlabs.com.

C. PESU
Aseta tulostetut kappaleet Formlabsin validoimaan pesuyksikköön, jossa on 99 % isopropyylialkoholia.
1. Form Wash, Form Wash (2. sukupolvi) – korkea nopeus* tai Form Wash L:
a. Pese 15 minuuttia tai kunnes kappale on puhdas Form Wash- tai Form Wash L -pesurissa.
b. Poista tulosteet pesuyksiköstä ja liota tuoreessa isopropyylialkoholissa 5 minuutin ajan.
c. Jos osat eivät näytä puhtailta pesun jälkeen, vaihda pesuyksikössä käytetty isopropyylialkoholi
uuteen liuottimeen.

SUOMI

Dental LT Clear Resin V2 -hartsi on valokovettuva polymeeripohjainen hartsi, joka on suunniteltu
bioyhteensopivien, pitkäaikaiseen käyttöön soveltuvien, irrotettavien hammashoidollisten laitteiden
ja oikomiskojeiden, kuten purentakiskojen, hammassuojien ja/tai valkaisualustojen, pikavalmistamista
varten. Tässä valmistusoppaassa annetaan laitteisto-, tulostus- ja jälkikäsittelysuosituksia ja -vaatimuksia
tämän materiaalin oikean ja turvallisen käytön varmistamiseksi.

* Form Wash (2. sukupolvi), korkean nopeudun asetukset on validoitu käyttöä varten.
2. Ultraäänipesuyksikkö:
HUOMAUTUS: Isopropyylialkoholin käyttö ultraäänikylvyssä aiheuttaa tulipalo- tai räjähdysvaaran. Kun
käytät ultraäänipesua, lue ja noudata kaikkia ultraäänipesun valmistajan antamia turvallisuussuosituksia.
a. Käytä puhdasta 99 %:n isopropyylialkoholia jokaisessa pesussa.
b. Aseta kappaleet toissijaiseen kertakäyttöiseen muovisäiliöön tai uudelleensuljettavaan
muovipussiin ja täytä se 99 %:n isopropyylialkoholilla varmistaen, että kappaleet ovat täysin
veden alla.
c. Aseta toissijainen säiliö ultraäänilaitteen vesihauteeseen ja sonikoi 2 minuutin ajan tai kunnes
kappale on puhdas.**Pesuteho riippuu ultraäänilaitteen koosta ja tehosta. Formlabsin testit suoritettiin ultraäänilaitteilla,
joiden teho oli vähintään 36 W/L.

D. KUIVAUS
1. Poista kappaleet isopropyylialkoholista ja anna kuivua huonelämpötilassa vähintään 30 minuutin
ajan. HUOMAA: Kuivumisaika voi vaihdella tulostetun kappaleen muotoilun ja ympäristön
olosuhteiden mukaan. Älä anna kappaleiden olla isopropyylialkoholissa kauemmin kuin on tarpeen.
2. Tarkista tulostetut osat varmistaaksesi, että ne ovat puhtaat ja kuivat. Pinnalla ei saa olla liuottimen
jäämiä, ylimääräistä nestemäistä hartsia tai jäännöshiukkasia ennen seuraaviin vaiheisiin siirtymistä.
3. Jos liuottimen jäämiä on yhä jäljellä, anna tulosteen kuivua pidempään. Jos ylimääräistä hartsia on
jäljellä, pese osat uudelleen kunnes ne ovat puhtaat ja anna niiden kuivua.

E. JÄLKIKOVETUS
Aseta tulostetut kappaleet Formlabsin validoimaan jälkikovetusyksikköön ja koveta vaaditun ajan.
1. Form Cure tai Form Cure L:
a. Koveta 60 minuuttia 60 °C:n lämpötilassab. Anna Form Cure- tai Form Cure L -yksikön jäähtyä huoneenlämpötilaan kovettumisjaksojen välillä.
2. Fast Cure:a. Koveta 6 minuuttia valon intensiteetillä 5b. Anna Fast Cure -yksikön jäähtyä vähintään 10 minuuttia kovettumisjaksojen välillä.

F. TUEN POISTO JA KIILLOTUS
1. Tukien jäljet voivat aiheuttaa kulumista, jos niitä ei poisteta ja kiilloteta. Irrota tuet käyttämällä
leikkauslaikkaa ja käsikappaletta, leikkauspihtejä tai muita sopivia viimeistelytyökaluja.
2. Kiillota tulostetut laitteet tavanomaisilla hammaslääketieteellisillä kiillotusmenetelmillä
ennen potilaskäyttöä.
3. Tarkista kappaleet murtumien varalta. Hävitä kappale, jos siinä on vaurioita tai murtumia.

G. PUHDISTUS JA DESINFIOINTI
1. Kokonaan jälkikäsitellyt tulosteet voidaan puhdistaa erityisellä pehmeällä hammasharjalla ja
neutraalilla saippualla ja huoneenlämpöisellä vedellä. Älä käsittele Dental LT Clear Resin V2-hartsilla tulostettuja kappaleita hammastahnalla tai muilla puhdistustuotteilla.
2. Laitteet voidaan puhdistaa ja desinfioida laitoksen toimintaohjeiden mukaisesti.
Testattu desinfiointimenelmä: valmiin laitteen liottaminen puhtaassa 70-prosenttisessa
isopropyylialkoholissa 5 minuutin ajan. Älä jätä tulostetta alkoholiliuokseen viittä minuuttia
pidemmäksi ajaksi.
3. Tarkista kappale vaurioiden tai murtumien varalta puhdistuksen ja desinfioinnin jälkeen
varmistaaksesi, että suunnitellun kappaleen eheys täyttää suorituskykyvaatimukset. Hävitä
kappale, jos siinä on vaurioita tai murtumia.

H. VAARAT, SÄILYTYS JA HÄVITTÄMINEN
1. Kovettunut hartsi ei ole vaarallista, ja se voidaan hävittää normaalina jätteenä.
2. Katso lisätietoja turvallisuustiedotteesta osoitteessa support.formlabs.com.

Konkrétní výrobní aspekty
Specifikace Dental LT Clear V2 Resin byly ověřeny pomocí níže uvedeného hardwaru a parametrů.
Z důvodu splnění požadavků na biokompatibilitu byla pryskyřice validována s vyhrazenou nádrží na
pryskyřici a směšovačem, tiskovou platformou, čistící stanicí a zařízením pro následné zpracování,které nebyly smíchány s žádnou jinou pryskyřicí.

1. Hardware:a. 3D tiskárna Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Příslušenství pro tisk: tiskové platformy Formlabs, nádrže na pryskyřici Formlabs

2. Software:a. Formlabs PreForm

3. Parametry tisku:
a. Orientace dílu: Hlubotiskový povrch směřuje na stranu odvrácenou od tiskové platformy podúhlem naklonění 0–40°
b. Tloušťka vrstvy: 100 μm
c. Tloušťka dílu:• Okluzní plochy: minimálně 2 mm
• Stěny: minimálně 1 mm

4. Doporučené vybavení a příslušenství následného zpracování:a. Příslušenství pro zpracování Formlabs: Form Auto, systém pro čerpání pryskyřice
b. Ověřená čisticí stanice Formlabs: Form Wash, Form Wash (2. generace), Form Wash L,
Ultrazvuková mycí jednotka
c. Ověřené vytvrzovací jednotky Formlabs: Form Cure, Form Cure L, Fast CureA. TISK
1. Protřepejte kazetu: Před každou tiskovou úlohou kazetu protřepejte. V případě nedostatečného
protřepání kazety může dojít k barevným odchylkám a chybám v tisku.
2. Nastavení: Vložte nádrž na pryskyřici a připojte k ní směšovač.
3. Tisk:a. Připravte tiskovou úlohu pomocí programu PreForm. Importujte požadovaný soubor STL části.
b. Nastavte orientaci podpor a vytvořte je.
c. Odešlete tiskovou úlohu do tiskárny.
d. Vyberte tiskovou úlohu z nabídky tisku a zahajte tisk. Postupujte podle pokynů nebo
dialogových oken zobrazených na obrazovce tiskárny. Tiskárna tisk dokončí automaticky.

B. ODSTRAŇOVÁNÍ ČÁSTÍ
Vyjměte tiskovou platformu z tiskárny. Části z tiskové platformy odstraníte tak, že zaklíníte nástroj pro
odstraňování částí pod základovou desku vytištěné části a otočíte nástrojem. Formlabs Build Platform 2
nebo Build Platform 2L lze použít pro snadné odstranění bez použití nářadí. Podrobné techniky jsou
uvedeny na webových stránkách support.formlabs.com.

C. MYTÍ
Vložte vytištěné díly do ověřené mycí jednotky Formlabs s 99% isopropylalkoholem.
1. Form Wash, Form Wash (2. generace) – vysokorychlostní* nebo Form Wash L:
a. Myjte 15 minut nebo do vyčištění ve Form Wash nebo Form Wash L.
b. Vyjměte části z čisticí jednotky a ponořte je do čerstvého isopropylalkoholu na dobu 5 minut.
c. Pokud se části po umytí nezdají být zcela čisté, zvažte výměnu použitého isopropylalkoholu v
mycí jednotce za čerstvé rozpouštědlo.

ČEŠTINA

Dental LT Clear V2 Resin je pryskyřice založená na světlem vytvrditelném polymeru určená provýrobu biokompatibilních snímatelných zubolékařských a ortodontických pomůcek pro dlouhodobě
používání, jako jsou okluzní dlahy, noční rovnátka, chrániče úst a/nebo bělicí pásky pomocí aditivnívýroby. Doporučení a požadavky pro vybavení, tisk a další zpracování pro zajištění správného abezpečného použití tohoto materiálu, naleznete v tomto průvodci výrobou.

*Pro Form Wash (2. generace) bylo ověřeno použití nastavení vysoké rychlosti.
2. Ultrazvuková mycí jednotka:POZNÁMKA: Použití isopropylalkoholu v ultrazvukové lázni představuje riziko požáru nebo výbuchu.
Při použití ultrazvukové mycí jednotky si přečtěte všechna bezpečnostní doporučení jejího výrobce adodržujte je.
a. Při každém mytí použijte čistý 99% isopropylalkohol.
b. Vložte části do sekundární jednorázové plastové nádoby nebo plastového uzavíratelného
sáčku a poté je naplňte 99% izopropylalkoholem, aby byly části zcela ponořené.
c. Umístěte sekundární nádobu do vodní lázně ultrazvukové jednotky a sonikujte po dobu
2 minut nebo dokud není čistá.**Účinnost mytí závisí na velikosti a výkonu ultrazvukové jednotky. Testy společnosti Formlabs byly
prováděny s ultrazvukovými jednotkami o výkonu 36 W/L nebo vyšším.

D. SUŠENÍ
1. Vyjměte části z isopropylalkoholu a nechte je nejméně 30 minut vyschnout při pokojové teplotě.
UPOZORNĚNÍ: Doba sušení se může lišit podle tvaru součásti a okolních podmínek. Nenechávejtečásti v isopropylalkoholu déle, než je nutné.
2. Zkontrolujte vytištěné části a ujistěte se, že jsou čisté a suché. Před provedením následujících
kroků by na povrchu nemělo zůstat žádné zbytkové rozpouštědlo, přebytečná kapalná pryskyřice
nebo zbytkové částice.
3. Pokud jsou přítomny zbytky rozpouštědla, prodlužte dobu sušení. Pokud jsou viditelné zbytky
pryskyřice, znovu součásti omývejte, až budou čisté a suché.

E. NÁSLEDNÉ VYTVRZENÍ
Vložte vytištěné části do jednotky pro následné vytvrzování ověřené společností Formlabs a nechte je
vytvrzovat po požadovanou dobu.
1. Form Cure nebo Form Cure L:a. Vytvrzování po dobu 60 minut při 60 °C
b. Mezi jednotlivými cykly vytvrzování nechte zařízení Form Cure nebo Form Cure L vychladnout
na pokojovou teplotu.
2. Rychlé vytvrzování:
a. Vytvrzování po dobu 6 minut při intenzitě světla 5b. Mezi jednotlivými cykly vytvrzování nechte zařízení Fast Cure alespoň 10 minut vychladnout.

F. ODSTRANĚNÍ PODPĚR A LEŠTĚNÍ
1. Neodstraněné a nevyleštěné známky podpěr mohou způsobit oděr. Podpěry odstraňte pomocířezného kotouče a ručního nástavce, řezacích kleští nebo jiných vhodných dokončovacích nástrojů.
2. Vyleštěte vytištěné pomůcky pomocí běžných způsobů leštění používaných v zubním lékařství
před tím, než je použije pacient.
3. Zkontrolujte části a zjistěte, zda se na nich neobjevily praskliny. Pokud u části zjistíte poškozenínebo praskliny, zlikvidujte ji.

G. ČIŠTĚNÍ A DEZINFEKCE
1. Části, které prošly celkovým následným zpracováním, lze vyčistit pomocí měkkého zubního kartáčku
určeného pro tento účel a neparfemovaného mýdla s vodou o pokojové teplotě. Na části vytištěné
pomocí pryskyřice Dental LT Clear V2 Resin nepoužívejte zubní pastu ani jiné čisticí prostředky.
2. Pomůcky lze čistit a dezinfikovat podle protokolů provozovny. Testovaný způsob dezinfekce:ponoření vytištěné pomůcky do čerstvého 70% roztoku isopropylalkoholu po dobu 5 minut.
Nenechávejte část v alkoholovém roztoku po dobu delší než 5 minut.
3. Po vyčištění a dezinfekci zkontrolujte, zda na části nejsou trhliny, abyste se ujistili, že celistvostnavržené části splňuje požadavky na výkon. Pokud u části zjistíte poškození nebo praskliny,
zlikvidujte ji.

H. NEBEZPEČÍ, SKLADOVÁNÍ A LIKVIDACE
1. Vytvrzená pryskyřice není nebezpečná a lze ji likvidovat jako běžný odpad.
2. Další informace naleznete v bezpečnostním listu na adrese support.formlabs.com.

Az anyagra vonatkozó gyártói megjegyzések
A Dental LT Clear V2 Resin műgyanta specifikációit az alábbiakban megadott hardver és paraméterek
alapján hitelesítették. A biokompatibilitási megfelelőség érdekében a hitelesítés külön gyantatartállyal
és keverővel, nyomtatási platformmal, mosóegységgel és utókezelő berendezéssel történt, amelyeket
nem használtak más műgyantákkal.

1. Hardver:a. Formlabs 3D nyomtató: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Nyomtatási kiegészítők: Formlabs Build Platform nyomtatási platformok, Formlabs gyantatartályok

2. Szoftver:
a. Formlabs PreForm

3. Nyomtatási paraméterek:a. Munkadarab tájolása: a benyomati felület a nyomtatási platformtól elfelé néz 0—40°-os dőlésszögben
b. Rétegvastagság: 100 μm
c. Munkadarab vastagsága:• Okkluzális felületek: legalább 2 mm
• Falak: legalább 1 mm

4. Ajánlott utókezelő berendezések és tartozékok:a. Formlabs feldolgozási tartozékok: Form Auto, Resin Pumping Systemb. Formlabs által hitelesített mosóegységek: Form Wash, Form Wash (2. generáció), Form Wash L,
Ultrahangos mosóegységc. Formlabs által hitelesített polimerizációs egységek: Form Cure, Form Cure L, Fast CureA. NYOMTATÁS
1. Rázza fel a patront: Minden nyomtatási feladat előtt rázza fel a patront. A patron elégtelenfelrázása színeltéréseket és nyomtatási hibákat okozhat.
2. Üzembe helyezés: Helyezze a gyantapatront egy kompatibilis Formlabs 3D nyomtatóba. Helyezze
be a gyantatartályt, és csatlakoztassa a keverőt a tartályhoz.
3. Nyomtatás:a. Készítse elő a nyomtatást a PreForm szoftver segítségével. Importálja a nyomtatandó
munkadarab STL fájlját.
b. Állítsa be a munkadarab tájolását, és alakítson ki támasztékokat.
c. Küldje el a nyomtatási feladatot a nyomtatóra.
d. Nyomtatáshoz nyissa meg a nyomtatási menüt, és válassza ki a megfelelő nyomtatási feladatot.
Kövesse a nyomtató képernyőjén megjelenő utasításokat vagy párbeszédablakokat. A nyomtató
automatikusan elvégzi a nyomtatást.

B. A MUNKADARAB ELTÁVOLÍTÁSA
Távolítsa el a nyomtató nyomtatási platformját. A munkadarabok nyomtatási platformról való
eltávolításához rögzítse a munkadarabeltávolító-eszközt a munkadarab alapja alá, és fordítsa el az eszközt.
A munkadarab egyszerű, szerszám nélküli eltávolításához használja a Formlabs Build Platform 2 vagy Build
Platform 2L nyomtatási platformokat. Az eljárás részletes leírásáért lásd a support.formlabs.com oldalt.

C. MOSÁSHelyezze a nyomtatott munkadarabokat egy Formlabs által hitelesített, 99%-os izopropil-alkoholt
tartalmazó mosóegységbe.

MAGYARA Dental LT Clear V2 egy fényre keményedő polimer alapú műgyanta, amelyet biokompatibilis, hosszú
távú használatra alkalmas, kivehető fogászati és fogszabályozó eszközök, például harapásemelő
sínek, fogcsikorgás gátlók, fogvédők és/vagy fogfehérítő sínek additív gyártására terveztek. Ez agyártási útmutató bemutatja a berendezésekre, nyomtatásra és utókezelésre vonatkozó ajánlásokatés követelményeket, hogy biztosítsa az anyag helyes és biztonságos használatát.

1. Form Wash, Form Wash (2. generáció) — nagy sebességen*, vagy Form Wash L:
a. Mossa a munkadarabokat a Form Wash vagy Form Wash L egységben 15 percig vagy addig,amíg tiszták nem lesznek.
b. Távolítsa el a munkadarabokat a mosóegységből, és áztassa őket friss izopropil-alkoholba
5 percre.
c. Ha a mosás után nem tűnnek tisztának a darabok, fontolja meg a mosóegységben található
használt izopropil-alkoholt friss oldószerre való cseréjét.
*A Form Wash (2. generáció) esetében a nagy sebességű beállítások használatát hitelesítették.
2. Ultrahangos mosóegység:
MEGJEGYZÉS: Az izopropil-alkohol ultrahangos fürdőben való használata tűz- és robbanásveszélyes.
Ultrahangos mosóegység használata esetén olvassa el és kövesse az ultrahangos mosóegység
gyártójának összes biztonsági ajánlását.
a. Minden mosáshoz használjon tiszta 99%-os izopropil-alkoholt.
b. Helyezze a munkadarabokat egy másodlagos, eldobható műanyag tartályba vagy visszazárhatóműanyag zacskóba. Töltse fel 99%-os izopropil-alkohollal úgy, hogy a munkadarabok teljesenelmerüljenek.
c. Helyezze a másodlagos tartályt az ultrahangos készülék vízfürdőjébe, és szonikálja 2 percig
vagy addig, amíg tiszta nem lesz.**A mosás hatékonysága az ultrahangos egység méretétől és teljesítményétől függ. A Formlabs
a tesztelést 36 W/L vagy annál nagyobb teljesítményű ultrahangos egységekkel végezte.

D. SZÁRÍTÁS
1. Vegye ki a munkadarabokat az izopropil-alkoholból, és hagyja szobahőmérsékletű levegőn
legalább 30 percig száradni. MEGJEGYZÉS: A száradási idő a munkadarabok kialakításától és akörnyezeti feltételektől függően változhat. Ne hagyja a munkadarabokat a szükségesnél hosszabb
ideig izopropil-alkoholban állni.
2. Ellenőrizze a nyomtatott munkadarabokat, hogy biztosan tiszták és szárazak legyenek. A következő
lépések megkezdése előtt minden oldószermaradványt, folyékony műgyantát és műgyantamaradványt
el kell távolítani a munkadarab felületéről.
3. Oldószermaradvány esetén szárítsa tovább a munkadarabokat. Ha továbbra is láthatókműgyantamaradványok, mossa át újra a munkadarabokat, amíg tiszták és szárazak nem lesznek.

E. UTÓPOLIMERIZÁCIÓHelyezze a nyomtatott munkadarabokat egy Formlabs által hitelesített utópolimerizációs egységbe,és polimerizálja azokat a kívánt ideig.
1. Form Cure vagy Form Cure L:
a. Végezzen polimerizációt 60 percig 60 °C-on
b. A polimerizációs ciklusok között hagyja szobahőmérsékletűre hűlni a Form Cure vagy
Form Cure L egységet.
2. Fast Cure:a. Végezzen polimerizációt 6 percig 5-ös fényintenzitáson
b. A polimerizációs ciklusok között hagyja legalább 10 percig hűlni a Fast Cure egységet.

F. TÁMASZTÉKOK ELTÁVOLÍTÁSA ÉS POLÍROZÁS
1. Ha nem távolítja el és polírozza a támasztékok nyomait, azok kopást okozhatnak. Távolítsa
el a támasztékokat vágókorong, mikromotor, vágófogó vagy más megfelelő utókezelő
szerszám segítségével.
2. A nyomtatott eszközöket a páciensek általi használat előtt a szokásos fogászati polírozási
módszerekkel polírozza.
3. Vizsgálja meg, hogy a munkadarabokon nincsenek-e repedések. Ha bármilyen sérülést vagy
repedést észlel, ne használja az eszközt.

G. TISZTÍTÁS ÉS FERTŐTLENÍTÉS
1. Az teljes utókezelésen átesett munkadarabokat speciális puha fogkefével, semleges szappannalés szobahőmérsékletű vízzel lehet tisztítani. Ne használjon fogkrémet vagy más tisztítószert a
Dental LT Clear V2 Resin használatával nyomtatott munkadarabokon.
2. A nyomtatott eszközök a létesítmény protokollja szerint tisztíthatók és fertőtleníthetők. Vizsgáltfertőtlenítési módszer: a kész eszközök friss 70%-os izopropil-alkoholba áztatása 5 percig.
Ne hagyja a munkadarabot 5 percnél tovább az alkoholos oldatban.
3. Tisztítás és fertőtlenítés után ellenőrizze, hogy nincsenek-e sérülések vagy repedések amunkadarabon, és bizonyosodjon meg róla, hogy a munkadarab sértetlensége megfelel ateljesítménykövetelményeknek. Ha bármilyen sérülést vagy repedést észlel, ne használja
a munkadarabot.

H. VESZÉLYEK, TÁROLÁS ÉS ÁRTALMATLANÍTÁS
1. A polimerizált műgyanta nem veszélyes, és általános hulladékként kezelendő.
2. További információkért lásd a biztonsági adatlapot a support.formlabs.com oldalon.

Ειδικά κατασκευαστικά ζητήματα
Οι προδιαγραφές της Dental LT Clear V2 Resin έχουν επικυρωθεί χρησιμοποιώντας το υλικό καιτις παραμέτρους που αναφέρονται παρακάτω. Για τη συμμόρφωση με τη βιοσυμβατότητα, κατάτην επικύρωση χρησιμοποιήθηκε ειδική δεξαμενή ρητίνης και διάταξη ανάμειξης, πλατφόρμα
κατασκευής, μονάδα πλύσης και εξοπλισμός μετεπεξεργασίας που δεν ήρθαν σε επαφή μεάλλες ρητίνες.

1. Υλισμικό:a. Εκτυπωτής 3D της Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Αξεσουάρ εκτύπωσης: Formlabs, Δεξαμενές ρητίνης Formlabs

2. Λογισμικό:a. Formlabs PreForm

3. Παράμετροι εκτύπωσης:a. Προσανατολισμός τεμαχίου: Επιφάνεια βαθυτυπίας στραμμένη μακριά από την πλατφόρμα
κατασκευής με γωνία κλίσης 0 - 40°b. Πάχος στρώματος: 100 μm
c. Πάχος τεμαχίου:• Αποφρακτικές επιφάνειες: τουλάχιστον 2 mm
• Τοιχώματα: 1 mm τουλάχιστον

4. Συνιστώμενος εξοπλισμός και αξεσουάρ μετεπεξεργασίας:a. Αξεσουάρ επεξεργασίας Formlabs: Form Auto, Σύστημα άντλησης ρητίνης
b. Επικυρωμένη μονάδα πλύσης της Formlabs: Form Wash, Form Wash (2ης γενιάς), Form Wash L,Μονάδα πλύσης με υπέρηχους
c. Πιστοποιημένη από τη Formlabs μονάδα σκλήρυνσης: Form Cure, Form Cure L, Fast CureA. ΕΚΤΥΠΩΣΗ
1. Ανακινήστε το φυσίγγιο: Ανακινείτε το φυσίγγιο πριν από κάθε εργασία εκτύπωσης.
Ενδέχεται να προκύψουν χρωματικές αποκλίσεις και αστοχίες εκτύπωσης, αν το φυσίγγιο
δεν ανακινηθεί επαρκώς.
2. Τοποθέτηση: Τοποθετήστε την κασέτα ρητίνης σε έναν συμβατό τρισδιάστατο εκτυπωτή της
Formlabs. Τοποθετήστε τη δεξαμενή ρητίνης και συνδέστε τη διάταξη ανάμειξης στη δεξαμενή.
3. Εκτύπωση:a. Προετοιμάστε μια εργασία εκτύπωσης, χρησιμοποιώντας το λογισμικό PreForm. Εισαγάγετε
το αρχείο STL του επιθυμητού μέρους.
b. Προσαρμόστε τον προσανατολισμό και δημιουργήστε στηρίγματα.
c. Στείλτε την εργασία εκτύπωσης στον εκτυπωτή.
d. Ξεκινήστε την εκτύπωση, επιλέγοντας μια εργασία εκτύπωσης από το μενού εκτύπωσης.
Ακολουθήστε τις οδηγίες ή τα παράθυρα διαλόγου που εμφανίζονται στην οθόνη τουεκτυπωτή. Ο εκτυπωτής θα ολοκληρώσει αυτόματα την εκτύπωση.

B. ΑΦΑΙΡΕΣΗ ΜΕΡΟΥΣ
Αφαιρέστε την πλατφόρμα κατασκευής από τον εκτυπωτή. Για να αφαιρέσετε τεμάχια από τηνπλατφόρμα κατασκευής, σφηνώστε το εργαλείο αφαίρεσης τεμαχίων κάτω από τη βάση εκτυπωμένων
τεμαχίων και περιστρέψτε το εργαλείο. Η Formlabs Build Platform 2 ή η Build Platform 2L μπορεί
να χρησιμοποιηθεί για εύκολη αφαίρεση χωρίς εργαλεία. Για αναλυτικές οδηγίες τεχνικής φύσης,επισκεφθείτε τη διεύθυνση support.formlabs.com.

ΕΛΛΗΝΙΚΆΗ ρητίνη Dental LT Clear V2 είναι μια φωτοσκληρυνόμενη ρητίνη με βάση πολυμερή υλικά πουέχει σχεδιαστεί για την κατασκευή βιοσυμβατών, μακράς χρήσης, αφαιρούμενων οδοντιατρικών
και ορθοδοντικών συσκευών, όπως νάρθηκες σύγκλεισης, μασελάκια βρουξισμού, προστατευτικά
στόματος ή/και δίσκους λεύκανσης, μέσω προσθετικής κατασκευής. Αυτός ο οδηγός κατασκευής
παρέχει τις συστάσεις και απαιτήσεις για τον εξοπλισμό, την εκτύπωση και τη μετεπεξεργασία,ώστε να διασφαλιστεί η σωστή και ασφαλής χρήση αυτού του υλικού.

C. ΠΛΥΣΗΤοποθετήστε τα εκτυπωμένα τεμάχια σε μια πιστοποιημένη από τη Formlabs μονάδα πλύσης με
ισοπροπυλική αλκοόλη 99%.
1. Form Wash, Form Wash (2ης γενιάς) - High speed* ή Form Wash L:a. Πλύνετε για 15 λεπτά, ή μέχρι να καθαριστεί πλήρως, με το Form Wash ή το Form Wash L.
b. Αφαιρέστε τα τεμάχια από τη μονάδα πλύσης και εμποτίστε τα με φρέσκια ισοπροπυλική
αλκοόλη για 5 λεπτά.
c. Εάν τα εξαρτήματα δεν φαίνονται καθαρά μετά το πλύσιμο, εξετάστε το ενδεχόμενο νααντικαταστήσετε τη χρησιμοποιημένη ισοπροπυλική αλκοόλη στη μονάδα πλύσης μεφρέσκο διαλύτη.
*Για το Form Wash (2ης γενιάς), οι ρυθμίσεις υψηλής ταχύτητας έχουν επικυρωθεί για χρήση.
2. Μονάδα πλύσης με υπερήχους:ΣΗΜΕΙΩΣΗ: Η χρήση ισοπροπυλικής αλκοόλης σε λουτρό υπερήχων ενέχει κίνδυνο πυρκαγιάςή έκρηξης. Κατά τη χρήση πλύσης με υπερήχους, διαβάστε και ακολουθήστε όλες τις συστάσεις
ασφαλείας του κατασκευαστή της μονάδας πλύσης με υπερήχους.
a. Χρησιμοποιείτε καθαρή ισοπροπυλική αλκοόλη 99% σε κάθε πλύση.
b. Τοποθετήστε τα τεμάχια σε ένα δευτερεύον πλαστικό δοχείο μίας χρήσης ή μια πλαστική
επανασφραγιζόμενη σακούλα και, στη συνέχεια, γεμίστε με ισοπροπυλική αλκοόλη 99%φροντίζοντας τα τεμάχια να είναι πλήρως βυθισμένα.
c. Τοποθετήστε το δευτερεύον δοχείο στο λουτρό νερού της μονάδας υπερήχων και κάντε
κατεργασία με υπερήχους για 2 λεπτά ή μέχρι να καθαρίσει.**Η αποτελεσματικότητα της πλύσης εξαρτάται από το μέγεθος και την ισχύ της μονάδας υπερήχων.
Οι δοκιμές της Formlabs διεξήχθησαν με μονάδες υπερήχων των 36 W/L ή περισσότερο.

D. ΣΤΕΓΝΩΜΑ
1. Αφαιρέστε τα τεμάχια από την ισοπροπυλική αλκοόλη και αφήστε τα να στεγνώσουν στοναέρα σε θερμοκρασία δωματίου για τουλάχιστον 30 λεπτά. ΣΗΜΕΙΩΣΗ: Το χρονικό διάστημα
στεγνώματος μπορεί να ποικίλλει ανάλογα με τον σχεδιασμό των τεμαχίων και τις συνθήκες
περιβάλλοντος. Μην αφήνετε τα τεμάχια να παραμείνουν μέσα στην ισοπροπυλική αλκοόλη γιαπερισσότερο χρόνο από όσο χρειάζεται.
2. Ελέγξτε τα εκτυπωμένα τεμάχια για να διασφαλίσετε ότι είναι καθαρά και στεγνά. Δεν πρέπει
να παραμένουν υπολείμματα διαλύτη, περίσσεια υγρής ρητίνης ή σωματίδια υπολειμμάτων στηνεπιφάνεια πριν προχωρήσετε στα επόμενα βήματα.
3. Εάν υπάρχουν ακόμα υπολείμματα διαλύτη, στεγνώστε τα τεμάχια για περισσότερο χρόνο.
Εάν εξακολουθούν να είναι ορατά υπολείμματα ρητίνης, πλύνετε ξανά τα τεμάχια έως ότουκαθαρίσουν και στεγνώστε τα.

E. ΜΕΤΑΣΚΛΗΡΥΝΣΗΤοποθετήστε τα εκτυπωμένα μέρη σε μια πιστοποιημένη από τη Formlabs μονάδα μετα-σκλήρυνσης
και σκληρύνετε για τον απαιτούμενο χρόνο.
1. Form Cure ή Form Cure L:a. Σκλήρυνση για 60 λεπτά στους 60 °C
b. Αφήστε τη μονάδα Form Cure ή Form Cure L να κρυώσει σε θερμοκρασία δωματίου μεταξύ
των κύκλων σκλήρυνσης.
2. Fast Cure:a. Σκλήρυνση για 6 λεπτά σε ένταση φωτός 5b. Αφήστε τη μονάδα ταχείας σκλήρυνσης να κρυώσει για τουλάχιστον 10 λεπτά μεταξύ τωνκύκλων σκλήρυνσης.

F. ΑΦΑΙΡΕΣΗ ΣΤΗΡΙΓΜΑΤΩΝ ΚΑΙ ΣΤΙΛΒΩΣΗ
1. Τα σημεία στηριγμάτων μπορεί να προκαλέσουν τριβή εάν δεν αφαιρεθούν και δεν γυαλιστούν.
Αφαιρέστε τα στηρίγματα χρησιμοποιώντας δίσκο κοπής και τεμάχιο χειρός, πένσα κοπής ήάλλα κατάλληλα εργαλεία φινιρίσματος.

2. Γυαλίστε τις εκτυπωμένες συσκευές με τις συνήθεις οδοντιατρικές μεθόδους στίλβωσης πριναπό τη χρήση σε ασθενή.
3. Ελέγξτε τα τεμάχια για τυχόν ρωγμές. Απορρίψτε τα εάν εντοπίσετε οποιαδήποτε ένδειξηζημιάς ή τυχόν ρωγμές.

G. ΚΑΘΑΡΙΣΜΟΣ ΚΑΙ ΑΠΟΛΥΜΑΝΣΗ
1. Μπορείτε να καθαρίσετε τα πλήρως μετεπεξεργασμένα μέρη, χρησιμοποιώντας μια ειδική
μαλακή οδοντόβουρτσα με ουδέτερο σαπούνι και νερό σε θερμοκρασία δωματίου. Μηχρησιμοποιείτε οδοντόκρεμα ή άλλα προϊόντα καθαρισμού σε τεμάχια που έχουν εκτυπωθεί μερητίνη Dental LT Clear V2.
2. Οι συσκευές μπορούν να καθαριστούν και να απολυμανθούν σύμφωνα με τα πρωτόκολλα τηςεκάστοτε εγκατάστασης. Δοκιμασμένη μέθοδος απολύμανσης: εμποτισμός της τελικής συσκευής
σε καθαρή IPA 70% για 5 λεπτά. Μην αφήνετε το τεμάχιο μέσα στο αλκοολούχο διάλυμα γιαπερισσότερα από 5 λεπτά.
3. Μετά τον καθαρισμό και την απολύμανση επιθεωρήστε το τεμάχιο για ζημιές ή ρωγμές, ώστε ναδιασφαλίσετε ότι η ακεραιότητα του σχεδιασμένου τεμαχίου πληροί τις απαιτήσεις απόδοσης.
Απορρίψτε το εάν εντοπίσετε οποιαδήποτε ένδειξη ζημιάς ή τυχόν ρωγμές.

H. ΚΙΝΔΥΝΟΙ, ΑΠΟΘΗΚΕΥΣΗ ΚΑΙ ΑΠΟΡΡΙΨΗ
1. Η σκληρυμένη ρητίνη δεν είναι επικίνδυνη και μπορεί να απορριφθεί μαζί με τα συνήθη απόβλητα.
2. Δείτε το ΔΔΑ για περισσότερες πληροφορίες στο support.formlabs.com.

Özel Üretim Hususları
Dental LT Clear V2 Resin teknik özellikleri aşağıda belirtilen donanım ve parametreler kullanılarakdoğrulanmıştır. Biyouyumluluk uyumluluğu için validasyonda başka hiçbir reçine ile karıştırılmamış özelbir reçine tankı ve mikseri, yapı platformu, yıkama ünitesi ve işleme sonrası ekipmanı kullanılmıştır.

1. Donanım:a. Formlabs 3D Yazıcı: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Baskı Aksesuarları: Formlabs Yapı Platformları, Formlabs Reçine Tankları

2. Yazılım:a. Formlabs PreForm

3. Baskı Parametreleri:a. Parça Yönü: Baskı yüzeyi yapı platformuna göre 0 - 30° eğimli açıyla yerleştirilirb. Katman Kalınlığı: 100 μm
c. Parça Kalınlığı:• Oklüzal Yüzeyler: Minimum 2 mm
• Duvarlar: Minimum 1 mm

4. Önerilen İşlem Sonrası Ekipman ve Aksesuarlar:a. Formlabs İşleme Aksesuarları: Form Auto, Reçine Pompalama Sistemi
b. Formlabs Onaylı Yıkama Ünitesi: Form Wash, Form Wash (2. Nesil), Form Wash L,
Ultrasonik Yıkama Ünitesic. Formlabs Onaylı Kürleme Ünitesi: Form Cure, Form Cure L, Fast CureA. YAZDIRMA
1. Kartuşu çalkalayın: Her yazdırma işinden önce kartuşu çalkalayın. Kartuş yeterince çalkalanmazsa
renk bozulmaları ve baskı hataları oluşabilir.
2. Kurulum: Reçine kartuşunu uyumlu bir Formlabs 3D yazıcıya yerleştirin. Reçine tankını yerleştirinve mikseri tanka takın.
3. Baskı:
a. PreForm yazılımını kullanarak bir yazdırma işi hazırlayın. İstenen parçanın STL dosyasını içe aktarın.
b. Parçanın yönünü seçin ve destekleri oluşturun.
c. Baskı işini yazıcıya gönderin.
d. Baskı menüsünden bir baskı işi seçerek baskıya başlayın. Yazıcı ekranında gösterilen komutları
veya iletişim kutularını takip edin. Yazıcı otomatik olarak yazdırmayı tamamlayacaktır.

B. PARÇALARI ÇIKARMA
Yapı platformunu yazıcıdan çıkarın. Parçaları yapı platformundan çıkarmak için, parça çıkarma aracını
yazdırılan parça radyesinin altına takıp aracı döndürün. Kolay ve aletsiz bir şekilde çıkarmak için Formlabs
Build Platform 2 veya Build Platform 2L kullanılabilir. Ayrıntılı teknikler için support.formlabs.com
adresini ziyaret edin.

C. YIKAMA
Basılı parçaları %99 İzopropil Alkol içeren Formlabs onaylı bir yıkama ünitesine yerleştirin.
1. Form Wash, Form Wash (2. Nesil) - Yüksek hız* veya Form L:
a. Form Wash veya Form Wash L’de 15 dakika boyunca veya temizlenene kadar yıkayın.
b. Parçaları yıkama ünitesinden çıkarın ve 5 dakika boyunca taze İzopropil Alkol içinde bekletin.
c. Yıkama sonrasında parçalar temiz görünmüyorsa yıkama ünitesindeki kullanılmış İzopropil
Alkolü taze solvent ile değiştirebilirsiniz.

TÜRKÇE

Dental LT Clear V2 Resin, oklüzal splintler, gece koruyucuları, ağız koruyucuları ve/veya beyazlatma
plakları gibi biyouyumlu, uzun süreli kullanıma uygun, çıkarılabilir dental ve ortodontik apareylerin ek
imalat ile üretimi için tasarlanmış, ışıkla kürlenebilen polimer bazlı bir reçinedir. Bu Üretim Kılavuzu,
malzemenin doğru ve güvenli kullanımını sağlamak üzere ekipman, baskı ve işleme sonrası önerileri
ve gereksinimleri sunmaktadır.

*Form Wash (2. Nesil) için Yüksek hız ayarları kullanım için onaylanmıştır.
2. Ultrasonik Yıkama Ünitesi:
NOT: Ultrasonik banyoda İzopropil Alkol kullanımı yangın veya patlama riski oluşturur. Ultrasonik
yıkama kullanırken ultrasonik yıkama üreticisinin tüm güvenlik önerilerini okuyun ve uygulayın.
a. Her yıkama için temiz %99 İzopropil Alkol kullanın.
b. Parçaları ikinci bir tek kullanımlık plastik kaba veya plastik kilitlenebilir torbaya yerleştirin,
ardından %99 İzopropil Alkol ile doldurun ve parçaların tamamen daldırıldığından emin olun.
c. İkinci kabı ultrasonik ünite su banyosuna yerleştirin ve 2 dakika boyunca veya temizlenene
kadar sonikasyon uygulayın.**Yıkama etkinliği ultrasonik ünitenin boyutuna ve gücüne bağlıdır. Formlabs testleri 36 W/L veya dahayüksek ultrasonik ünitelerle gerçekleştirilmiştir.

D. KURUTMA
1. Parçaları İzopropil Alkolden çıkarın ve oda sıcaklığında en az 30 dakika kurumaya bırakın. NOT:
Kurutma süreleri parçaların tasarımına ve ortam koşullarına göre değişebilir. Parçaları gerekenden
daha uzun süre İzopropil Alkol içinde bekletmeyin.
2. Basılan parçaları temiz ve kuru olduklarından emin olmak için inceleyin. Sonraki adımlara
geçmeden önce yüzeyde solvent kalıntısı, fazla sıvı reçine veya kalıntı parçacıkları bulunmamalıdır.
3. Hala çözücü kalıntısı varsa parçaları daha uzun süreyle kurutun. Hala reçine kalıntısı görülüyorsa
parçalar temizlenene kadar yeniden yıkayın ve kurutun.

E. SON KÜRLEME
Basılı parçaları Formlabs tarafından doğrulanmış bir son kürleme ünitesine yerleştirin ve gerekli süreboyunca kürleyin.
1. Form Cure veya Form Cure L:
a. 60 °C’de 60 dakika kürlenmeb. Form Cure veya Form Cure L ünitesinin kürleme döngüleri arasında oda sıcaklığına kadarsoğumasını bekleyin.
2. Hızlı Kürleme:a. Işık Yoğunluğu 5’te 6 dakika kürleyin
b. Fast Cure ünitesinin kürleme döngüleri arasında en az 10 dakika soğumasını bekleyin.

F. DESTEĞİ ÇIKARMA VE CİLALAMA
1. Destek izleri çıkarılmaz ve cilalanmazsa aşınmaya neden olabilir. Destekleri bir kesme diski ve elaleti, kesici pense veya diğer uygun son işlem aletlerini kullanarak çıkarın.
2. Basılı apareyleri hasta kullanmadan önce normal diş parlatma yöntemlerini kullanarak cilalayın.
3. Parçalarda çatlak olup olmadığını inceleyin. Herhangi bir hasar veya çatlak tespit ederseniz parçayı atın.

G. TEMİZLİK VE DEZENFEKSİYON
1. Eksiksiz son işlemden geçmiş parçalar, nötr sabun ve oda sıcaklığında su ile özel bir yumuşak
diş fırçası kullanılarak temizlenebilir. Dental LT Clear V2 Resin ile basılmış parçalar üzerinde dişmacunu veya başka temizlik ürünleri kullanmayın.
2. Apareyler tesis protokollerine göre temizlenebilir ve dezenfekte edilebilir. Test edilen dezenfeksiyon
yöntemi: bitmiş apareyi 5 dakika boyunca taze %70 IPA içinde bekletmek. Parçayı 5 dakikadan
uzun bir süre alkol çözeltisinde bırakmayın.
3. Temizlik ve dezenfeksiyondan sonra, tasarlanan parçanın bütünlüğünün performans
gereksinimlerini karşıladığından emin olmak için parçada hasar veya çatlak olup olmadığını
inceleyin. Herhangi bir hasar veya çatlak tespit ederseniz parçayı atın.

H. TEHLİKELER, DEPOLAMA VE BERTARAF
1. Kürlenmiş reçine tehlikeli değildir ve normal atık olarak bertaraf edilebilir.
2. Daha fazla bilgi için support.formlabs.com adresindeki Güvenlik Veri Sayfası’na bakınız.

Aspecte specifice privind fabricarea
Specificațiile Dental LT Clear V2 Resin au fost validate utilizând hardware-ul și parametrii indicați mai
jos. Pentru conformitatea cu biocompatibilitatea, validarea s-a efectuat utilizând un rezervor specificpentru rășină și un malaxor, o platformă de construcție, o unitate de spălare și un echipament de postprelucrare, care nu au fost amestecate cu alte rășini.

1. Hardware:a. Imprimantă Formlabs 3D: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Accesorii de imprimare: platforme de construcție Formlabs Built Platform, rezervoare Formlabs
Resin Tank

2. Software:a. Formlabs PreForm

3. Parametri de imprimare:a. Orientarea pieselor: suprafața adâncită este orientată în direcția opusă platformei de construcție
la un unghi de înclinare de 0°–40°
b. Grosimea stratului: 100 μm
c. Grosimea piesei:• Suprafețe ocluzale: minimum 2 mm
• Pereți: minimum 1 mm

4. Echipamente post-prelucrare și accesorii recomandate:a. Accesorii de prelucrare Formlabs: Form Auto, Resin Pumping Systemb. Unitate de spălare validată de Formlabs: Form Wash, Form Wash (a 2-a generație), Form Wash L,
unitate de spălare cu ultrasunetec. Unitate de polimerizare validată de Formlabs: Form Cure, Form Cure L, Fast Cure

A. IMPRIMARE
1. Agitați cartușul: agitați cartușul înainte de fiecare imprimare. Pot apărea modificări ale culorii sau
defecte de imprimare în cazul în care cartușul nu este agitat suficient.
2. Configurare: Introduceți rezervorul de rășină și atașați malaxorul la rezervor.
3. Imprimare:a. Pregătiți o lucrare de imprimare utilizând software-ul PreForm. Importați fișierul STL alpiesei dorite.
b. Orientați și generați suporturile.
c. Trimiteți lucrarea de imprimare la imprimantă.
d. Începeți imprimarea selectând o lucrare de imprimare din meniul de imprimare. Urmați
instrucțiunile sau casetele de dialog afișate pe ecranul imprimantei. Imprimanta va finaliza
automat imprimarea.

B. SCOATEREA PIESELOR
Îndepărtați platforma de construcție de pe imprimantă. Pentru a scoate piesele de pe platforma deconstrucție, introduceți instrumentul de îndepărtare a piesei sub stiva de piese imprimate și rotiți
instrumentul. Platforma de construcție Formlabs 2 sau platforma de construcție Formlabs 2L poate fi
utilizată pentru o scoatere ușoară, fără instrumente. Pentru tehnici detaliate, accesați support.formlabs.com.

C. SPĂLARE
Așezați piesele imprimate într-o unitate de spălare validată de Formlabs cu alcool izopropilic 99%.
1. Form Wash, Form Wash (a 2-agenerație) – viteză mare* sau Form Wash L:
a. Se spală în Form Wash sau Form Wash L timp de 15 minute sau până când sunt curate.

ROMÂNĂ

Dental LT Clear V2 Resin este o rășină polimerică fotopolimerizabilă, concepută pentru fabricarea deaparate dentare și ortodontice detașabile, biocompatibile, cu utilizare pe termen lung, cum ar fi ateleocluzale, apărători de noapte, apărători de gură și/sau tăvi de albire, prin fabricație aditivă. Acest ghidde fabricație va oferi recomandări și cerințe privind echipamentul, imprimarea și post-prelucrarea
pentru a vă asigura că utilizați acest material într-un mod corect și sigur.

b. Scoateți piesele din unitatea de spălare și înmuiați-le în alcool izopropilic proaspăt timp de
5 minute.
c. Dacă piesele nu par curate după spălare, luați în considerare înlocuirea alcoolului izopropilic
utilizat în unitatea de spălare cu un solvent nou.
*Pentru Form Wash (a 2-a generație), setările de viteză mare sunt validate pentru utilizare.
2. Unitate de spălare cu ultrasunete:NOTĂ: utilizarea alcoolului izopropilic într-o cuvă ultrasonică prezintă risc de incendiu sau de explozie.
Atunci când utilizați un aparat de spălare cu ultrasunete, citiți și urmați toate recomandările desiguranță ale producătorului.
a. Folosiți alcool izopropilic 99% curat pentru fiecare spălare.
b. Așezați piesele într-un recipient secundar de unică folosință din plastic sau într-o pungă deplastic resigilabilă, apoi umpleți cu alcool izopropilic 99%, asigurându-vă că piesele suntcomplet scufundate.
c. Așezați recipientul secundar în baia de apă a aparatului cu ultrasunete și supuneți sonicării
timp de 2 minute sau până când este curat.**Eficacitatea spălării depinde de mărimea și puterea unității cu ultrasunete. Testele Formlabs au fostefectuate cu unități cu ultrasunete la 36 W/L sau mai mult.

D. USCARE
1. Scoateți piesele din alcoolul izopropilic și lăsați-le să se usuce la aer, la temperatura camerei,
timp de cel puțin 30 de minute. NOTĂ: timpii de uscare pot varia în funcție de designul pieselor și decondițiile ambientale. Nu lăsați piesele să stea în alcool izopropilic mai mult timp decât este necesar.
2. Inspectați piesele imprimate pentru a vă asigura că sunt curate și uscate. Înainte de a trece laetapele următoare, asigurați-vă că pe suprafață nu a rămas niciun solvent rezidual, exces de rășină
lichidă sau particule de reziduuri.
3. În cazul în care solventul rezidual este încă prezent, uscați piesele mai mult timp. Dacă reziduurilede rășină sunt încă vizibile, spălați din nou piesele până când sunt curate și uscate.

E. ULTIMA POLIMERIZAREAșezați piesele imprimate într-o unitate pentru ultima polimerizare validată de Formlabs și polimerizațile pentru timpul necesar.
1. Form Cure sau Form Cure L:
a. Polimerizați timp de 60 de minute la 60 °C.
b. Lăsați unitatea Form Cure sau Form Cure L să se răcească la temperatura camerei între
ciclurile de polimerizare.
2. Polimerizare rapidă:a. Polimerizați timp de 6 minute la Light Intensity 5 (Intensitatea luminii 5)b. Lăsați unitatea Fast Cure să se răcească timp de cel puțin 10 minute între ciclurile de polimerizare.

F. SCOATEREA ȘI LUSTRUIREA SUPORTULUI
1. Semnele lăsate de suporturi pot cauza abraziune dacă nu sunt scoase și lustruite. Scoateți suporturile
folosind un disc de tăiere și o piesă manuală, un clește de tăiat sau alte instrumente de finisare adecvate.
2. Lustruiți aparatele imprimate folosind metodele obișnuite de lustruire dentară înainte de utilizarea
la pacient.
3. Inspectați piesele pentru a vedea dacă există fisuri. Aruncați-le dacă se detectează deteriorări
sau fisuri.

G. CURĂȚARE ȘI DEZINFECȚIE
1. Piesele complet post-prelucrate pot fi curățate folosind o periuță de dinți moale specială, cu săpun
cu PH neutru și apă la temperatura camerei. Nu folosiți pastă de dinți sau alte produse de curățare
pe piesele imprimate cu Dental LT Clear V2.
2. Aparatele pot fi curățate și dezinfectate în conformitate cu protocoalele unității. Metoda dedezinfecție testată: înmuierea aparatului finit în IPA 70% proaspăt timp de 5 minute. Nu lăsați piesa
în soluția de alcool mai mult de 5 minute.

3. După curățare și dezinfectare, inspectați piesa pentru a verifica dacă există deteriorări sau fisuri,
pentru a vă asigura că integritatea piesei proiectate îndeplinește cerințele de performanță.
Aruncați-o dacă se detectează deteriorări sau fisuri.

H. PERICOLE, DEPOZITARE ȘI ELIMINARE LA DEȘEURI
1. Rășina polimerizată nu este periculoasă și poate fi eliminată ca deșeurile obișnuite.
2. Pentru mai multe informații, consultați fișa cu date de securitate la adresa support.formlabs.com.

Spesifikke produksjonshensyn
Spesifikasjonene for Dental LT Clear V2 Resin er validert med maskinvare og parametrene som er
indikert nedenfor. For biokompatibilitetssamsvar ble det i godkjenningsprosessen brukt harpikstankog blander, byggeplattform, vaskeenhet og etterbehandlingsutstyr som ikke ble blandet med andre
typer harpiks.

1. Maskinvare:a. Formlabs 3D-skriver: Form 2, Form 3B/3B+, Form 3BL, Form 4B, Form 3B/3B+
b. Tilbehør til utskrift: Formlabs-byggeplattformer, Formlabs-harpikstanker

2. Programvare:a. Formlabs PreForm

3. Utskriftsparametere
a. Delorientering: Intaglio-overflate bort fra byggeplattformen i en forskjøvet vinkel på 0 - 40°
b. Lagtykkelse: 100 μm
c. Deltykkelse:• Okklusaloverflater: Minimum 2 mm
• Vegger: Minimum 1 mm

4. Anbefalt etterbehandlingsutstyr og tilbehør:
a. Formlabs tilbehør til behandling: Form Auto, pumpesystem for harpiks
b. Formlabs-validert vaskeenhet: Form Wash, Form Wash (2. generasjon), Form Wash L,
ultrasonisk vaskeenhet
c. Formlabs-godkjent herdeenhet: Form Cure, Form Cure L, Fast CureA. UTSKRIFT
1. Rist sylinderampullen: Rist sylinderampullen før hver utskriftsjobb. Fargeavvik og utskriftsfeil kan
oppstå hvis sylinderampullen ikke ristes tilstrekkelig.
2. Oppsett: Sett inn harpikspatronen i en kompatibel 3D-skriver fra Formlabs. Sett inn harpikstanken
og fest mikseren til tanken.
3. Utskrift:
a. Klargjør en utskriftsjobb ved hjelp av PreForm-programvaren. Importer ønsket del STL-fil.
b. Orienter og generer støtter.
c. Send utskriftsjobben til skriveren.
d. Begynn å skrive ut ved å velge en utskriftsjobb fra utskriftsmenyen. Følg eventuelle meldinger
eller dialogbokser som vises på skriverskjermen. Skriveren fullfører utskriften automatisk.

B. FJERNING AV DEL
Fjern byggeplattformen fra skriveren. Når du skal fjerne delene fra byggeplattformen, løsner du delenved å smette fjerneverktøyet under den utskrevne delen, og rotere verktøyet. Formlabs Build Platform 2eller Build Platform 2L kan brukes for enkel, verktøyfri fjerning. De detaljerte teknikkene finner du på
support.formlabs.com.

C. VASKING
Plasser de utskrevne delene i en Formlabs-godkjent vaskeenhet med 99 % isopropanol.
1. Form Wash, Form Wash (2. generasjon) – høy hastighet* eller Form Wash L:
a. Vaskes i 15 minutter til den er ren, i Form Wash eller Form Wash L.
b. Fjern delene fra vaskeenheten og senk ned i fersk isopropylalkohol i fem minutter.
c. Dersom delene ikke ser rene ut etter vask, bør du vurdere å bytte ut brukt isopropylalkohol ivaskeenheten med nytt løsemiddel.

NORSK

Dental LT Clear V2 Resin er en lysherdbar, polymerbasert resin som er utviklet for produksjon
av biokompatible, avtakbare tannskinner og kjeveortopediske enheter som okklusjonsskinner,
nattbeskyttere, tannbeskyttere og/eller blekeskinner ved hjelp av additiv produksjon. Denne
produksjonsveiledningen inneholder anbefalinger og krav til utstyr, utskrifter og etterbehandlingfor å sikre riktig og trygg bruk av materialet.

*For Form Wash (2. generasjon) er innstillinger for høy hastighet validert for bruk.
2. Ultrasonisk vaskeenhet:
MERK: Det å bruke isopropanol i et ultrasonisk bad medfører brann- og eksplosjonsfare. Når dubruker en ultrasonisk vask må du lese og følge alle sikkerhetsanbefalinger fra produsenten av den
ultrasoniske vasken.
a. Bruk ren 99 % isopropanol for hver vask.
b. Plasser deler i en annen engangs plastikkbeholder eller lukkbar plastikkpose og fyll med
99 % isopropylalkohol. Pass på at alle delene er helt dekket av væske.
c. Plasser den andre beholderen i den ultrasoniske enhetens vannbad og soniker i to minutter
eller til den er ren.
*Effektiviteten på vasken avhenger av størrelsen og styrken til den ultrasoniske enheten. Formlabstestingen ble gjort med ultrasoniske enheter på 36 W/L eller høyere.

D. TØRKING
1. Fjern delene fra isopropanolen og la dem tørke i romtemperatur i minst 30 minutter. NOTE:
Tørketiden kan variere avhengig av utformingen på delene og omgivelsene. Ikke la deler ligge iisopropanol lenger enn nødvendig.
2. Inspisert utskrevne deler for å forsikre deg om at de er rene og tørre. Ingen gjenværende
løsemidler eller flytende harpiks skal være igjen på overflaten når du går videre til neste steg.
3. Dersom det fremdeles finnes gjenværende løsemiddel på delen må du la den tørke lenger.
Dersom du fremdeles ser rester av harpiks, vask delene på nytt til de er rene og tørre.

E. ETTERHERDING
Plasser det utskrevne delene i en herdeenhet som er godkjent av Formlabs, og la dem herde så lenge
som kreves.
1. Form Cure eller Form Cure L:
a. Herd i 30 minutter ved 80 °C.
b. La Form Cure eller Form Cure L-enheten kjøles ned til romtemperatur mellom herde-syklusene.
2. Fast Cure:a. Herd i seks minutter ved Light Intensity 5b. La Fast Cure-enheten kjøles ned i minst 10 minutter mellom herde-syklusene.

F. FJERNING AV STØTTE OG POLERING
1. Støttemerker kan forårsake skraping hvis de ikke fjernes og poleres. Fjern støtter ved hjelp av en
kutte-disk og et håndstykke, vinkelkutter eller andre passende verktøy.
2. Poler det utskrevne apparatet med vanlig tannpoleringsmidler, før pasienten tar det i bruk.
3. Inspiser delene for eventuelle sprekker. Kast dersom du finner skader eller sprekker.

G. VASKING OG DESINFISERING
1. Ferdige, post-prossesserte deler kan vaskes med en egen, my tannbørste med nøytral såte og
vann i romtemperatur. Ikke bruk tannkrem eller andre vaskemidler på deler som er skrevet ut med
Dental LT Clear V2 Resin.
2. Apparatene kan vaskes og desinfiseres slik som beskrevet i fasilitets-protokollene. Testet
desinfiseringsmetode: Senk det ferdige apparatet i fersk 70 % IPA i fem minutter. Ikke la delene
ligge i alholooppløsningen i mer enn fem minutter.
3. Etter vasking og desinfisering må delene inspiseres for skader og sprekker for å sjekke at deutformede delene er hele og møter prestasjonskravene. Kast dersom du finner skader eller sprekker.

H. FARE, OPPBEVARING OG AVHENDING
1. Herdet harpisk er ikke farlig og kan kastes som vanlig avfall.
2. Se SDS for mer informasjon på support.formlabs.com.

Īpaši ražošanas apsvērumi
Dental LT Clear V2 Resin specifikācijas ir apstiprinātas, izmantojot turpmāk norādīto aparatūru un
parametrus. Lai nodrošinātu atbilstību biosaderības prasībām, validācijā tika izmantota īpaša sveķu
tvertne, veidošanas platforma, mazgāšanas iekārta un pēcapstrādes iekārta, kas netika sajauktas arcitiem sveķiem.

1. Aparatūra:a. Formlabs 3D Printer: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Drukas piederumi: Formlabs Build Platforms, Formlabs Resin Tanks

2. Programmatūra:a. Formlabs PreForm

3. Drukāšanas parametri:a. Daļas orientācija: Iekšparauga virsma, kas vērsta prom no veidošanas platformas 0 - 40° slīpuma leņķī
b. Slāņa biezums: 100 μm
c. Daļas biezums:• Okluzālās virsmas: vismaz 2 mm
• Sienas: minimālais biezums: 1 mm

4. Ieteicamais pēcapstrādes aprīkojums un piederumi:
a. Formlabs apstrādes piederumi: Form Auto, Resin Pumping Systemb. Formlabs validēts mazgāšanas bloks: Form Wash, Form Wash (2. paaudzes), Form Wash L,
Ultrasonic Wash Unitc. Formlabs validēta cietināšanas iekārta: Form Cure, Form Cure L, Fast Cure

A. DRUKĀŠANA
1. Sakratiet kārtridžu: Pirms katra drukāšanas uzdevuma sakratiet kārtridžu. Krāsu novirzes undrukāšanas kļūdas var rasties, ja kārtridžs nav pietiekami sakratīts.
2. Uzstādīšana: Ievietojiet sveķu tvertni un pievienojiet maisītāju tvertnei.
3. Drukāšana:a. Sagatavojiet drukāšanas uzdevumu, izmantojot PreForm programmatūru. Importējiet vēlamo
STL failu.
b. Orientējiet un izveidojiet balstus.
c. Nosūtiet drukāšanas uzdevumu uz printeri.
d. Sāciet drukāšanu, drukāšanas izvēlnē izvēloties drukāšanas uzdevumu. Izpildiet visus printera
ekrānā parādītos norādījumus vai dialoglodziņus. Printeris automātiski pabeigs drukāšanu.

B. DAĻU NOŅEMŠANANoņemiet veidošanas platformu no printera. Lai noņemtu daļas no veidošanas platformas, ievietojietdaļu noņemšanas rīku zem drukātās daļas plosta un pagrieziet rīku. Formlabs Build Platform 2 vai Build
Platform 2L var izmantot ērtai noņemšanai bez instrumentiem. Sīkāku informāciju par metodēm skatiet
vietnē support.formlabs.com.

C. MAZGĀŠANA
Ievietojiet izdrukātās daļas Formlabs validētā mazgāšanas iekārtā ar 99 % izopropilspirtu.
1. Form Wash, Form Wash (2. paaudze) - liela ātruma* vai Form Wash L:
a. Mazgājiet daļas Form Wash vai Form Wash L 15 minūtes vai līdz tīrībai.
b. Izņemiet daļas no mazgāšanas iekārtas un iemērciet svaigā izopropilspirtā uz 5 minūtēm.
c. Ja pēc mazgāšanas daļas nešķiet tīras, apsveriet iespēju mazgāšanas ierīcē izmantoto
izopropilspirtu aizstāt ar svaigu šķīdinātāju.

LATVIEŠUVALODĀ

Dental LT Clear V2 Resin ir uz gaismā cietējošu polimēru bāzes veidots sveķu materiāls, kas paredzēts
bioloģiski saderīgu, ilgstoši lietojamu, noņemamu zobārstniecības un ortodontijas piederumu, piemēram,sakodiena šinu, nakts aizsargu, mutes aizsargu un/vai balināšanas paplākšņu izgatavošanai, izmantojot
piedevu ražošanu. Šajā ražošanas rokasgrāmatā ir sniegti ieteikumi un prasības attiecībā uz aprīkojumu,
drukāšanu un pēcapstrādi, lai nodrošinātu pareizu un drošu šī materiāla izmantošanu.

*Form Wash (2. paaudzes) ir lietošanai apstiprināti liela ātruma iestatījumi.
2. Ultrasonic Wash Unit:PIEZĪME: Izopropilspirta izmantošana ultraskaņas vannā rada ugunsgrēka vai eksplozijas risku.
Lietojot ultraskaņas mazgāšanas iekārtu, izlasiet un ievērojiet visus ultraskaņas mazgāšanas iekārtas
ražotāja drošības ieteikumus.
a. Katrai mazgāšanas reizei izmantojiet tīru 99 % izopropilspirtu.
b. Ievietojiet daļas sekundārā vienreizlietojamā plastmasas traukā vai atkārtoti aizveramā plastmasas
maisiņā, pēc tam piepildiet ar 99 % izopropilspirtu, nodrošinot, ka daļas ir pilnībā iegremdētas.
c. Ievietojiet sekundāro trauku ultraskaņas iekārtas ūdens vannā un apstrādājiet ar ultraskaņu
2 minūtes vai līdz tīrībai.**Mazgāšanas efektivitāte ir atkarīga no ultraskaņas iekārtas lieluma un jaudas. Formlabs testēšana
tika veikta ar ultraskaņas iekārtām ar 36 W/L vai lielāku jaudu.

D. ŽĀVĒŠANA
1. Izņemiet daļas no izopropilspirta un atstājiet vismaz 30 minūtes nožūt istabas temperatūrā.
PIEZĪME: Žāvēšanas laiks var atšķirties atkarībā no daļu konstrukcijas un apkārtējās vides
apstākļiem. Neļaujiet daļām atrasties izopropilspirtā ilgāk, nekā nepieciešams.
2. Pārbaudiet izdrukātās daļas, lai pārliecinātos, ka tās ir tīras un sausas. Pirms turpmāko darbību
veikšanas uz virsmas nedrīkst palikt šķīdinātāja pārpalikumi, šķidro sveķu pārpalikumi vai
pārpalikumu daļiņas.
3. Ja šķīdinātāja pārpalikumi vēl ir saglabājušies, žāvējiet daļas ilgāk. Ja joprojām ir redzami sveķu
pārpalikumi, vēlreiz nomazgājiet daļas, līdz tās ir tīras un sausas.

E. PĒCCIETINĀŠANA
Ievietojiet izdrukātās daļas Formlabs apstiprinātā pēccietināšanas iekārtā un atstājiet tās sacietēt
nepieciešamo laika periodu.
1. Form Cure vai Form Cure L:
a. Cietiniet 60 minūtes 60 °C temperatūrāb. Starp cietināšanas cikliem ļaujiet Form Cure vai Form Cure L atdzist līdz istabas temperatūrai.
2. Ātra cietināšana:a. Lieciet cietināt 6 minūtes ar gaismas intensitāti 5
b. Starp cietināšanas cikliem ļaujiet Fast Cure iekārtai atdzist vismaz 10 minūtes.

F. BALSTU NOŅEMŠANA UN PULĒŠANA
1. Balstu aizzīmes var būt abrazīvas, ja tās netiek noņemtas un pulētas. Noņemiet balstus, izmantojot
griešanas disku un rokas instrumentu, griešanas knaibles vai citus piemērotus apdares instrumentus.
2. Pirms lietošanas pacientam izdrukātās ierīces pulē, izmantojot parastās zobu pulēšanas metodes.
3. Pārbaudiet, vai daļās nav radušās plaisas. Izmetiet, ja tiek konstatēti bojājumi vai plaisas.

G. TĪRĪŠANA UN DEZINFEKCIJA
1. Pilnībā apstrādātas daļas var tīrīt, izmantojot īpašu mīkstu zobu suku ar neitrālām ziepēm un
istabas temperatūras ūdeni. Neizmantojiet zobu pastu vai citus tīrīšanas līdzekļus daļām, kas
izdrukātas ar Dental LT Clear V2 Resin.
2. Ierīces var tīrīt un dezinficēt saskaņā ar iestādes protokoliem. Pārbaudīta dezinfekcijas metode:
gatavās ierīces mērcēšana svaigā 70 % IPA uz 5 minūtēm. Neatstājiet daļu spirta šķīdumā ilgāk
par 5 minūtēm.
3. Pēc tīrīšanas un dezinfekcijas pārbaudiet, vai daļa nav bojāta vai ieplaisājusi, lai pārliecinātos,ka projektētās daļas integritāte atbilst veiktspējas prasībām. Izmetiet, ja tiek konstatēti bojājumi
vai plaisas.

H. APDRAUDĒJUMI, GLABĀŠANA UN IZNĪCINĀŠANA
1. Cietinātie sveķi nav bīstami un tos var izmest kā parastos atkritumus.
2. Plašāku informāciju skatīt SDS vietnē support.formlabs.com.

Specialūs gamybos aspektai„Dental LT Clear V2 Resin“ specifikacijos buvo patvirtintos naudojant toliau nurodytą techninę įrangą
ir parametrus. Siekiant užtikrinti biologinio suderinamumo atitiktį, patvirtinant buvo naudojama speciali
dervos talpa ir mikesrį, konstravimo platforma, plovimo įrenginys ir tolesnio apdorojimo įranga, kuriose
nebuvo naudojama jokia kita derva.

1. Techninė įranga:a. Formlabs 3D spausdintuvas: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Spausdinimo priedai: Formlabs Build Platforms, Formlabs dervos talpos

2. Programinė įranga:a. Formlabs PreForm

3. Spausdinimo parametrai:
a. Dalies padėtis: giliaspaudės paviršius nukreiptas nuo platformos 0 - 40° pakreiptu kampu
b. Sluoksnio storis: 100 μm
c. Dalies storis:• Okliuziniai paviršiai: mažiausiai 2 mm
• Sienos: mažiausiai 1 mm

4. Rekomenduojama tolesnio apdorojimo įranga ir priedai:a. Formlabs apdorojimo priedai: Form Auto, dervos pumpavimo sistema
b. Formlabs patvirtintas plovimo įrenginys: Form Wash, Form Wash (2-os kartos), Form Wash L,
ultragarsinis plovimo įrenginysc. Formlabs patvirtintas kietėjimo įrenginys:Form Cure, Form Cure L, Fast Cure

A. SPAUSDINIMAS
1. Sukratykite kasetę: prieš kiekvieną spausdinimo užduotį sukratykite kasetę. Nepakankamai
sukračius kasetę, gali atsirasti spalvų nuokrypių ir spausdinimo sutrikimų.
2. Nustatykite: Įstatykite dervos rezervuarą ir prie rezervuaro pritvirtinkite maišytuvą.
3. Spausdinimas:
a. Paruoškite spausdinimo užduotį naudodami „PreForm“ programinę įrangą. Importuokite
norimos dalies STL failą.
b. Orientuokite ir generuokite atramas.
c. Siųskite spausdinimo užduotį į spausdintuvą.
d. Pradėkite spausdinti pasirinkdami spausdinimo užduotį iš spausdinimo meniu. Vykdykite
visus spausdintuvo ekrane ar dialogo lange rodomus raginimus. Spausdintuvas automatiškaiužbaigs spausdinimą.

B. DALIES PAŠALINIMAS
Pašalinkite kūrimo platformą iš spausdintuvo. Norėdami nuimti dalis nuo kūrimo platformos, dalių
išėmimo įrankį įkiškite po atspausdinta dalimi ir pasukite įrankį. Formlabs Build 2 platformą arba
Formlabs Build 2L platformą galima paprastai išimti nenaudojant jokių įrankių. Išsamesnės informacijos
apie metodus rasite svetainėje support.formlabs.com.

C. PLOVIMAS
Atspausdintas dalis įdėkite į Formlabs patvirtintą plovimo įrenginį su 99 % izopropilo alkoholiu.
1. Form Wash, Form Wash (2-os kartos) – High speed* arba Form Wash L:
a. Plaukite 15 minučių arba kol plovimo forma arba plovimo forma L bus švari.
b. Išimkite dalis iš plovimo įrenginio ir 5 minutes pamirkykite šviežiame izopropilo alkoholyje.

LIETUVIŲ

Dental LT Clear V2 Resin – tai šviesoje kietėjanti polimero pagrindu pagaminta derva, skirta
biologiškai suderinamiems, ilgalaikiams, išimamiems odontologiniams ir ortodontiniams aparatams,
tokiems kaip sąkandžio įtvarai, naktinės apsaugos, burnos apsaugosir (arba) balinimo padėklai,
priedams gaminti. Šiame gamybos vadove bus pateiktos įrangos, spausdinimo ir tolesnio apdorojimo
rekomendacijos bei reikalavimai, siekiant užtikrinti teisingą ir saugų šios medžiagos naudojimą.

c. Jei po plovimo dalys neatrodo švarios, apsvarstykite galimybę plovimo įrenginyje panaudotą
izopropilo alkoholį pakeisti nauju tirpikliu.
*Form Wash (2-os kartos) Didelio greičio nustatymai yra patvirtinti naudojimui.
2. Ultragarsinis plovimo įrenginys:
PASTABA: naudojant izopropilo alkoholį ultragarso vonioje kyla gaisro arba sprogimo pavojus.
Naudodami ultragarso plovimą, perskaitykite ir laikykitės visų ultragarso plovyklos gamintojo
saugos rekomendacijų.
a. Kiekvieno plovimo metu naudokite švarų 99 % izopropilo alkoholį.
b. Sudėkite dalis į antrinį vienkartinį plastikinį indą arba plastikinį uždaromą maišelį ir užpilkite
99 % izopropilo alkoholiu, kad dalys būtų visiškai panardintos.
c. Įdėkite antrinį indą į ultragarso įrenginio vandens vonelę ir 2 minutes sonikuokite arba tol,
kol jis bus švarus .**Plovimo veiksmingumas priklauso nuo ultragarso įrenginio dydžio ir galios. Formlabs bandymai buvo
atliekami su ultragarso įrenginiais, kurių galia 36 W/L arba didesnė.

D. DŽIOVINIMAS
1. Išimkite dalis iš izopropilo alkoholio ir palikite džiūti kambario temperatūroje bent 30 minučių.
PASTABA: džiūvimo laikas gali skirtis priklausomai nuo dalių konstrukcijos ir aplinkos sąlygų.
Nepalikite dalių izopropilo alkoholyje ilgesniam laikui nei reikia.
2. Apžiūrėkite spausdinamas dalis, kad įsitikintumėte, jog jos yra švarios ir sausos. Prieš pradedant
tolesnius veiksmus ant paviršiaus neturi likti tirpiklio likučių, skystos dervos pertekliaus ar likučių dalelių.
3. Jei vis dar yra tirpiklio likučių, ilgiau džiovinkite dalis. Jei vis dar matomi dervos likučiai, dar kartą
nuplaukite dalis, kol jos bus švarios ir sausos.

E. PO KIETINIMO PROCEDŪROS
Įdėkite atspausdintas dalis į Formlabs patvirtintą įrenginį po kietinimo ir kietinkite reikiamą laiką.
1. Kietinimo forma arba kietinimo forma L:
a. Kietinimas 60 minučių 60 °C temperatūroje
b. Tarp kietinimo ciklų leiskite kietinimo formos arba kietinimo formos L įrenginiui atvėsti iki
kambario temperatūros.
2. Greitas kietinimas:a. 6 minutes kietinti 5 šviesos intensyvumu
b. Tarp kietinimo ciklų leiskite greito kietinimo įrenginiui atvėsti bent 10 minučių.

F. ATRAMŲ PAŠALINIMAS IR POLIRAVIMAS
1. Atramos žymės gali sukelti dilimą, jei jos nepašalinamos ir nepoliruojamos. Atramas pašalinkite
naudodami pjovimo diską ir rankinį antgalį, pjovimo žnyples arba kitus tinkamus apdailos įrankius.
2. Prieš naudodami spausdintus prietaisus, poliruokite juos įprastais dantų poliravimo metodais.
3. Apžiūrėkite, ar dalyse nėra įtrūkimų. Jei yra pažeidimų ar įtrūkimų, išmeskite.

G. VALYMAS IR DEZINFEKAVIMAS
1. Visiškai po procedūros apdorotas dalis galima nuvalyti naudojant tam skirtą minkštą dantų šepetėlį
su neutraliu muilu ir kambario temperatūros vandeniu. Nenaudokite dantų pastos ar kitų valymo
priemonių dalims, atspausdintoms su Dental LT Clear V2 Resin.
2. Prietaisus galima valyti ir dezinfekuoti pagal įrenginio protokolus. Išbandytas dezinfekavimo būdas:paruoštas prietaisas 5 minutes mirkomas šviežiame 70 % IPA tirpale. Nelaikykite dalies alkoholio
tirpale ilgiau nei 5 minutes.
3. Po valymo ir dezinfekavimo patikrinkite, ar dalis nėra pažeista ar įtrūkusi, kad įsitikintumėte,jog suprojektuotos dalies vientisumas atitinka eksploatacinius reikalavimus. Jei yra pažeidimųar įtrūkimų, išmeskite.

H. PAVOJAI, LAIKYMAS IR UTILIZAVIMAS
1. Sukietėjusi derva yra nepavojinga ir gali būti išmesta kaip įprastos atliekos.
2. Daugiau informacijos rasite SDS adresu support.formlabs.com.

Konkreetsed valmistamisega seotud kaalutlused
Dental LT Clear V2 Resin tehnilised nõuded on valideeritud allpool esitatud riistvara ja parameetreid
kasutades. Bioloogilise ühilduvuse tagamiseks kasutati valideerimisel spetsiaalset vaigupaaki ja miksrit,ehitusplatvormi, pesemisseadet ja järeltöötlusseadmeid, mis ei puutunud kokku teiste vaikudega.

1. Riistvara:a. Formlabs 3D-printer: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Printimistarvikud: Formlabs ehitusplatvormid, Formlabs vaigupaagid

2. Tarkvara:a. Formlabs PreForm

3. Printimise parameetrid:a. Detaili asetus: sügavtrükipind on suunatud ehitusplatvormist eemale 0-40° kallutatud nurga allb. Kihi paksus: 100 μm
c. Detaili paksus:• Oklusaalsed pinnad: vähemalt 2 mm
• Seinad: minimaalselt 1 mm

4. Soovitatavad järeltöötlusseadmed ja tarvikud:a. Formlabs töötlemistarvikud: Form Auto, Resin Pumping Systemb. Formlabs valideeritud pesemisseade: Form Wash, Form Wash (2. põlvkond), Form Wash L,
Ultrasonic Wash Unitc. Formlabsi valideeritud järeltöötlusseade: Form Cure, Form Cure L, Fast CureA. PRINTIMINE
1. Kassetti raputamine: Raputage kassetti enne iga printimistööd. Kui kassetti ei raputata piisavalt,võivad tekkida värvide kõrvalekalded ja printimisvigastused.
2. Ülesseadmine: Sisestage vaigupaak ja kinnitage mikser paagile.
3. Printimine:a. Valmistage printimistöö ette, kasutades PreForm tarkvara. Importige soovitud detaili STL-fail.
b. Suunistage ja looge toed.
c. Saatke printimistöö printerisse.
d. Alustage printimist, valides printimismenüüst printimistöö. Järgige kõiki printeri ekraanil
kuvatavaid juhiseid või dialooge. Printer lõpetab printimise automaatselt.

B. DETAILI EEMALDAMINE
Eemaldage ehitusplatvorm printerist. Detailide konstruktsiooniplatvorm eemaldamiseks kinnitage
kiiluga detailide eemaldamise tööriist prinditud detaili platvormi alla ja pöörake tööriista. Formlabs
Build Platform 2 või Build Platform 2L võib kasutada lihtsaks, tööriistavabaks eemaldamiseks.
Üksikasjalikud tehnikad leiate aadressilt support.formlabs.com.

C. PESEMINE
Asetage prinditud detailid Formlabs-i valideeritud pesemissseadmesse 99% isopropüülalkoholiga.
1. Form Wash, Form Wash (2. põlvkond) - High Speed*, või Form Wash L:
a. Peske Form Wash või Form Wash L tarviku abil 15 minutit või kuni detail on puhas.
b. Võtke detailid pesemisseadmest välja ja leotage neid 5 minutit värskes isopropüülalkoholis.
c. Kui detailid ei tundu pärast pesemist puhtad, kaaluge pesemisseadmes kasutatud
isopropüülalkoholi asendamist värske lahustiga.
*Form Wash (2. põlvkond) puhul on suure kiiruse seadistus kasutamiseks kinnitatud.

EESTI KEELES

Dental LT Clear V2 Resin on valguskõvenev polümeeripõhine vaik, mis on mõeldud bioloogiliseltühilduvate, pikaajaliseks kasutamiseks mõeldud eemaldatavate hambaravi- ja ortodontiliste
abivahendite, näiteks hambumust korrigeerivate kapede, öökaitsmete, suukaitsmete ja/või
valgendusaluste valmistamiseks additiivse tootmise teel. Käesolev tootmisjuhend annab soovitusi
ja sisaldab nõudeid materjali õige ning ohutu kasutamise tagamiseks seadmete, printimise ja
järeltöötlusele kohta.

2. Ultrasonic Wash Unit:MÄRKUS: Isopropüülalkoholi kasutamine ultrahelivannis tekitab tule- või plahvatusohu. Ultrahelipesuri
kasutamisel lugege ja järgige kõiki tarviku tootja ohutusnõudeid.
a. Kasutage igaks pesuks puhast 99% isopropüülalkoholi.
b. Asetage detailid sekundaarsesse ühekordselt kasutatavasse plastkonteinerisse võitaassuletavasse kilekotti ja täitke see 99% isopropüülalkoholiga, tagades, et detailid oleksidtäielikult vedeliku sees.
c. Asetage sekundaarne konteiner ultrahelipesuri vesivanni ja töödelge ultraheliga 2 minutit või
kuni konteiner on puhas.**Pesemise tõhusus sõltub ultraheliseadme suurusest ja võimsusest. Formlabs testid viidi läbi
ultraheliseadmetega, mille võimsus oli 36 W/L või kõrgem.

D. KUIVATAMINE
1. Eemaldage detailid isopropüülalkoholist ja laske toatemperatuuril vähemalt 30 minutit õhu
käes kuivada. MÄRKUS: Kuivamisajad võivad varieeruda sõltuvalt detailide disainist ja
keskkonnatingimustest. Ärge laske detailidel isopropüülalkoholis olla kauem kui vaja.
2. Kontrollige prinditud detaile, veendumaks, et need on puhtad ja kuivad. Enne järgmiste etappidega
jätkamist, veenduge, et detaili pindadel ei oleks lahusti jääke, liigset vedelat vaiku ega jääkosakesi.
3. Kui lahusti jäägid on alles, kuivatage osi kauem. Kui vaigujäägid on endiselt nähtavad, peske
detaile uuesti, kuni need on puhtad ja kuivad.

E. JÄRELTÖÖTLUS
Asetage prinditud detailid Formlabs-i valideeritud järelkõvenemise seadmesse ja töödelge neidnõutava aja jooksul.
1. Form Cure või Form Cure L:
a. Töödelda 60 minutit 60 °C juuresb. Laske Form Cure või Form Cure L seadmel kõvastumistsüklite vahel jahtuda toatemperatuurini.
2. Kiire ravi:
a. Töödelge 6 minutit valgustugevuse 5 juuresb. Laske kiirtöötlusseadmel kõvenemistsüklite vahel jahtuda vähemalt 10 minutit.

F. TOE EEMALDAMINE JA POLEERIMINE
1. Tugede jäljed võivad korralikult eemaldamata ja poleerimata jätmisel põhjustada suushõõrdumist. Eemaldage toed lõikeketta ja käsiinstrumendi, lõiketangide või muude sobivate
viimistlusvahendite abil.
2. Poleerige prinditud detailid, kasutades tavapäraseid hambapoleerimismeetodeid enne patsiendi
kasutusse andmist.
3. Kontrollige detaile võimalike mõrade suhtes. Mistahes kahjustuse või mõra avastamisel, visake
detail minema.

G. PUHASTAMINE JA DESINFITSEERIMINE
1. Täielikult järeltöödeldud osi saab puhastada spetsiaalse pehme hambaharjaga, kasutades
neutraalset seepi ja leiget vett. Ärge kasutage Dental LT Clear V2 Resin prinditud detailide
puhastamiseks hambapastat ega muid puhastusvahendeid.
2. Abivahendeid võib puhastada ja desinfitseerida vastavalt seadme protokollidele. Testitud
desinfitseerimismeetod: valmisoleva detaili leotamine värskes 70% IPA lahuses 5 minuti jooksul.
Ärge jätke detaili alkoholilahusesse kauemaks kui 5 minutit.
3. Pärast puhastamist ja desinfitseerimist kontrollige detaili kahjustuste või mõrade suhtes, et tagada
projekteeritud detaili terviklikkus vastavalt jõudlusnõuetele. Mistahes kahjustuse või mõraavastamisel, visake detail minema.

H. OHUD, LADUSTAMINE JA KÕRVALDAMINE
1. Kõvenenud vaik ei ole ohtlik ja selle võib kõrvaldada olmejäätmena.
2. Ohutuskaartide lisateave on saadaval aadressil support.formlabs.com.

Špecifické výrobné aspektyŠpecifikácie živice Dental LT Clear V2 Resin boli overené pomocou nižšie uvedeného hardvéru aparametrov. Na účely splnenia požiadaviek na biokompatibilitu bolo vykonané overenie s vyhradenounádržou na živicu a zmiešavačom, stavebnou podložkou, čistiacou stanicou a zariadením na následné
spracovanie, ktoré neboli v kontakte so žiadnou inou živicou.

1. Hardvér:a. 3D tlačiareň Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Príslušenstvo pre tlač: Platformy Formlabs Build Platform, nádrže Formlabs Resin Tank

2. Softvér:
a. Formlabs PreForm

3. Parametre tlače:a. Orientácia dielov: povrch hĺbkotlače smerom od stavebnej podložky pod uhlom 0 – 40 °b. Hrúbka vrstvy: 100 μm
c. Hrúbka dielu:• Oklúzne plochy: aspoň 2 mm
• Steny: aspoň 1 mm

4. Odporúčané zariadenia a príslušenstvo na následné spracovanie:a. Príslušenstvo Formlabs na spracovanie: Form Auto, systém na čerpanie živiceb. Čistiaca stanica overená spoločnosťou Formlabs: Form Wash, Form Wash (2. generácia),
Form Wash L, ultrazvuková čistiaca stanicac. Vytvrdzovacia stanica overená spoločnosťou Formlabs: Form Cure, Form Cure L, Fast CureA. TLAČ
1. Potraste kazetu: pred každou tlačovou úlohou potraste kazetu. Pri nedostatočnom potrasení
kazety môže dôjsť k farebným odchýlkam a poruchám tlače.
2. Nastavenie: Vložte kazetu so živicou do kompatibilnej 3D tlačiarne Formlabs. Vložte nádrž naživicu a pripojte k nej zmiešavač.
3. Tlač:a. Pripravte tlačovú úlohu pomocou softvéru PreForm. Importujte požadovaný súbor STL.
b. Nastavte orientáciu a vygenerujte podpery.
c. Odošlite tlačovú úlohu do tlačiarne.
d. Spustite tlač výberom tlačovej úlohy z ponuky tlače. Postupujte podľa všetkých výziev alebo
dialógových okien zobrazených na obrazovke tlačiarne. Tlačiareň dokončí tlač automaticky.

B. ODSTRÁNENIE DIELU
Odstráňte stavebnú podložku z tlačiarne. Ak chcete odstrániť diely zo stavebnej podložky, upevnite
nástroj na odstránenie dielov pod vytlačenú medzivrstvu dielu a otáčajte nástrojom. Na jednoduché
odstránenie bez použitia nástrojov možno použiť Formlabs Build Platform 2 alebo Build Platform 2L.
Podrobné postupy nájdete na stránke support.formlabs.com.

C. ČISTENIE
Umiestnite vytlačené diely do čistiacej stanice overenej spoločnosťou Formlabs s 99 % izopropylalkoholom.
1. Form Wash, Form Wash (2. generácia) - vysoká rýchlosť* alebo Form Wash L:a. Čistite v stanici Form Wash alebo Form Wash L 15 minút alebo kým nebudú diely čisté.
b. Vyberte diely z čistiacej stanice a namočte ich na 5 minút do čerstvého izopropylalkoholu.
c. Ak sa diely po umytí nezdajú čisté, zvážte výmenu použitého izopropylalkoholu v umývacej
stanici za čerstvé rozpúšťadlo.

SLOVENČINA

Dental LT Clear V2 Resin je svetlom vytvrdzovaná živica na báze polyméru určená na aditívnu výrobu
biokompatibilných, dlhodobo použiteľných snímateľných zubných a ortodontických pomôcok, ako
sú okluzálne dlahy, nočné chrániče, chrániče zubov a/alebo bieliace vaničky. V tomto sprievodcovivýrobou sú uvedené odporúčania a požiadavky týkajúce sa zariadenia, tlače a následného
spracovania, aby sa zabezpečilo správne a bezpečné používanie tohto materiálu.

*Pre Form Wash (2. generácia) boli schválené nastavenia vysokej rýchlosti.
2. Ultrazvuková čistiaca stanica:POZNÁMKA: Používanie izopropylalkoholu v ultrazvukovom čističi predstavuje riziko požiaru alebovýbuchu. Pri používaní ultrazvukového čističa si prečítajte a dodržiavajte všetky bezpečnostné
odporúčania jeho výrobcu.
a. Pri každom čistení použite čistý 99 % izopropylalkohol.
b. Umiestnite diely do sekundárnej jednorazovej plastovej nádoby alebo plastového uzatvárateľného
vrecka a potom ich naplňte 99 % izopropylalkoholom tak, aby boli diely úplne ponorené.
c. Umiestnite sekundárnu nádobu do vodného kúpeľa v ultrazvukovom čističi a aplikujte
ultrazvukové vibrácie 2 minúty alebo kým nebudú diely čisté.** Účinnosť čistenia závisí od veľkosti a výkonu ultrazvukovej stanice. Testovanie spoločnosti Formlabs
bolo uskutočnené s ultrazvukovými jednotkami s výkonom 36 W/l alebo vyšším.

D. SUŠENIE
1. Vyberte diely z izopropylalkoholu a nechajte ich schnúť pri izbovej teplote aspoň 30 minút.
POZNÁMKA: Čas schnutia sa môže líšiť v závislosti od konštrukcie dielov a okolitých podmienok.
Nenechávajte diely v izopropylalkohole dlhšie, ako je potrebné.
2. Skontrolujte, či sú vytlačené diely čisté a suché. Pred pokračovaním v ďalších krokoch by na
povrchu nemali zostať zvyšky roztoku, prebytočná tekutá živica ani zvyšky iných častíc.
3. Ak sú zvyšky roztoku stále prítomné, sušte diely dlhšie. Ak sú zvyšky živice stále viditeľné, vyčistite
diely znovu, kým nebudú čisté a suché.

E. NÁSLEDNÉ VYTVRDZOVANIE
Umiestnite vytlačené diely do stanice na dodatočné vytvrdzovanie overenej spoločnosťou Formlabs avytvrdzujte ich požadovaný čas.
1. Forma Cure alebo Forma Cure L:a. Vytvrdzovanie 60 minút pri teplote 60 °C
b. Medzi vytvrdzovacími cyklami nechajte stanicu Form Cure alebo Form Cure L vychladnúť na
izbovú teplotu.
2. Rýchle vytvrdzovanie:
a. Vytvrdzujte 6 minút pri intenzite svetla 5b. Medzi jednotlivými vytvrdzovacími cyklami nechajte stanicu Fast Cure vychladnúť aspoň 10 minút.

F. ODSTRÁNENIE PODPERY A LEŠTENIE
1. Neodstránené alebo nevyleštené značky po podperách môžu spôsobiť odieranie. Podpery
odstráňte pomocou rezacieho kotúča, dentálnej násady (handpiece), štípacích klieští alebo iných
vhodných nástrojov na dokončovanie.
2. Vytlačené pomôcky pred použitím pacientom vyleštite bežnými spôsobmi dentálneho leštenia.
3. Skontrolujte, či na dieloch nie sú praskliny. Ak zistíte akékoľvek poškodenie alebo praskliny, diel vyhoďte.

G. ČISTENIE A DEZINFEKCIA
1. Úplne následne spracované diely možno čistiť pomocou špeciálnej mäkkej zubnej kefky sneutrálnym mydlom a vodou izbovej teploty. Na čistenie dielov vytlačených s použitím živice
Dental LT Clear V2 nepoužívajte zubnú pastu ani iné čistiace prostriedky.
2. Pri čistení a dezinfiekcii je potrebné postupovať podľa protokolov pracoviska. Testovaná
metóda dezinfekcie: namočenie hotového dielu do čerstvého roztoku 70 % IPA počas 5 minút.
Nenechávajte diel v alkoholovom roztoku dlhšie ako 5 minút.
3. Po vyčistení skontrolujte, či diel nie je poškodený alebo prasknutý, aby ste sa uistili, že celistvosť
navrhnutého dielu spĺňa požiadavky na funkčnosť. Ak zistíte akékoľvek poškodenie alebopraskliny, diel vyhoďte.

H. NEBEZPEČENSTVÁ, SKLADOVANIE A LIKVIDÁCIA
1. Vytvrdnutá živica nie je nebezpečná a môže byť zlikvidovaná ako bežný odpad.
2. Viac informácií nájdete v karte bezpečnostných údajov na support.formlabs.com.

Posebni proizvodni dejavniki
Specifikacije smole Dental LT Clear V2 Resin so bile potrjene z uporabo spodaj navedene strojne
opreme in parametrov. Zaradi skladnosti z biokompatibilnostjo so bili pri potrjevanju uporabljeni
poseben rezervoar za smolo, platforma za izdelavo, enota za pranje in oprema za naknadno obdelavo,
ki niso bili pomešani z drugimi smolami.

1. Strojna oprema:a. 3D tiskalnik Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Dodatki za tiskanje: Formlabs: platforme za izdelavo, posode za smolo Formlabs

2. Programska oprema:a. Formlabs PreForm

3. Parametri tiskanja:a. Usmeritev dela: Površina za globoki tisk je obrnjena stran od izdelovalne platforme pod kotom 0-40°
b. Debelina plasti: 100 μm
c. Debelina dela:• Okluzalne površine: najmanj 2 mm
• Stene: najmanj 1 mm

4. Priporočena oprema in dodatki za naknadno obdelavo:
a. Formlabsov pribor za obdelavo: Form Auto, sistem za črpanje smole
b. Formlabsova potrjena enota za pranje: Form Wash, Form Wash (2. generacija), Form Wash L,
ultrazvočna enota za pranjec. Formlabs potrjena enota za utrjevanje: Form Cure, Form Cure L, Fast CureA. TISKANJE
1. Pretresite kartušo: Pred vsakim tiskanjem pretresite kartušo. Če kartušo premalo stresete, lahko
pride do barvnih odstopanj in napak pri tiskanju.
2. Nastavitev: Vstavite posodo za smolo in nanjo pritrdite mešalnik.
3. Tiskanje:a. S programsko opremo PreForm pripravite nalogo tiskanja. Uvozite datoteko STL želenega dela.
b. Usmerite in ustvarite podpore.
c. Pošljite nalogo tiskanja v tiskalnik.
d. Tiskanje začnite tako, da v meniju za tiskanje izberete nalogo tiskanja. Upoštevajte vse pozive
in pogovorna okna, prikazane na zaslonu tiskalnika. Tiskalnik bo samodejno dokončal tiskanje.

B. ODSTRANJEVANJE DELOVS tiskalnika odstranite izdelovalno platformo. Če želite odstraniti dele z izdelovalne platforme,
orodje za odstranjevanje delov zataknite pod ploščad natisnjenega dela in ga zavrtite. Za enostavno
odstranjevanje brez orodja lahko uporabite Formlabs Build Platform 2 ali Build Platform 2L. Za podrobne
tehnike obiščite spletno mesto support.formlabs.com.

C. PRANJE
Natisnjene dele postavite v enoto za pranje z 99-odstotnim izopropilnim alkoholom, ki jo je potrdiladružba Formlabs.
1. Form Wash, Form Wash (2. generacija) - visoka hitrost* ali Form Wash L:
a. Perite 15 minut ali dokler ni čist v Form Wash ali Form Wash L.
b. Odstranite dele iz enote za pranje in jih za 5 minut namočite v svež izopropilni alkohol.
c. Če deli po pranju niso videti čisti, zamenjajte uporabljeni izopropil alkohol v enoti za pranje ssvežim topilom.

SLOVENŠČINA

Dental LT Clear V2 Resin je polimerna smola, ki se utrjuje s svetlobo in je zasnovana za izdelavo
biokompatibilnih snemljivih zobnih in ortodontskih pripomočkov, kot so okluzalne šablone, nočniščitniki, ustni ščitniki in/ali belilniki, z metodo izdelave z dodajanjem. V tem priročniku za izdelavo
so navedena priporočila in zahteve glede opreme, tiskanja in naknadne obdelave, da se zagotovi
pravilna in varna uporaba tega materiala.

*Za pralni stroj Form Wash (2. generacija) so za uporabo potrjene nastavitve visoke hitrosti.
2. Ultrazvočna pralna enota:
OPOMBA: Uporaba izopropilnega alkohola v ultrazvočni kopeli predstavlja nevarnost požara ali
eksplozije. Pri uporabi ultrazvočnega pranja preberite in upoštevajte vsa varnostna priporočila
proizvajalca ultrazvočnega pranja.
a. Za vsako pranje uporabite čist 99-odstotni izopropilni alkohol.
b. Dele položite v sekundarno plastično posodo za enkratno uporabo ali plastično vrečko, ki jo
je mogoče ponovno zapreti, nato pa jih napolnite z 99-odstotnim izopropilnim alkoholom in
poskrbite, da so deli popolnoma potopljeni.
c. Sekundarno posodo postavite v vodno kopel ultrazvočne enote in jo sonicirajte 2 minuti ali
dokler ni čista.**Učinkovitost pranja je odvisna od velikosti in moči ultrazvočne enote. Formlabsovo preskušanje jebilo opravljeno z ultrazvočnimi enotami pri 36 W/l ali več.

D. SUŠENJE
1. Odstranite dele iz izopropilnega alkohola in jih pustite, da se sušijo na zraku pri sobni temperaturi
vsaj 30 minut. OPOMBA: Čas sušenja se lahko razlikuje glede na zasnovo delov in okoliške
razmere. Ne pustite delov v izopropilnem alkoholu dlje, kot je potrebno.
2. Preverite, ali so natisnjeni deli čisti in suhi. Pred naslednjimi koraki na površini ne smejo ostati
ostanki topila, odvečne tekoče smole ali ostanki delcev.
3. Če so ostanki topila še vedno prisotni, dele sušite dlje. Če so ostanki smole še vedno vidni, deleponovno operite, dokler niso čisti in suhi.

E. NAKNADNO UTRJEVANJE
Natisnjene dele postavite v enoto za naknadno utrjevanje, ki jo je potrdila družba Formlabs, in jih
utrjujte zahtevani čas.
1. Form Cure ali Form Cure L:
a. Utrjevanje 60 minut pri 60 °C
b. Počakajte, da se enota Form Cure ali Form Cure L med cikli utrjevanja ohladi na sobno temperaturo.
2. Hitro utrjevanje:a. Utrjevanje 6 minut pri intenzivnosti svetlobe 5b. Počakajte, da se enota za hitro utrjevanje med cikli utrjevanja ohladi za vsaj 10 minut.

F. ODSTRANJEVANJE PODPORE IN POLIRANJE
1. Podporne oznake lahko povzročijo odrgnine, če niso odstranjene in zloščene. Podpore odstranite
z rezalnim diskom in ročnim nastavkom, rezalnimi kleščami ali drugimi ustreznimi orodji za dodelavo.
2. Natisnjene pripomočke pred uporabo pri pacientu polirajte z običajnimi metodami za poliranje zob.
3. Na delih preverite morebitne razpoke. Če odkrijete poškodbe ali razpoke, del zavrzite.

G. ČIŠČENJE IN RAZKUŽEVANJE
1. Popolnoma naknadno obdelane dele lahko očistite z namensko mehko zobno ščetko z nevtralnim
milom in vodo sobne temperature. Ne uporabljajte zobne paste ali drugih čistilnih sredstev na
delih, natisnjenih s smolo Dental LT Clear V2 Resin.
2. Pripomočki se lahko očistijo in razkužijo v skladu s protokoli ustanove. Preizkušena metoda
razkuževanja: namakanje pripravljenega pripomočka v svežem 70-odstotnem izopropilnem
alkoholu za 5 minut. Dela ne puščajte v alkoholni raztopini dlje kot 5 minut.
3. Po čiščenju in razkuževanju preverite, ali je del poškodovan ali razpokan, da zagotovite, dacelovitost zasnovanega dela izpolnjuje zahteve glede zmogljivosti. Če odkrijete poškodbe ali
razpoke, del zavrzite.

H. NEVARNOSTI, SKLADIŠČENJE IN ODSTRANJEVANJE
1. Utrjena smola ni nevarna in se lahko odstrani kot običajni odpadki.
2. Za več informacij glejte varnostni list na support.formlabs.com.

Szczególne uwagi dotyczące produkcji
Specyfikacja Dental LT Clear V2 Resin została zweryfikowana przy użyciu sprzętu i parametrów
wyszczególnionych poniżej. W celu zapewnienia zgodności w zakresie biokompatybilności podczas
weryfikacji zastosowano specjalny zbiornik na żywicę i mieszadło, platformę roboczą, urządzenia do
mycia oraz sprzęt do obróbki poprocesowej, które nie miały kontaktu z żadnymi innymi żywicami.

1. Sprzęt:a. Drukarka 3D Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Akcesoria do drukowania: platformy robocze Formlabs, zbiorniki na żywicę Formlabs

2. Oprogramowanie:
a. Formlabs PreForm

3. Parametry druku:
a. Orientacja części: Powierzchnia wklęsłodrukowa odwrócona od platformy roboczej pod kątem
0–40°.
b. Grubość warstwy: 100 μm
c. Grubość części:• Powierzchnie okluzyjne: minimum 2 mm
• Ściany: minimum 1 mm

4. Zalecane wyposażenie i akcesoria do obróbki poprocesowej wydruków:
a. Akcesoria do przetwarzania Formlabs: Form Auto, system pompowania żywicy
b. Urządzenia myjące zatwierdzone przez Formlabs: Form Wash, Form Wash (2. generacji),
Form Wash L, ultradźwiękowe urządzenie myjące
c. Urządzenia do utwardzania zatwierdzone przez Formlabs: Form Cure, Form Cure L, Fast Cure

A. DRUKOWANIE
1. Potrząsanie kartridżem: Zawsze przed rozpoczęciem drukowania mocno potrząśnij kartridżem.
W przeciwnym wypadku mogą wystąpić odchylenia kolorystyczne i błędy w druku.
2. Przygotowanie: Włóż zbiornik z żywicą i podłącz do niego mieszadło.
3. Drukowanie:a. Przygotuj zadanie drukowania przy użyciu oprogramowania PreForm. Zaimportuj plik STL
dla pożądanej części.
b. Określ orientację podpór i wygeneruj je.
c. Prześlij zadanie drukowania do drukarki.
d. Aby rozpocząć drukowanie, wybierz zadanie drukowania z menu drukowania. Postępuj
zgodnie z podpowiedziami lub oknami dialogowymi wyświetlanymi na ekranie drukarki.
Drukarka wykona wydruk automatycznie.

B. WYJMOWANIE CZĘŚCI
Wyjmij z drukarki platformę roboczą. Aby wyjąć części z platformy roboczej, podważ wydrukowaną
część narzędziem do wyjmowania wydruków i obróć narzędzie. Platforma robocza Formlabs 2 lub
Platforma robocza 2L mogą być używane do łatwego wyjmowania części bez użycia narzędzi.
Bardziej szczegółowy opis poszczególnych technik można znaleźć na witrynie support.formlabs.com.

C. MYCIEUmieść wydrukowane części w zatwierdzonym przez Formlabs urządzeniu do mycia z alkoholem
izopropylowym o stężeniu 99%.

POLSKI

Dental LT Clear V2 Resin to światłoutwardzalna żywica na bazie polimerów, przeznaczona do
wytwarzania biokompatybilnych, długotrwałych, wyjmowanych aparatów stomatologicznych i
ortodontycznych – takich jak szyny zgryzowe, wkładki na noc, ochraniacze na zęby lub nakładki
wybielające – poprzez obróbkę przyrostową. Niniejszy przewodnik produkcyjny zawiera zalecenia iwymagania dotyczące sprzętu, drukowania i obróbki poprocesowej w celu zapewnienia prawidłowego
i bezpiecznego użytkowania tego materiału.

1. Form Wash, Form Wash (2. generacji) – duża prędkość* lub Form Wash L:
a. Myć przez 15 minut lub do czysta w Form Wash lub Form Wash L.
b. Wyjmij części z urządzenia do mycia i namaczaj w świeżym alkoholu izopropylowym przez
5 minut.
c. Jeśli części po umyciu nie wyglądają na czyste, rozważ wymianę zużytego alkoholu
izopropylowego w urządzeniu do mycia na świeży rozpuszczalnik.
*W przypadku Form Wash (2. generacji) ustawienia wysokiej prędkości są zatwierdzone do użycia.
2. Ultradźwiękowe urządzenie do mycia:
UWAGA: Używanie alkoholu izopropylowego w kąpieli ultradźwiękowej stwarza zagrożenie pożarem
lub wybuchem. Podczas korzystania z urządzenia do mycia ultradźwiękowego należy przeczytać
wszystkich zaleceń dotyczących bezpieczeństwa wydanych przez producenta urządzenia do mycia
ultradźwiękowego i przestrzegać ich.
a. Do każdego mycia używać czystego alkoholu izopropylowego o stężeniu 99%.
b. Umieść części w dodatkowym plastikowym pojemniku jednorazowego użytku lub w
plastikowej szczelnie zamykanej torbie, a następnie napełnij alkoholem izopropylowym ostężeniu 99% i upewnij się, że części są całkowicie zanurzone.
c. Umieścić dodatkowy pojemnik w kąpieli wodnej w urządzeniu do mycia ultradźwiękowego i
poddawaj działaniu ultradźwięków przez 2 minuty lub do momentu wyczyszczenia.**Skuteczność mycia zależy od wielkości i mocy urządzenia ultradźwiękowego. Testy Formlabs
przeprowadzono z użyciem jednostek ultradźwiękowych o mocy 36 W/L lub większej.

D. SUSZENIE
1. Wyjmij części z alkoholu izopropylowego i pozostaw do wyschnięcia na powietrzu w temperaturze
pokojowej na co najmniej 30 minut. UWAGA: Czas suszenia może się różnić w zależności odbudowy części i warunków otoczenia. Nie pozostawiać części w alkoholu izopropylowym dłużej
niż to konieczne.
2. Sprawdź, czy części są suche i oczyszczone. Przed przejściem do kolejnych czynności na
powierzchni nie powinny pozostać żadne resztki rozpuszczalnika, nadmiar płynnej żywicy ani
drobinki odpadków.
3. Jeśli pozostałości rozpuszczalnika są nadal obecne, susz części jeszcze dłużej. Jeżeli resztkiżywicy są wciąż widoczne, umyj ponownie części do czysta i wysusz je.

E. UTWARDZANIE PO DRUKOWANIUUmieść wydrukowane części w zatwierdzonym przez Formlabs urządzeniu do utwardzania i utwardzaj
przez wymagany czas.
1. Form Cure lub Form Cure L:
a. Utwardzaj przez 60 minut w temperaturze 60°C
b. Poczekaj, aż urządzenie Form Cure lub Form Cure L ostygnie do temperatury pokojowejpomiędzy cyklami utwardzania.
2. Szybkie utwardzanie:
a. Utwardzaj przez 6 minut przy intensywności światła 5b. Pozostaw urządzenie Fast Cure do ostygnięcia na co najmniej 10 minut pomiędzy
cyklami utwardzania.

F. USUWANIE PODPÓR I POLEROWANIE
1. Ślady po podporach mogą powodować ścieranie, jeśli nie zostaną usunięte i wypolerowane.
Usuń podpory za pomocą tarczy tnącej i rękojeści, szczypiec lub innych odpowiednich narzędzi dowykańczania powierzchni.
2. Wypoleruj wydrukowane elementy z wykorzystaniem typowych metod polerowania dentystycznego
przed użyciem przez pacjenta.
3. Sprawdź, czy na częściach nie ma żadnych pęknięć. Wyrzuć części, na których wykryjesz
jakiekolwiek uszkodzenia lub pęknięcia.

G. CZYSZCZENIE I DEZYNFEKCJA
1. Części poddane pełnej obróbce poprocesowej można oczyścić za pomocą specjalnej miękkiej
szczoteczki do zębów i neutralnego mydła z wodą o temperaturze pokojowej. Do czyszczeniaczęści wydrukowanych przy użyciu Dental LT Clear V2 Resin nie należy używać pasty do zębów
ani żadnych innych środków czyszczących.
2. Aparaty mogą być czyszczone i dezynfekowane zgodnie z protokołami zakładowymi. Sprawdzona
metoda dezynfekcji: namoczenie gotowej części przez 5 minut w świeżym IPA o stężeniu 70%.
Nie należy pozostawiać części w roztworze alkoholu dłużej niż na 5 minut.
3. Po czyszczeniu i dezynfekcji sprawdź część pod kątem uszkodzeń lub pęknięć, aby zapewnić,
że integralność zaprojektowanej części spełnia wymagania eksploatacyjne. Wyrzuć części,na których wykryjesz jakiekolwiek uszkodzenia lub pęknięcia.

H. ZAGROŻENIA, PRZECHOWYWANIE I UTYLIZACJA
1. Utwardzona żywica nie jest niebezpieczna i można ją usuwać jako zwykły odpad.
2. Więcej informacji można znaleźć w karcie charakterystyki produktu na witrynie support.formlabs.com.

Особые указания производителя
Технические характеристики Dental LT Clear V2 Resin были проверены с использованием
оборудования и параметров, указанных ниже. При проверке биосовместимости использовался
специальный резервуар для полимеров и смеситель, рабочая платформа, машина промывки иоборудование для постобработки, которые не использовались для работы с другими материалами.

1. Аппаратное обеспечение:a. 3D-принтер Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Принадлежности для печати: рабочие платформы Formlabs, резервуарыдля полимеров Formlabs

2. Программное обеспечение:a. Formlabs PreForm

3. Параметры печати:a. Ориентация: поверхность оттиска обращена в противоположную от рабочей платформы
сторону на 0–40° угла наклона
b. Толщина слоя: 100 мкм
c. Толщина модели:• Окклюзионные поверхности: минимум 2 мм• Стены: минимум 1 мм

4. Рекомендуемое оборудование и принадлежности для постобработки:a. Аксессуары Formlabs для обработки: Form Auto, система закачки полимера
b. Проверенная машина промывки Formlabs: Form Wash, Form Wash (2-ое поколение),Form Wash L, ультразвуковая машина промывки
c. Проверенная машина для финальной полимеризации Formlabs: Cure Unit: Form Cure,
Form Cure L, Fast CureA. Печать
1. Встряхивайте картридж: встряхивайте картридж перед каждой печатью. Если картридж
встряхнуть недостаточно хорошо, это может привести к другому цвету напечатанной моделиили возникновению дефектов печати.
2. Подготовка: вставьте картридж для полимеров в совместимый 3D-принтер Formlabs.
Вставьте резервуар полимера и подсоедините к нему смеситель.
3. Печать:a. Подготовьте задачу на печать в программном обеспечении PreForm. Импортируйте
нужный файл модели в формате STL.
b. Расположите и создайте поддерживающие структуры.
c. Отправьте задачу на печать на принтер.
d. Запустите печать, выбрав задачу в меню. Следуйте указаниям и сообщениям на экране
принтера. Принтер завершит печать автоматически.

B. Извлечение моделей
Извлеките рабочую платформу из принтера. Для извлечения моделей из рабочей платформы
вставьте инструмент для извлечения моделей под основание напечатанной модели и поверните
его. Для простого извлечения без инструментов используйте Formlabs Build Platform 2
или Build Platform 2L. Для получения более подробной информации о снятии посетите сайтsupport.formlabs.com.

РУССКИЙ

Dental LT Clear V2 Resin — это легкоотверждаемый полимер, разработанный для аддитивного
производства биосовместимых многоразовых стоматологических и ортодонтических изделий,таких как окклюзионные шины, ночные капы, зубные капы и капы для отбеливания зубов.
Ознакомьтесь с рекомендациями и требованиями к оборудованию, печати и постобработке дляправильного и безопасного использования материала в этом руководстве по производству.

C. Промывка
Поместите напечатанные модели в проверенную компанией Formlabs машину промывки
с 99% изопропиловым спиртом.
1. Form Wash, Form Wash (2-ое поколение) — высокоскоростная* или Form Wash L:a. Промывайте в течение 15 минут или до полной очистки в Form Wash или Form Wash L.
b. Затем модели нужно извлечь из машины промывки и погрузить в свежий
изопропиловый спирт на 5 минут.
c. Если после промывки детали не выглядят чистыми, замените использованный
изопропиловый спирт в машине промывки свежим растворителем.
*Для Form Wash (2-ое поколение) подтверждены настройки высокой скорости.
2. Ультразвуковая машина промывки:ПРИМЕЧАНИЕ: использование изопропилового спирта в ультразвуковой ванне сопряженос риском возгорания или взрыва. При использовании ультразвуковой машины промывки
прочитайте и соблюдайте все рекомендации по безопасности от производителя
ультразвуковой машины промывки.
a. Используйте чистый изопропиловый спирт (99%) для каждой промывки.
b. Поместите модели во вспомогательный одноразовый пластмассовый контейнер илипластиковый герметичный пакет, затем налейте изопропиловый спирт (99%) до полного
погружения моделей.
c. Поместите вспомогательный контейнер в водяную баню ультразвуковой машины
промывки и проведите обработку ультразвуком в течение 2 минут или до полной очистки.**Эффективность промывки зависит от размера и мощности ультразвуковой установки.
Испытания Formlabs проводились с ультразвуковыми аппаратами мощностью 36 Вт/л и выше.

D. Сушка
1. Извлеките модели из изопропилового спирта и просушите их при комнатной температурене менее 30 минут. ПРИМЕЧАНИЕ: время высыхания может меняться в зависимости отконструкции моделей и условий окружающей среды. Не позволяйте моделям находитьсяв изопропиловом спирте дольше, чем это необходимо.
2. Осмотрите напечатанные модели на предмет чистоты и сухости. Перед выполнением
дальнейших действий убедитесь, что на поверхности моделей не остался спирт,растворитель, жидкий полимер или какие-либо частицы.
3. Если растворитель еще остался, дополнительно просушите модели. Если остатки полимеравсе еще видны, повторно промойте модели, пока они не станут чистыми и сухими.

E. Финальная полимеризация
Поместите напечатанные модели в проверенную компанией Formlabs машину для финальной
полимеризации и полемизируйте в течение необходимого времени.
1. Form Cure или Form Cure L:a. Выполните 30-минутную полимеризацию при 60 °C
b. Между циклами финальной полимеризации устройство Form Cure или Form Cure Lдолжно остывать до комнатной температуры.
2. Fast Cure:a. Выполните 6-минутную полимеризацию при интенсивности света 5b. Между циклами финальной полимеризации устройство Fast Cure должно остыватьв течение не менее 10 минут.

F. Удаление и полировка поддерживающих структур
1. Следы от поддерживающих структур следует удалить и отполировать, чтобы избежать
абразивного износа. Удалите поддерживающие структуры с помощью отрезного дискаи режущего инструмента, плоскогубцев или других подходящих инструментов.
2. Прежде чем использовать напечатанные модели для пациентов, отполируйте их с помощью
методов, применяемых в стоматологии.

3. Осмотрите модели на отсутствие трещин. При обнаружении повреждений или трещин
выбросите модель.

G. Очистка и дезинфекция
1. Модели, полностью прошедшие постобработку, можно очистить с помощью специальной
мягкой кисти, а также нейтрального мыла и воды комнатной температуры. Для моделей,напечатанных с помощью Dental LT Clear Resin (V2), запрещается использовать зубную
пасту или другие средства для очистки.
2. Модели можно очищать и дезинфицировать согласно правилам медицинского учреждения.
Проверенный метод дезинфекции: погружение отшлифованной модели в свежий 70%раствор ИПС на 5 минут. Запрещается оставлять модель в растворе дольше, чем на 5 минут.
3. После очистки и дезинфекции проверьте напечатанные модели на отсутствие поврежденийи трещин, чтобы обеспечить их целостность. При обнаружении повреждений или трещин
выбросите модель.

H. Опасности, хранение и утилизация
1. Отвержденный полимер не представляет опасности и может быть утилизирован какобычные отходы.
2. Более подробную информацию см. в паспорте безопасности на сайте support.formlabs.com.

Специфични производствени съображения
Спецификациите на смолата Dental LT Clear V2 Resin са валидирани с помощта на хардуераи параметрите, посочени по-долу. За да се поддържа биосъвместимостта, за валидирането саизползвани специален контейнер за смола и смесител, платформа за изграждане, устройствоза измиване и оборудване за последваща обработка, които не са смесени с други смоли.

1. Хардуер:a. 3D принтер на Formlabs: Form 2, Form 3B/3B+, Form 3BL, Form 4B
b. Аксесоари за печат: платформите за изграждане на Formlabs, контейнерите за смола
на Formlabs

2. Софтуер:a. Formlabs PreForm

3. Параметри на печатане:a. Ориентация на частта: Intaglio повърхността с дълбок печате обърната встрани отплатформата за изграждане под 0 – 40° ъгъл на наклона
b. Дебелина на слоя: 100 μm
c. Дебелина на частта:• Оклузални повърхности: минимум 2 mm
• Стени: минимум 1 mm

4. Препоръчително оборудване и аксесоари за последваща обработка:a. Аксесоари за обработка на Formlabs: Form Auto, помпена система за смола
b. Валидирани от Formlabs устройства за измиване: Form Wash, Form Wash (2-ро поколение),Form Wash L, ултразвуково устройство за измиване
c. Валидирани от Formlabs устройства за втвърдяване: Form Cure, Form Cure L, Fast CureA. ПЕЧАТ
1. Разклатете касетата: Разклатете касетата преди всяка задача за печат. Възможное да възникнат отклонения в цвета и грешки при отпечатването, ако касетата нее разклатена достатъчно.
2. Подготовка: Поставете контейнера за смола и прикрепете смесителя към контейнера.
3. Печат:a. Подгответе задачата за печат със софтуера PreForm. Импортирайте желаната частна STL файла.
b. Регулирайте ориентацията и генерирайте подпори.
c. Изпратете задачата за печат към принтера.
d. Започнете печатането, като изберете задача за печат от менюто за печат. Следвайте
всички подкани или диалогови прозорци, показани на екрана на принтера. Принтерът
автоматично ще завърши отпечатването.

B. ОТСТРАНЯВАНЕ НА ЧАСТИзвадете платформата за изграждане от принтера. За да отстраните части от платформатаза изграждане, заклинете инструмента за отстраняване на части под плота на отпечатаната
част и завъртете инструмента. Платформата за изграждане на Formlabs Build Platform 2 или
Build Platform 2L може да се използва за лесно отстраняване без инструменти. За подробни
техники вж. support.formlabs.com.

БЪЛГАРСКИ

Смолата Dental LT Clear V2 Resin е светлинно втвърдяваща се смола на полимерна основа,предназначена за производството на биосъвместими, премахващи се стоматологичнии ортодонтски уреди за дългосрочна употреба, като например оклузални шини, нощни
предпазители, предпазители за уста и/или шини за избелване, чрез адитивно производство.
Това ръководство за производство предоставя препоръки и изисквания за оборудването,печата и последващата обработка, за да се гарантира правилната и безопасна употребана този материал.

C. ИЗМИВАНЕ
Поставете отпечатаните части във валидирано от Formlabs устройство за измиване
с 99% изопропилов алкохол.
1. Form Wash, Form Wash (2-ро поколение) – висока скорост* или Form Wash L:a. Мийте в продължение на 15 минути или докато се почисти с Form Wash или Form Wash L.
b. Извадете частите от устройството за измиване и ги накиснете в пресен изопропилов
алкохол в продължение на 5 минути.
c. Ако частите не изглеждат чисти след измиване, можете да замените използвания
изопропилов алкохол в устройството за измиване с пресен разтворител.
*За Form Wash (2-ро поколение), настройките за висока скорост са валидирани за използване.
2. Ултразвуково устройство за измиване:ЗАБЕЛЕЖКА: Използването на изопропилов алкохол в ултразвукова вана представлява рискот пожар или експлозия. Когато използвате ултразвуково устройство за измиване, прочетете иследвайте всички препоръки за безопасност от производителя на ултразвуковото устройствоза измиване.
a. Използвайте чист 99% изопропилов алкохол за всяко измиване.
b. Поставете частите в страничен пластмасов контейнер за еднократна употреба илипластмасова торбичка, която може да се затваря повторно, след което напълнете
с 99% изопропилов алкохол, като се уверите, че частите са напълно потопени.
c. Поставете страничния контейнер във ваната за ултразвуковото измиване и мийте сустразвук в продължение на 2 минути или докато се почисти.**Ефикасността на измиването зависи от размера и мощността на ултразвуковото устройство.
Тестовете на Formlabs са проведени с ултразвукови устройства с 36 W/L или по-високи стойности.

D. СУШЕНЕ
1. Извадете частите от изопропиловия алкохол и оставете да изсъхнат на стайна температураза минимум 30 минути. ЗАБЕЛЕЖКА: Времето за сушене може да варира в зависимост отдизайна на частите и условията на околната среда. Не оставяйте частите да престояват визопропилов алкохол по-дълго от необходимото.
2. Проверете отпечатаните части, за да се уверите, че са чисти и сухи. Преди да продължитесъс следващите стъпки се уверете, че на повърхността няма остатъчен разтворител,излишна течна смола или остатъчни частици.
3. Ако все още има остатъчен разтворител, изсушете частите по-дълго. Ако остатъците отсмола все още са видими, измийте частите докато станат чисти и сухи.

E. ПОСЛЕДВАЩО ВТВЪРДЯВАНЕ
Поставете отпечатаните части във валидирано от Formlabs устройство за последващо
втвърдяване и втвърдявайте в продължение на нужното време.
1. Form Cure или Form Cure L:a. Втвърдявайте на 60°C в продължение на 60 мин.
b. Оставете устройството Form Cure или Form Cure L да се охлади до стайна температура
между циклите на втвърдяване.
2. Fast Cure:a. Втвърдявайте в продължение на 6 минути при интензивност на светлината 5b. Оставете уреда за бързо втвърдяване Fast Cure да се охлади в проддължение на поне10 минути между циклите на втвърдяване.

F. ОТСТРАНЯВАНЕ НА ПОДПОРИТЕ И ПОЛИРАНЕ
1. Следите от подпорите може да причинят протърквания, ако не бъдат отстранени или полирани.
Отстранете подпорите с помощта на режещ диск и накрайник, режещи клещи или други
подходящи инструменти за довършителни работи.
2. Полирайте отпечатаните уреди съобразно обичайните методи за стоматологично полиране
преди употреба от пациента.

3. Проверете частите за пукнатини Изхвърлете частите, ако откриете каквито и да са повредиили пукнатини по тях.

G. ПОЧИСТВАНЕ И ДЕЗИНФЕКЦИЯ
1. Напълно обработените части могат да се почистят с помощта на специална мека четка зазъби с неутрален сапун и вода със стайна температура. Не използвайте паста за зъби илидруги почистващи препарати върху части, отпечатани със смола Dental LT Clear V2 Resin.
2. Уредите да се почистват и дезинфекцират съгласно протоколите на учреждението.
Тестваният метод за дезинфекция: накисване на готовия уред в пресен 70% IPA за 5 минути.
Не оставяйте частта в алкохолния разтвор в продължение на повече от 5 минути.
3. След почистване и дезинфекция проверете частта за повреди или пукнатини, за да сеуверите, че целостта на проектираната част отговаря на изискванията за функционалност.
Изхвърлете частите, ако откриете каквито и да са повреди или пукнатини по тях.

H. ОПАСНОСТИ, СЪХРАНЕНИЕ И ИЗХВЪРЛЯНЕ
1. Втвърдената смола не е опасна и може да се изхвърля като обикновен отпадък.
2. За повече информация прочетете Информационния лист за безопасност на адрес
support.formlabs.com.

製作に使用する際の注意特記事項

Dental LT Clear V2レジンの仕様については、以下のハードウェアおよびパラメータを使用して検証を行っています。
生体適合性関連の基準に準拠し、検証には他のレジンとの混合のない専用のレジンタンクとミ
キサー、
ビルドプラットフォーム 、洗浄ユニット、後処理装置を使用しいます。

1. ハードウェア：

a. Formlabs 3Dプリンター：Form 2、Form 3B/3B+、Form 3BL、Form 4B
b. プリント用周辺機器：Formlabsビルドプラットフォーム、Formlabsレジンタンク

2. ソフトウェア：

a. Formlabs PreForm

3. プリントパラメータ：

a. 配置向き：粘膜面をビルドプラットフォーム面に対して反対に向け、0 ～ 40°傾斜させて配置
b. 積層ピッチ：100μm
c. 造形品厚さ：• 咬合面：2mm以上• 壁：1mm以上

4. 推奨後処理装置と関連機器：

a. Formlabs製加工用機器：Form Auto、Resin Pumping Systemb. Formlabs検証済み洗浄ユニット：Form Wash、Form Wash（第2世代）、Form Wash L、超音波洗浄ユニット
c. Formlabs検証済み二次硬化ユニット：Form Cure、Form Cure L、Fast CureA. プリント手順

1. カートリッジを振る：プリントの都度、使用前にカートリッジをしっかり振ってください。
よく振らずに使用した場合、色むらやプリント失敗につながる場合があります。
2. セットアップ：レジンカートリッジを互換性のあるFormlabs 3Dプリンタにセットします。
レジンタンクを挿入し、ミキサーをタンクに取り付けます。
3. プリント：a. PreFormソフトウェアを使用してプリントジョブを作成します。
プリントするSTLファイルをインポートします。
b. プリントの向きを決め、サポート材を生成します。
c. プリンタにプリントジョブを送信します。
d. プリントメニューに表示されるプリントジョブの中からジョブを選択し、プリントを開始します。
プリン
ターの画面に表示されるメッセージやダイアログに従って操作を進めます。
プリンターが自動的にプリントを完了します。

B. プリント品の取り外し

プリンタからビルドプラットフォーム を取り外します。
ビルドプラットフォームからプリント品を取り外すには、
リムーバルツールをプリント品のラフト下に差し込み、
リムーバルツールを回転させます。
Formlabs Build
Platform 2やBuild Platform 2Lを使用すれば、ツールなしで簡単に取り外すことが可能です。
詳細手順は、
support.formlabs.comをご覧ください。

C. 洗浄

99%イソプロピルアルコール（IPA）を入れたFormlabs検証済み洗浄ユニットに、プリント品を入れます。
1. Form Wash、Form Wash（第2世代）の高速洗浄*、またはForm Wash Lを使用する場合：
a. Form WashまたはForm Wash Lで、15分間またはきれいになるまで洗浄します。
b. 洗浄後、洗浄ユニットから造形品を取り出し、新品のイソプロピルアルコール（IPA）に5分間漬けます。
c. 洗浄後、完全にきれいになっていない場合は、洗浄ユニット内の使用済みイソプロピルアルコールを新しいものと交換することをお勧めします。

日本語

Dental LT Clear V2レジンは、咬合スプリント、
ナイトガード、
マウスガード、
ブリーチングトレー等の取り外し可能な歯科および矯正歯科装置の製作用に設計された、生体適合性を備え長期使用に適する積層造形用の光硬化性樹脂です。
本マニュファクチャリングガイドでは、この材料を正しく安全に使用するための機器、
プリントおよび後処理方法に関する推奨事項や必須事項を説明しています。

*Form Wash（第2世代）を使用した高速洗浄は弊社検証済み。
2. 超音波洗浄ユニットを使用する場合：
注意：イソプロピルアルコールを超音波洗浄槽で使用すると、火災や爆発の危険がありますのでご注意く
ださい。
超音波洗浄機を使用する場合は、超音波洗浄機メーカーが推奨するすべての安全事項を読み、それに従ってください。
a. 洗浄の都度、新しい99％イソプロピルアルコールを使用してください。
b. プリント品を使い捨てのプラスチック容器またはジッパー付きのプラスチック袋に入れ、プリント品が完全に浸かるまで99％のイソプロピルアルコールを入れます。
c. 別の容器を超音波ユニットの水槽に入れ、2分間、
またはきれいになるまで超音波処理を行います*。
*洗浄効果は、超音波ユニットのサイズと強度によって変わります。
Formlabsのテストは、36W/L以上の超音波ユニットで実施しています。

D. 乾燥

1. プリント品をイソプロピルアルコールから取り出し、室温で30分以上自然乾燥させます。
注記：乾燥時間は、プリント品の形状や周囲の環境によって異なる場合があります。
プリント品をイソプロピルアルコールに必要以上に長時間浸けないでください。
2. プリント品の全体を点検して、汚れがなく、きれいに乾いていることを確認します。
次のステップに進む
前に、溶剤や液体レジン、粉体が表面に残っていないことを確認してください。
3. 溶剤が残っている場合は、さらに乾燥させてください。
レジンが残っている場合は、
きれいになるまで再度洗浄した後、乾燥させてください。

E. 二次重合

プリント品をFormlabs認定品の二次重合ユニットに入れ、必要な時間重合させます。
1. Form CureまたはForm Cure L：
a. 60℃で 60分間硬化させます。
b. 次の硬化サイクルを実行する前に、Form CureまたはForm Cure Lユニットが室温まで冷めるのを待ちます。
2. Fast Cure：a. 光強度5で6分間硬化させます。
b. 次の硬化サイクルを実行する前に、Fast Cureユニットを10分以上放置して冷まします。

F. サポートの取り外しと研磨

1. サポート痕を除去して研磨しておかなければ、使用時の擦り傷の原因になります。カッティングディスクとハンドピース、
カッティングニッパー、
またはその他の適切な仕上げ用ツールを使用して、サポート材を取り除きます。
2. 製作した装置を患者様に使用する前に、歯科の通常の手法を用いて研磨してください。
3. 造形品の表面に亀裂などが発生していないかを点検します。
損傷や亀裂が見つかった場合は破棄してください。

G. 洗浄と消毒

1. 完全に後処理を済ませた後の造形品の洗浄は、Dental LT Clear V2レジン 専用に用意した柔らかい歯
ブラシに中性石鹸と室温の水を使って行ってください。
Dental LT Clear V2レジンでプリントした装置の洗浄には、歯磨き粉などの研磨剤入り洗浄剤を使用しないでください。
2. 装置の洗浄と消毒は、各歯科医院で決められて手順に従って行うことが可能です。
試験で有効性が確認されている消毒法は、仕上げ後のプリ ント品を純度70％のIPAに5分間浸漬する方法です。
アルコー
ルには５分以上漬けたままにしないでください。
3. 洗浄および消毒後、損傷や亀裂の有無を点検し、造形した装置が総合的にデザインどおりの性能要件を満たしていることを確認してください。
損傷や亀裂が見つかった場合は、破棄してください。

H. 危険性、保管、廃棄

1. 硬化したレジンは危険物ではないため、一般ごみとして廃棄可能です。
2. 詳細は、support.formlabs.comにある安全データシートをご覧ください。

具体生产注意事项

Dental LT Clear Resin (V2) 规格已通过以下硬件和参数进行了验证。为了符合生物相容性要求，我们已使用专用的树脂槽和混合器、构建平台、清洗设备与后处理设备，在未与任何其他树脂混用的情况
下进行了验证。

1. 硬件：

a. Formlabs 3D 打印机：Form 2、Form 3B/3B+、Form 3BL、Form 4B
b. 打印配件：Formlabs 构建平台、Formlabs 树脂槽

2. 软件：

a. Formlabs PreForm

3. 打印参数：

a. 部件定向：凹面以 0－40° 倾斜角背对构建平台b. 打印层厚：100μm
c. 部件厚度：• 咬合面：≥2mm• 壁面：≥1mm

4. 建议使用的后处理设备和配件：

a. Formlabs 后处理配件：Form Auto（自动化系统）、Resin Pumping System（树脂泵送系统）b. 经 Formlabs 验证的清洗设备：Form Wash、Form Wash（第二代）、Form Wash L、超声波清洗装置
c. 经 Formlabs 验证的固化设备：Form Cure、Form Cure L、Fast Cure

A. 打印

1. 摇晃树脂盒：请在每次打印任务开始前摇晃树脂盒。如果未能充分摇晃树脂盒，可能会出现颜色偏差并造成打印失败。
2. 设置：将树脂盒放入兼容的 Formlabs 3D 打印机。插入树脂槽并将混合器安装到树脂槽中。
3. 打印：
a. 使用 PreForm 软件准备打印任务。导入所需的部件 STL 文件。
b. 定向并生成支撑结构。
c. 将打印任务发送至打印机。
d. 从打印菜单中选择打印任务以开始打印。请遵循打印机屏幕上的所有提示或对话框。打印机将自动完成打印。

B. 移除部件

从打印机中取出构建平台。如需从构建平台上移除部件，请将部件移除工具楔入打印部件基座下方，然后旋转工具。在不使用工具的情况下，用户可以从 Formlabs Build Platform 2 或 Build Platform 2L
上轻松移除部件。有关详细技术信息，请访问 support.formlabs.com。

C. 清洗

将打印好的部件放入经过 Formlabs 验证的装有 99% 异丙醇的清洗装置中。
1. Form Wash、Form Wash（第二代）－高速*，或 Form Wash L：a. 在 Form Wash 或 Form Wash L 中清洗 15 分钟或直至部件洁净。
b. 从清洗设备中取出部件，然后将其放入纯净的异丙醇中浸泡 5 分钟。
c. 如果部件在清洗后仍有脏污，请考虑使用纯净的溶剂替换清洗设备中使用过的异丙醇。
*Form Wash（第二代）的高速设置经验证可以使用。
2. 超声波清洗装置：
注：在超声波浴中使用异丙醇有发生火灾或爆炸的风险。在使用超声波清洗时，请阅读并遵守超声波清洗装置制造商的所有安全建议。
a. 每次清洗均需使用纯净的 99% 异丙醇。

中文

Dental LT Clear Resin (V2) 是一款以光固化聚合物为原料的树脂，旨在通过增材制造技术制造具有生
物相容性、可长期使用的可摘牙科和正畸器械，例如咬合夹板、夜间保护器、护齿套和/或漂白托盘。
本制造指南中包含了设备、打印和后处理相关建议和要求，可确保用户正确且安全地使用该材料。

b. 将部件放在辅助一次性塑料容器或可重新密封的塑料袋中，然后注入 99% 异丙醇，以确保完
全浸没部件。
c. 将辅助容器放在超声波装置的水浴中，超声处理 2 分钟或直至部件洁净。**清洗效果取决于超声波装置的大小和功率。Formlabs 采用了 36W/L 或更高的超声波装置进行测试。

D. 干燥

1. 从异丙醇中取出部件，并在室温下风干至少 30 分钟。注：干燥时间会因部件设计和环境条件而异。
请勿将部件在异丙醇中放置超过所需时间。
2. 检查打印部件，确保部件清洁干燥。确保部件表面无残留溶剂、多余的液态树脂或残余颗粒物，然后再进行后续步骤。
3. 如果仍然残留溶剂，则需延长部件干燥时间。如果仍存在可见的树脂残留物，请重新清洗部件，
直至清洁干燥。

E. 后固化

将打印部件放置于经 Formlabs 验证的后固化设备中，并按所需时间进行固化。
1. Form Cure 或 Form Cure L：
a. 在 60℃ 下固化 60 分钟
b. 每个固化周期结束后，请等待 Form Cure 或 Form Cure L 冷却至室温。
2. Fast Cure：a. 在光照强度 5 下固化 6 分钟b. 每个固化周期结束后，让 Fast Cure 冷却至少 10 分钟。

F. 支撑移除和抛光

1. 如果未能移除支撑并抛光，则支撑标记可能造成部件磨损。 使用切割盘、切割钳和手持工具或是使用其他后处理工具移除支撑。
2. 在患者使用之前，请使用标准的牙科抛光方法对打印器具进行抛光。
3. 检查部件是否有裂痕。如果发现任何损坏或裂痕，则请将该部件丢弃。

G. 清洁和消毒1. 经过完整后处理的部件可以使用专用软牙刷、中性肥皂和室温水进行清洁。请勿在使用 Dental LT
Clear Resin (V2) 打印的部件上使用牙膏或任何其他清洁产品。
2. 部件可根据设备规程进行清洁和消毒。经测试的消毒方法：将成品用具浸入纯净的 IPA（浓度为
70%）中浸泡 5 分钟。请勿将部件在酒精溶液中放置超过 5 分钟。
3. 完成清洁和消毒后，检查打印部件是否损坏或存在裂缝，以确保设计的部件结构完整，可满足性能要求。如果发现任何损坏或裂痕，则请将该部件丢弃。

H. 危害、储存和处置

1. 固化树脂无害，可作为普通垃圾进行处置。
2. 请访问 support.formlabs.com 参阅安全数据表以获取更多信息。